Finite element modelling of composite materials and structures F L Matthews, G A O Davies, D Hitchings and C Soutis
Ca...
258 downloads
2217 Views
2MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
Finite element modelling of composite materials and structures F L Matthews, G A O Davies, D Hitchings and C Soutis
Cambridge England
Published by Woodhead Publishing Limited, Abington Hall, Abington Cambridge CB1 6AH, England www.woodheadpublishing.com Published in North America by CRC Press LLC, 2000 Corporate Blvd, NW Boca Raton FL 33431, USA First published 2000, Woodhead Publishing Ltd and CRC Press LLC Reprinted 2003 © 2000, Woodhead Publishing Ltd The authors have asserted their moral rights. This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. Reasonable efforts have been made to publish reliable data and information, but the authors and the publishers cannot assume responsibility for the validity of all materials. Neither the authors nor the publishers, nor anyone else associated with this publication, shall be liable for any loss, damage or liability directly or indirectly caused or alleged to be caused by this book. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming and recording, or by any information storage or retrieval system, without permission in writing from the publishers. The consent of Woodhead Publishing and CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from Woodhead Publishing or CRC Press for such copying. Trademark notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library. Library of Congress Cataloging in Publication Data A catalog record for this book is available from the Library of Congress. Woodhead Publishing ISBN 1 85573 422 2 CRC Press ISBN 0849308461 CRC Press order number: WP0846 Cover design by The ColourStudio Typeset by Bestset Typesetter Ltd., Hong Kong Printed by TJI Digital, Padstow, Cornwall, England
Contents
Preface Authors Acknowledgement Part I
vii ix X
Overview and review of composite materials F. L . M AT T HE W S
3 3 4
1
1.1 1.2
Overview Composite materials Structural analysis
2 2.1 2.2 2.3 2.4
Fundamentals of composites Basic characteristics Fibres and matrices Summary Reference
6 6 11 16 16
3 3.1 3.2 3.3 3.4 3.5 3.6
Stiffness and strength of composites Stiffness of unidrectional composites and laminates Micromechanics of unidirectional composites Strength of unidirectional composites and laminates Application to structures Summary References
17 17 27 30 34 36 37
Part II
Fundamentals of finite element analysis G . A . 0. DAVIES
4
4.1 4.2
Fundamentals of finite element analysis Basic theoretical foundations Princide of virtual disdacements
41 41 45 ... 111
iv
4.3 4.4 4.5 4.6 4.7 4.8 4.9 4.10
Contents
An arbitrary structure Finite element approximations Brick, beam, plate and shell elements Model generation Solution procedures Results verification Summary Reference
46 49 56 61 63 65 67 68
Part 111 Finite elements applied to composite materials D. HITCHINGS
5 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8
6 6.1 6.2 6.3 6.4 6.5 6.6 6.7 6.8 6.9 6.10 6.11 6.12 6.13 6.14
Composites and finite element analysis Elements used for composite laminate analysis Accuracy of the finite element solution Other modelling techniques useful for composite analysis Changes of mesh density Modelling of composite materials Examples of finite element composite analysis Effect of layup on plate response Summary Definition of composite materials in finite element analysis Introduction Geometry and topology Fibre orientation Volume fraction and ply thickness variations Laminate ply dropoff Modelling real structures Nonlinearities in composite analysis Failure models Determination of energy release rates Crack propagation modelling Micromechanical models using finite element analysis Smart composites: the inclusion of piezoelectric effects Summary References
71 71 78
79 82 84 87 90 93
94 94 94 96 99 100 101 104 107 110 112
113 116 118 119
Contents
V
Part IV Analytical and numerical modelling C . SOUTIS
7 7.1 7.2 7.3 7.4 7.5 7.6
lnterlaminar stresses and free edge stresses Introduction Development of classical analysis Finite element analysis of straight edges Finite element analysis of curved edges Summary References
123 123 126 129 130 135 136
8 8.1 8.2 8.3 8.4 8.5 8.6 8.7
Fracture and fracture mechanics Introduction Crack tip behaviour in homogeneous solids Crack extension in composites Application of fracture mechanics to composites Progressive failure models Summary References
139 139 140 142 146 155 156 157
9 9.1 9.2 9.3 9.4 9.5 9.6 9.7
Delamination Introduction A continuum model Twodimensional finite element analysis Discussion of VCC results Finite element analysis using interface elements Summary References
158 158 159 164 168 171 172 173
10
Joining Introduction Adhesively bonded joints Mechanically fastened joints Summary References
175 175 175 183 190 191
11
Fatigue Introduction Damage modes in composite laminates Fatigue of unidirectional laminates Fatigue of multidirectional laminates Fatigue damage effects on mechanical properties
194 194 194 196 198 201
10.1 10.2 10.3 10.4 10.5 11.1 11.2 11.3 11.4 11.5
vi
11.6 11.7 11.8 11.9
Contents Fatigue damage modelling A finite element model for fatigue life prediction of CFRP components Summary References
203
Index
211
204 207 208
Preface
The Centre for Composite Materials at Imperial College has for many years organised a series of training courses on various aspects of composite materials. In 1996, recognising the increasing interest in structural analysis, a new course on ‘Finite Element Analysis of Composites’ was launched. The course was given jointly by the Centre and the Department of Aeronautics, and supported by the Engineering & Physical Sciences Research Council (EPSRC) as an MSc level module. This book is based on the lecture notes prepared for the above course. The emphasis throughout is on long fibrereinforced polymer (FRP) matrix composites, although any general analysis would be applicable to other forms of composite. The book starts with a review of the basic behaviour of FRP. Then, the fundamentals of finite element (FE) analysis are rehearsed. Following this, special issues relating to the applications of FE to FRP are discussed. Finally, a number of particular situations, such as holes and free edges, are presented, with FE results set alongside classical analysis and experimental data.
vi i
This page intentionally left blank
Authors
The authors of this text are all from the Imperial College of Science Technology & Medicine, University of London. Prof. F. L. Matthews Prof. G. A. 0. Davies Mr D. Hitchings Dr C. Soutis
Director, Centre for Composite Materials Senior Research Fellow & Senior Research Investigator, Department of Aeronautics Senior Lecturer, Department of Aeronautics Reader, Department of Aeronautics
ix
Acknowledgement
The authors, and especially E L. Matthews in his editorial role, are indebted to Mrs Sabine Grune von Stieglitz for her invaluable contribution in assembling this book from a multitude of electronic and paper sources.
X
Part I Overview and review of composite materials F. L. MATTHEWS
This part serves merely to ‘set the scene’ for the remainder of the book and also to revise the fundamentals of composite materials. The basic nature of fibrereinforced plastic and its constituents is reviewed. Following this, twodimensional stress–strain analysis is covered, leading to laminated plate theory. Finally some limitations of the latter are discussed.
This page intentionally left blank
1 Overview
1.1
Composite materials
1.1.1 General The group of materials known as ‘composites’ is extremely large, although its boundaries depend on definition. Basically, we can consider a composite as any material that is a combination of two or more distinct constituents. This definition would encompass bricks, concrete, wood, bone, as well as modern synthetic composites such as fibrereinforced plastics (FRP). The latter have become increasingly important over the past 50 years, and are now the first choice for fabricating structures where low weight in combination with high strength and stiffness are required. Such materials are sometimes referred to as ‘highperformance’ composites, and would often be composed of carbon fibres and epoxy resin. Of course, composites can also be made by combining fibres with a metal or a ceramic matrix, but at the moment these have a very small market share and would be considered as specialist materials.
1.1.2 Properties and applications Density, stiffness (modulus) and strength are the properties that initially come to mind when thinking of FRP, and these would certainly be the design drivers for materials’ selection for transport applications such as aircraft, motor vehicles and trains. However, this is a very narrow view of the potential of such materials, and they often score over metals and other conventional materials because of other mechanical, physical or chemical properties. For example, FRPs are extremely corrosionresistant and are, in consequence, used for chemical plant, water transport and storage, and flue gas desulphurisation plant. They have interesting electromagnetic properties and because of this glass fibrereinforced resin is used to construct mine 3
4
Overview and review of composite materials
counter measures naval vessels, the requirement being a nonmagnetic material. As another illustration, carbon fibrereinforced epoxy is used in medical applications because it is transparent to Xrays. Thermal properties can also be important; such materials have a low conductivity, making them useful for fire protection, and can have a zero coefficient of expansion, hence making possible the construction of temperaturestable components. A key issue is that of cost. Although the constituents of FRP are relatively expensive, compared with conventional materials, the final component may well be less costly than one fabricated from metal, say. This is due, in part, to having a more integrated construction (lower ‘parts count’), but depends crucially on the level of automation in the manufacturing process.
1.1.3 Production methods The important factor about FRP is that, unlike metals, the material is made at the same time as the component. While this gives an increased freedom to the design process, it does mean that designers/analysts must pay close attention to the fabrication of the component or structure. The same constituents if processed by one method, could produce a composite with some properties modified compared with those produced by another method. Also, it is important to realise that the designer may call for a particular configuration that cannot actually be fabricated; for example, it is not possible to maintain a constant fibre angle and wall thickness along the length of a tapered cylinder produced by filament winding. Good communication at all levels throughout the whole design/fabrication/evaluation process is, therefore, essential.
1.2
Structural analysis
1.2.1 Classical analysis The use of classical (continuum) methods of stress analysis has developed over many decades to give techniques that can be applied satisfactorily to a vast range of situations. Such analyses are based on the application of the equations of equilibrium and compatibility, together with the stress–strain relations for the material, to produce governing equations which must be solved to obtain displacements and stresses. Usually, assumptions must be made before a solution can be effected. So, for example, problems are considered as one or twodimensional, as when considering beams and plates, respectively. Often we take the material to be isotropic, but many analyses also exist for anisotropic materials.
Overview
5
As we move away from simple situations, say from a plain rectangular plate to one containing a cutout, the governing equations become increasingly complicated and require evermore sophisticated mathematical techniques to solve them. Classical methods are limited to simple geometries and ‘real’ structural features, e.g. the details of attachment of a stringer to a skin panel, cannot be analysed. In such cases we have to resort to finite element methods.
1.2.2 Finite element analysis Finite element (FE) analysis is merely an alternative approach to solving the governing equations of a structural problem. Hence, FE and classical methods will produce identical results for the same problem, provided the former method is correctly applied. The method consists of imagining the structure to be composed of discrete parts (i.e. finite elements), which are then assembled in such a way as to represent the distortion of the structure under the specified loads. Each element has an assumed displacement field, and part of the skill of applying the method is in selecting appropriate elements of the correct size and distributions (the FE ‘mesh’). The FE method was initially developed for isotropic materials and the majority of elements available (the ‘library’) in any software package would be for such materials. To apply the technique to composites requires different element formulations that adequately represent their anisotropic, or orthotropic, stiffness and strength, as well as the laminated form of construction often used. The main purpose of this book is to discuss the special issues that must be considered when using the FE method to analyse composite materials and structures. One of the key factors is the low throughthickness stiffness and strength; the former results in the need to adapt elements used for plates, and the latter results in the need to model delamination. Also some features of composite construction, such as filament winding, cannot easily be represented (if at all) by some FE packages. Following a review of composites and the FE method, the application of the method to composites is discussed in detail. The particular issues are then illustrated via a number of examples taken from particular situations.
2 Fundamentals of composites
2.1
Basic characteristics
2.1.1 Definitions and classification A composite is a mixture of two or more distinct constituents or phases. In addition three other criteria are normally satisfied before we call a material a composite. Firstly, both constituents have to be present in reasonable proportions. Secondly, the constituent phases should have distinctly different properties, such that the composite’s properties are noticeably different from the properties of the constituents. Lastly, a synthetic composite is usually produced by deliberately mixing and combining the constituents by various means. We know that composites have two (or more) chemically distinct phases on a microscopic scale, separated by a distinct interface, and it is important to be able to specify these constituents. The constituent that is continuous and is often, but not always, present in the greater quantity in the composite is termed the matrix. The normal view is that it is the properties of the matrix that are improved upon when incorporating another constituent to produce a composite. A composite may have a ceramic, metallic or polymeric matrix. The mechanical properties of these three classes of material differ considerably. As a generalisation, polymers have low strengths and Young’s moduli, ceramics are strong, stiff and brittle, and metals have intermediate strengths and moduli, together with good ductilities, i.e. they are not brittle. Because of their economic importance, the emphasis in this text will be on polymer matrix composites (PMCs). The second constituent is known to as the reinforcing phase, or reinforcement, as it enhances or reinforces the mechanical properties of the matrix. In most cases the reinforcement is harder, stronger and stiffer than the matrix, although there are some exceptions; for example, ductile metal reinforcement in a ceramic matrix and rubberlike reinforcement in a brittle polymer matrix. At least one of the dimensions of the reinforcement is 6
Fundamentals of composites
7
Composite material
A Fibrereinforced composites (fibrous composites)
Particlereinforced composites (particulate composites)
B C
Singlelayer composites (including composites having same orientation & properties in each layer)
E
Multilayered (angleply composites)
Laminates Continuous fibrereinforced composites
Random orientation
Preferred orientation
Hybrids
Discontinuous fibrereinforced composites
D Random Unidirectional Bidirectional orientation reinforcement reinforcement (woven reinforcements)
Preferred orientation
2.1 Classification of composite materials.
small, say less than 500 mm and sometimes only of the order of a micrometre. The geometry of the reinforcing phase is one of the major parameters in determining the effectiveness of the reinforcement; in other words, the mechanical properties of composites are a function of the shape and dimensions of the reinforcement. We usually describe the reinforcement as being either fibrous or particulate. Figure 2.1 represents a commonly employed classification scheme for composite materials which utilizes this designation for the reinforcement (Fig. 2.1, block A). Particulate reinforcements have dimensions that are approximately equal in all directions. The shape of the reinforcing particles may be spherical, cubic, platelet or any regular or irregular geometry. The arrangement of the particulate reinforcement may be random or with a preferred orientation, and this characteristic is also used as a part of the classification scheme (block B). In the majority of particulatereinforced composites the orientation of the particles is considered, for practical purposes, to be random. A fibrous reinforcement is characterized by its length being much greater than its crosssection dimensions. However, the ratio of length to a crosssection dimension, known as the aspect ratio, can vary considerably. In singlelayer composites long fibres with high aspect ratios give what are called continuous fibrereinforced composites, whereas discontinuous fibre composites are fabricated using short fibres of low aspect ratio (block C). The orientation of the discontinuous fibres may be random or preferred. The frequently encountered preferred orientation in the case of a continuous fibre composite is termed unidirectional and the corresponding random
8
Overview and review of composite materials
situation can be approximated to by bidirectional woven reinforcement (block D). Multilayered composites are another category, and commonly used form, of fibrereinforced composites. These are classified as either laminates or hybrids (block E). Laminates are sheet constructions which are made by stacking layers (also called plies or laminae and usually unidirectional) in a specified sequence. The layers are often in the form of ‘prepreg’ (fibres preimpregnated with partly cured resin) which are consolidated in an autoclave. A laminate may have between 4 and 400 layers and the fibre orientation changes from layer to layer in a regular manner through the thickness of the laminate, e.g. a 0/90/0 stacking sequence results in a crossply composite. We shall refer in detail to the stress analysis of laminates in Chapter 3. Hybrids are composites with mixed fibres and are becoming commonplace. The fibres may be mixed within a ply or layer by layer, and these composites are designed to benefit from the different properties of the fibres employed. For example, a mixture of glass and carbon fibres incorporated into a polymer matrix gives a relatively inexpensive composite, owing to the low cost of glass fibres, but with mechanical properties enhanced by the excellent stiffness of carbon.
2.1.2 The matrix and reinforcement Most composites are designed to exploit an improvement in mechanical properties. Even for composites produced essentially for their physical properties, the mechanical properties can play an important role during component manufacture and service. The strengths of fibres are generally much higher than those of their monolithic counterparts owing to the presence of defects in the latter. There are of course many properties other than strength that we have to take into account when selecting a reinforcement. In the case of fibres the flexibility is important as it determines whether the fibres may be easily woven or not, and influences the choice of method for composite manufacture. The flexibility of a fibre depends on Young’s modulus and the diameter of the fibre, decreasing as diameter increases. Clearly, single fibres, because of their small crosssection dimensions, are not directly usable in structural applications. This problem may be overcome by embedding the fibres in a material to hold the fibres apart, to protect the surface of the fibres, and to facilitate the production of components. The embedding material is the matrix. The amount of reinforcement that can be incorporated in a given matrix is limited by a number of factors. For example with particulatereinforced metals the reinforcement content is usually kept to less than 40 vol% (0.4 volume fraction) owing to
Fundamentals of composites
9
processing difficulties and increasing brittleness at higher contents. On the other hand, the processing methods for fibrereinforced polymers are capable of producing composites with a high proportion of fibres, and the upper limit of about 70 vol% (0.7 volume fraction) is set by the need to avoid fibre–fibre contact, which results in fibre damage. Finally, the fact that the reinforcement is bonded to the matrix means that any loads applied to a composite are carried by both constituents. As in most cases the reinforcement is the stiffer and stronger constituent, it is the principal loadbearer. The matrix is said to have transferred the load to the reinforcement.
2.1.3 Factors that determine properties The fabrication and properties of composites are strongly influenced by the proportions and properties of the matrix and the reinforcement. The proportions can be expressed either via the weight fraction (w), which is relevant to fabrication, or via the volume fraction (v), which is commonly used in property calculations. The definitions of w and v are related simply to the ratios of weight (W) or volume (V) as shown below. Volume fractions: vf = Vf Vc
and vm = Vm Vc
[2.1a]
Weight fractions: wf = Wf Wc
and wm = Wm Wc
[2.1b]
where the subscripts m, f and c refer to the matrix, fibre (or in the more general case, reinforcement) and composite respectively. We note that: vf + vm = 1 and wf + wm = 1 We can relate weight to volume fractions by introducing the density, r, of the composite and its constituents. We can show that: rc = rfvf + rmvm
[2.2]
1 wf wm = + rc r f rm
[2.3]
and
10
Overview and review of composite materials
Also we have: wf =
Wf r f Vf Ê r f ˆ = = vf Wc rcVc Ë rc ¯
and similarly wm =
Wm rm Vm Ê rm ˆ = = vm Wc rcVc Ë rc ¯
[2.4]
We can see that we can convert from weight fraction to volume fraction, and vice versa, provided the densities of the reinforcement (rf) and the matrix (rm) are known. The chemical and strength characteristics of the interface between the fibres and the matrix are particularly important in determining the properties of the composite. The interfacial bond strength has to be sufficient for load to be transferred from the matrix to the fibres if the composite is to be stronger than the unreinforced matrix. On the other hand, if we are also concerned with the toughness of the composite, the interface must not be so strong that it does not fail and allow toughening mechanisms such as debonding and fibre pullout to take place. Other parameters that may significantly affect the properties of a composite are the shape, size, orientation and distribution of the reinforcement, and various features of the matrix such as the grain size for polycrystalline matrices. These, together with volume fraction, constitute what is called the microstructure of the composite. The volume fraction is generally regarded as the single most important parameter influencing the composite’s properties. Also, it is an easily controllable manufacturing variable by which the properties of a composite may be altered to suit the application. A problem encountered during manufacture is maintaining a uniform distribution of the reinforcement. Ideally, a composite should be homogeneous, or uniform, but this is difficult to achieve. Homogeneity is an important characteristic that determines the extent to which a representative volume of the material may differ in physical and mechanical properties from the average properties of the material. Nonuniformity of the system should be avoided as much as possible because it reduces those properties that are governed by the weakest part of the composite. The orientation of the reinforcement within the matrix affects the isotropy of the system. When the reinforcement is in the form of equiaxial particles, the composite behaves essentially as an isotropic material whose properties are independent of direction. When the dimensions of the reinforcement are unequal, the composite can behave as if isotropic provided the reinforcement is randomly oriented, as in a randomly oriented short fibrereinforced composite. In other cases the manufacturing process may
Fundamentals of composites
11
Table 2.1 Typical properties of some artificial fibres Density (Mg/m3) r
Young’s modulus (GPa) Ef
Tensile strength (MPa) sˆ Tf
Failure strain (%)
Eglass
2.54
70
2200
3.1
Aramid (Kevlar 49)
1.45
130
2900
2.5
SiC (Nicalon)
2.60
250
2200
0.9
Alumina (FP)
3.90
380
1400
0.4
Boron
2.65
420
3500
0.8
Polyethylene (S1000)
0.97
172
2960
1.7
Carbon (HM)
1.86
380
2700
0.7
induce orientation of the reinforcement and hence loss of isotropy; the composite is then said to be anisotropic. In components manufactured from continuous fibrereinforced composites, such as unidirectional or crossply laminates, anisotropy may be desirable as it can be arranged for the maximum service stress to be in the direction that has the highest strength. Indeed, a primary advantage of these composites is the ability to control the anisotropy of a component by design and fabrication.
2.2
Fibres and matrices
2.2.1 Fibres We have seen that the reinforcement in a composite may be fibrous or particulate. A wide range of both these forms of reinforcement is available for use in the production of composite materials but most of the major developments in recent times have been in the area of fibrous reinforcement. The underlying philosophy in the design of fibre composite materials is to find or to make a fibre material of high elastic modulus and strength, and preferably low density, and then to arrange the fibres in a suitable manner to give useful engineering properties to the final product. Many different fibres are manufactured for the reinforcement in composites and some typical properties are given in Table 2.1.1 The values for stiffness and strength given in the table should be viewed with some caution. The manufacture of the fibres involves a number of processing steps and variability of properties from one fibre to another can be large, even when made by the same process. Between fibres of the same material
12
Overview and review of composite materials
made by different processes, the resulting microstructure and properties can differ even more markedly. Furthermore, the high tensile strength of freshly made fibres is normally reduced by surface damage caused during subsequent handling and storage. Finally, any variation in size leads to a range of strength values. Most fibres are brittle and show only elastic extension before fracture.
2.2.2 Synthetic organic fibres The organic reinforcement market is dominated by aramid fibres, although there is increasing interest in polyethylene fibres.
2.2.2.1 Aramid There are a number of commercially available aramid fibres, e.g. Kevlar (Du Pont), Twaron (Akzo) and Technora (Teijin); of these Kevlar is the most well known. The aramids can be viewed as nylon with extra benzene rings in the polymer chain to increase stiffness. Alternative nomenclature that the reader might encounter is aromatic polyamide or poly(phenylene teraphthalamide). Aramid fibres have good high temperature properties for a polymeric material. They have a glass transition temperature of about 360 °C, burn with difficulty and do not melt like nylon. A loss in performance due to carburation occurs around 425 °C but they can be used at elevated temperatures for sustained periods and even at 300 °C for a limited time. Aramid fibres do have a tendency to degrade in sunlight and when exposed to moisture. Also, they have low compressive strength. Their dimensional stability is good as the coefficient of thermal expansion is low (approximately 4 ¥ 106 K1). Other properties that are important in certain applications are low electrical and thermal conductivity and high thermal capacity.
2.2.2.2 Polyethylene In the late 1980s a number of polyethylene fibres became commercially available including Spectra (Allied Signal) and Dyneema (DSM). Polyethylene has the lowest density of any readily available fibre (about 0.97 Mg/m3) and hence its specific properties are good and superior to those of Kevlar. However, polyethylene has a low melting point of 135 °C and readily creeps at elevated temperature, so use is restricted to temperatures below 100 °C.
Fundamentals of composites
13
2.2.3 Synthetic inorganic fibres 2.2.3.1 Glass Glass is a noncrystalline material with a shortrange network structure. As such it has no distinctive microstructure and the properties, which are determined mainly by composition and surface finish, are isotropic. There are many groups of glasses, for example silica, oxynitride, phosphate and halide glasses, but from the point of view of composite technology only the silica glasses are currently of importance. However, even within this group of glasses the composition, and hence properties, vary considerably. The most commonly used glass fibre is Eglass, the E being an abbreviation for ‘electrical’. This glass is based on the ternary system CaO–Al2O3– SiO2. Freshly drawn and carefully handled fibres have tensile strengths of approximately Ef/20 but a typical value may be nearer to Ef/50, where Ef is Young’s modulus (typically about 70 GPa). Sglass, known as Rglass in Europe, is based on the SiO2–Al2O3–MgO system. This fibre has higher stiffness and strength (hence the designation S) than Eglass. It also retains its improved properties to higher temperatures. However, it is more difficult to draw into fibres because of its limited working range and is therefore more expensive. Although the performance of the widely used generalpurpose Eglass is satisfactory in near neutral aqueous solutions, it is liable to degradation in environments which are highly acidic or alkaline.
2.2.3.2 Carbon Carbon fibres are produced by many companies and the world production capacity exceeds 20 000 tonnes. In spite of this large production capacity carbon fibres are still relatively expensive. Nevertheless the usage for carbon fibres continues to increase, and many companies have recently increased their production capacity. The structure and properties of these fibres vary considerably and new fibres are always under test. For example two recent introductions are hollow fibres and coiled fibres. The former are designed to impart better impact toughness to carbonreinforced polymers, whereas the latter are capable of extending many times their original length without loss of elasticity. Carbon has two wellknown crystalline forms (diamond and graphite) but it also exists in quasicrystalline and glassy states. As far as fibre technology is concerned, graphite is the most important structural form of carbon. The graphitic structure consists of strongly bonded hexagonal layers, which are called the basal planes, with weak interlayer van der Waals bonds.
14
Overview and review of composite materials
Alignment of the basal planes parallel to the fibre axis gives stiff fibres with relatively low density. Graphite sublimes at 3700 °C but starts to oxidise in air at around 500 °C; carbon fibres can, however, be used at temperatures exceeding 2500 °C if protected from oxygen. Carbon is a good electrical conductor which, depending on the circumstances, can be advantageous or not. Carbon fibres are produced from a variety of precursors. The mechanical properties vary greatly with the precursor used and the processing conditions employed, as these determine the perfection and alignment of the crystals. The main precursors are polyacrylonitrile (PAN) and pitch. An unusual characteristic of carbon fibres is their very low, or even slightly negative, coefficient of longitudinal expansion. As for other properties, the coefficient of thermal expansion depends on the fabrication route and hence degree of graphitization and crystal orientation. Ultrahigh modulus carbon fibres have negative coefficients of expansion of approximately 1.4 ¥ 106 K1 and are employed in the production of polymer matrix composites with nearzero thermal expansion.
2.2.4 Polymer matrices The most common matrix materials for composites are polymeric. The reasons for this are twofold. Firstly, in general the mechanical properties of polymers are inadequate for many structural purposes. In particular their strength and stiffness are low compared with metals and ceramics. This means that there is a considerable benefit to be gained by reinforcing polymers, and that the reinforcement does not have to have exceptional properties. Secondly, and most importantly, the processing of polymer matrix composites (PMCs) need not involve high pressures and does not require high temperatures. It follows that problems associated with the degradation of the reinforcement during manufacture are less significant for PMCs than for composites with other matrices. Also the equipment required for PMCs may be simpler. There are three classes of polymers, thermosets, thermoplastics and rubbers, all important as far as matrices of PMCs are concerned. Rubbers will not be dealt with here, although they constitute an important group, being widely used in reinforced form in motor car tyres, for example. Within any class there are many different polymers, e.g. epoxy, polyester, polyimide and phenolic are all thermosets. Even a given polymer, such as a polyester, exists in many forms; there are a large number of formulations, curing agents and fillers, which results in an extensive range of properties for polyesters. Indeed, polyesters, and other polymers, are often marketed according to their properties by the employment of descriptive terms including
Fundamentals of composites
15
Table 2.2 Some typical properties of polymer matrices Epoxy
Nylon (6.6)
Polycarbonate
Polyester
Density (Mg/m3)
1.1–1.4
1.1
1.1–1.2
1.1–1.5
Young’s modulus (GPa)
2.1–6.0
1.4–2.8
2.2–2.4
1.3–4.5
Tensile strength (MPa)
35–90
60–70
45–70
45–85
30–100
90–110
Ductility (%) Fracture toughness KIC (MPa m1/2) GIC (kJ/m2)
0.6–1.0 0.02
Thermal expansion (106 K1)
55–110
Glass transition temperature (°C) Melting point (°C)
0.5
90
120–190
100–200 150
261
‘general purpose’, ‘chemically resistant’ and ‘heat resistant’. Bearing in mind also the variety of materials used for reinforcement, and the possible arrangements of the reinforcement (random chopped fibres, unidirectional, numerous weaves, etc.) it is clear that the range of properties exhibited by PMCs is quite remarkable. The main disadvantages of PMCs are their low maximum working temperatures, high coefficients of thermal expansion and hence dimensional instability, and sensitivity to radiation and moisture.The absorption of water from the environment may have many harmful effects which degrade mechanical performance, including swelling, formation of internal stresses and lowering of the glass transition temperature. It has been estimated that over threequarters of all matrices of PMCs are thermosetting polymers. Thermosetting polymers, or thermosets, are resins that readily crosslink during curing. Curing involves the application of heat and pressure, or the addition of a catalyst known as a curing agent or hardener. Thermosets are brittle at room temperature and have low fracture toughness values. Also, because of the crosslinks, thermosets cannot be reheated and reshaped; thermosets just degrade on reheating, and in some cases may burn, but do not soften sufficiently for reshaping. Thermosets may be used at higher temperatures as they have higher softening temperatures and better creep properties than thermoplastics. Finally, they are more resistant
16
Overview and review of composite materials
to chemical attack than most thermoplastics. Typical properties are given in Table 2.2.1 Thermoplastics readily flow under stress at elevated temperatures, so allowing them to be fabricated into the required component, and become solid and retain their shape when cooled to room temperature. These polymers may be repeatedly heated, fabricated and cooled and consequently scrap may be recycled, though there is evidence that this slightly degrades the properties, probably because of a reduction in molecular weight. Wellknown thermoplastics include acrylic, nylon (polyamide), polystyrene, polyethylene, polypropylene and polyetheretherketone. Some typical properties are given in Table 2.2.
2.3
Summary
Polymer matrix composites (PMCs) are the best established form of advanced composite materials. Of the three classes of polymers used as matrices, thermosets, thermoplastics and rubbers, thermosets dominate the market for structural applications. The mechanical properties of PMCs can vary widely depending on the choice of fibre and matrix, the coating applied to the fibres, and the manufacturing route. The main reason for the popularity of PMCs is their ease of processing.
2.4
Reference
1 Matthews F L & Rawlings R D, Composite Materials: Engineering and Science, Cambridge, Woodhead, 1999.
3 Stiffness and strength of composites
3.1
Stiffness of unidirectional composites and laminates
3.1.1 Introduction When analysing composite structures using finite elements we need to supply to the software appropriate input data for the material being used. Typically for composites we shall need moduli and strength of the single plies that constitute a laminate. Occasionally we may input the laminate properties directly. In this chapter we shall address the essential background relating to the above issues. Initially we shall work with ‘macromechanics’ in which case we ignore the details of the fibres and matrix and their interactions. Later in the chapter we shall look at these interactions in what is known as ‘micromechanics’. When calculating the mechanical properties of composites it is convenient to start by considering a composite in which all the fibres are aligned in one direction (i.e. a unidirectional composite). This basic ‘building block’ can then be used to predict the behaviour of continuous fibre multidirectional laminates, as well as short fibre, nonaligned systems. The essential point about a unidirectional fibre composite is that its stiffness (and strength) are different in different directions. This behaviour contrasts with a metal with a random orientation of grains, or other isotropic material, which has the same elastic properties in all directions. In a unidirectional composite the fibre distribution implies that the behaviour is essentially isotropic in a crosssection perpendicular to the fibres (Fig. 3.1). In other words, if we were to conduct a mechanical test by applying a stress in the ‘2’ direction or in the ‘3’ direction (both normal to the fibre’s longitudinal axis), we would obtain the same elastic properties from each test. We say the material is ‘transversely isotropic’. Clearly the properties in the longitudinal (‘1’) direction are very different from those 17
18
Overview and review of composite materials
3.1 Orientation of principal material axes.
in the other two directions. We call such a material ‘orthotropic’. The elastic properties are symmetric with respect to the chosen (1–2–3) axes, which are usually called the ‘principal material axes’.
3.1.2 Basic stress–strain relations The stress–strain relations for the unidirectional material can readily be found, provided we take account of the fact that the properties are directiondependent. Considering the composite illustrated in Fig. 3.1, we see that if the directions of the applied stresses coincide with the principal material axes (‘specially orthotropic’), the strains in terms of the stresses are given by s1 s2  u 21 E11 E22 s1 s2 e 2 =  u12 + E11 E22 t 12 g 12 = G12 e1 =
[3.1]
where E11 is the elastic modulus in the ‘1’, or longitudinal direction E22 is the elastic modulus in the ‘2’, or transverse direction G12 is the shear modulus in the 1–2 axes u12 is the ‘major’ Poisson’s ratio u21 is the ‘minor’ Poisson’s ratio It should be clear that u12 gives the transverse (‘2’ direction) strain caused by a strain applied in the longitudinal (‘1’) direction; conversely for u21. Because of the presence of the high stiffness fibres we would intuitively expect u12 to be larger than u21. This is confirmed by a fundamental law of elasticity which shows that
Stiffness and strength of composites
19
Table 3.1 Representative elastic properties of unidirectional fibrereinforced epoxy resins u12
G12 (GPa)
8.96
0.30
7.10
200.0
11.10
0.32
8.35
0.46
39.5
8.22
0.26
4.10
0.60
76.0
5.50
0.33
2.35
Material
Fibre volume fraction vf
E11 (GPa)
E22 (GPa)
CFRP (AS fibre)
0.66
138.0
CFRP (IM6 fibre)
0.65
GFRP (Eglass fibre) KFRP (Kevlar49 fibre)
u12 u 21 = E11 E22 E11 or u12 = u 21 E22 E11 and as > 1, u12 > u 21 E22
[3.2]
To get stresses in terms of strains we can rearrange equation [3.1] to give u 21E11e 2 E11e 1 + 1  u12 u 21 1  u12 u 21 u12 E22 e 1 E22 e 2 s2 = + 1  u12 u 21 1  u12 u 21 t 12 = G12 g 12 s1 =
[3.3]
Representative, experimentally determined, values of elastic properties are given in Table 3.1 for carbon, glass and Kevlar fibrereinforced epoxy resins (CFRP, GFRP, KFRP respectively). As we shall see later, it is sometimes possible to calculate elastic constants from the properties of the fibre and matrix using micromechanics. The important point to note from equations [3.1] and [3.3] is that we need four elastic constants to characterise our unidirectional composite; E11, E22, u12 (or u21) and G12. Contrast this with an isotropic material where only two quantities are needed. For the composite the shear modulus cannot be calculated from E and u, as it can for isotropic materials. For convenience when dealing with laminates it is helpful to rewrite equations [3.1] and [3.3] in matrix form. So [3.1] becomes
20
Overview and review of composite materials
e12 = Ss12 where e12 = {e1 e2 g12} and s12 = {s1 s2 t12}
[3.4]
Note that { } denotes a column vector written as a row vector and we define the compliance matrix È 1 Í E11 Í u12 S = ÍÍ E11 Í Í 0 Î
u 21 E22 1 E22

0
˘ 0 ˙ ˙ 0 ˙ ˙ 1 ˙ ˙ G12 ˚
Note that S12 = S21 and [3.3] becomes s12 = Qe12
[3.5]
where the stiffness matrix is defined by È E11 Í 1  u12 u 21 Í u12 E22 Q=Í Í 1  u12 u 21 Í 0 Í Î
u 21E11 1  u12 u 21 E22 1  u12 u 21 0
˘ 0 ˙ ˙ 0 ˙ ˙ G12 ˙ ˙ ˚
Note that Q12 = Q21. We see that the first column of S gives the strains caused by a unit value of s1, the second column of Q gives the stresses needed to cause a unit value of e2, and so on. It should be clear from the properties of matrices that Q = S1.
3.1.3 Offaxis loading of a unidirectional composite In later sections we shall refer frequently to laminates. As noted in Chapter 2, these platelike entities are often constructed by assembling layers (or laminae, or plies), usually unidirectional, one on top of another, the direction of the fibres normally being changed from layer to layer. Consequently there will be layers for which the fibres are no longer aligned with the applied stresses (the situation considered in the previous section). We term these ‘rotated layers’ and say that they are subjected to ‘offaxis loading’.
Stiffness and strength of composites y
21
y
1
xy
2
x
x
Fibres
3.2 Unidirectional lamina with principal axes rotated by q relative to the x–y axes.
To prepare ourselves for the analysis of laminates, it is useful at this stage to consider in isolation one of these rotated laminae. The situation, which is illustrated in Fig. 3.2, is seen to correspond to the analysis of principal stress for isotropic materials. We can write, then [3.6] [3.7]
s 12 = Ts xy and
e 12 = T e xy
where s 12 = {s1 s 2 t 12 } s xy = {s x s y t xy } e 12 = {e 1 e 2
1 2
g 12 }
e xy = {e x e y
1 2
g xy }
and the transformation matrix 2 2 mn ˘ n2 Èm Í 2 2 T= n m 2 mn ˙ Í ˙ ÍÎ mn mn (m 2  n 2 )˙˚
[3.8]
with m = cos q and n = sin q. As with any elasticity analysis we wish to determine the strains for a known set of applied stresses (or vice versa). We can do this provided we
22
Overview and review of composite materials
know the elastic properties of the material. The situation we are faced with here is that while we know the properties referred to the 1–2 axes, we do not know them with reference to the x–y axes. So, before we can solve the problem, we need to do some mathematical manipulation, which leads eventually to:1 sxy = Q exy
[3.9]
The transformed stiffness matrix is Q , the elements of which are Q11 = Q11 m 4 + 2(Q12 + 2Q33 ) n 2 m 2 + Q22 n 4 Q22 = Q11 n 4 + 2(Q12 + 2Q33 ) n 2 m 2 + Q22 m 4 Q12 = (Q11 + Q22  4Q33 ) n 2 m 2 + Q12 ( m 4 + n 4 ) Q33 = (Q11 + Q22  2Q12  2Q33 ) n 2 m 2 + Q33 ( m 4 + n 4 ) Q13 = (Q11  Q12  2Q33 ) nm 3 + (Q12  Q22 + 2Q33 ) n 3 m Q23 = (Q11  Q12  2Q33 ) n 3 m + (Q12  Q22 + 2Q33 ) nm 3
[3.10]
We see that knowledge of the orientation (q) and unidirectional properties (Q) in the principal directions enables us to calculate the stiffness of the rotated lamina. In the general form derived we would call this a ‘generally orthotropic lamina’. If conditions are such that Q13 = Q23 = 0, we have what is called a ‘specially orthotropic lamina’. If we require strains in terms of stresses then we invert equation [3.9] to give e xy = Q 1s xy or
e xy = S s xy
[3.11]
where S is the transformed compliance matrix, the elements of which can be obtained by a similar process to that used for finding the elements of Q , i.e. S11 = S11 m 4 + (2 S12 + S33 )n 2 m 2 + S 22 n 4 S 22 = S11 n 4 + (2 S12 + S33 )n 2 m 2 + S 22 m 4 S12 = (S11 + S 22  S33 )n 2 m 2 + S12 (m 4 + n 4 ) S33 = 2(2 S11 + 2 S 22  4 S12  S33 )n 2 m 2 + S33 (m 4 + n 4 ) S13 = (2 S11  2 S12  S33 )m3 n + (2 S12  2 S 22 + S33 )mn3 S 23 = (2 S11  2 S12  S33 )n3 m + (2 S12  2 S 22 + S33 )m3 n
[3.12]
For general loading of an offaxis ply we see that in addition to an extension in the direction of the applied stress and a lateral contraction, as we would expect, there is also a shear strain. This phenomenon, which is known as extensionshear coupling, would not be observed with an isotropic material. We see that the shear strain is determined by the S13 term, when only
Stiffness and strength of composites
23
sx is acting. Had we applied only sy, there would have been a shear strain arising from the S23 term. In other words there will be no extensionshear coupling if S13 = S23 = 0. This is clearly the case when the fibres of a unidirectional layer are parallel to the stress axes, i.e. q = 0 or 90°. It is also possible for S13 and S23 to be zero with fibres at intermediate angles; whether, or not, this occurs depends on the relative values of E11, E22 and G12.
3.1.4 Stiffness of laminates Thin sheet constructions, known as laminates, are an important class of composite. They are made by stacking together, usually, unidirectional layers (also called plies or laminae) in predetermined directions and thicknesses to give the desired stiffness and strength properties. Such constructions are frequently encountered. The skins of aeroplane wings and tails, the hull sides and decking of ships, the sides and bottom of water tanks are typical examples. Even cylindrical components, such as filament wound tanks, can be treated as laminates, provided the radiustothickness ratio is sufficiently large (say >50). Laminates will be typically between 4 and 40 layers, each ply being around 0.125 mm thick if it is carbon or glass fibre/epoxy prepreg. Typical layups (the arrangement of fibre orientations) are crossply, angle ply and quasiisotropic. When making a laminate we must decide on the order in which the plies are placed through the thickness (known as the stacking sequence). This has an important influence on the flexural performance of the laminate. There is an established convention for denoting both the layup and stacking sequence of a laminate. Thus, a fourply crossply laminate which has ply fibre orientations in the sequence 0°, 90°, 90°, 0° from the upper to the lower surface, would be denoted (0/90°)s. The suffix ‘s’ means that the stacking sequence is symmetric about the midthickness of the laminate. Laminates denoted by (0/45/90°)s and (45/90/0°)s have the same layup but different stacking sequences. The way in which they are used means that laminated plates may be subjected to both inplane and transverse (normal to the plate) loading. In other words they will stretch and bend, and both these effects must be taken into account when describing the overall behaviour of the plate. The two effects are separated by considering the total strain to be the superposition of inplane strains, e°, constant across the plate thickness, and strains caused by bending, linear across the thickness, as shown in Fig. 3.3. The bending strains can be defined in terms of the plate curvatures. For example, ex = zkx, z being the coordinate normal to the plate measured from the laminate midplane, and is positive downwards (as shown in Fig. 3.3).
24
Overview and review of composite materials
kz z
3.3 The two components of laminate strain: e°, inplane, constant over the thickness; ex = zkx, bending, linear variation over the thickness.
1 hj z
hj –1 tj
j p
3.4 Definition of plies within a laminate.
So we have
or
∞ È ex ˘ È e x ˘ Èk x ˘ Í e ˙ = Í e ∞ y ˙ + zÍ k ˙ ˙ Í y˙ Í y˙ Í ÍÎg xy ˙˚ ÍÎg ∞ xy ˙˚ ÍÎk xy ˙˚
[3.13]
exy = e° + zk
[3.14]
Because all the plies are bonded together in the manufacturing process, we assume that they each have the same inplane strains and curvatures. So, for any one layer, say the jth (Fig. 3.4) we have, using equation [3.9], s xyj = Q j e ∞ + z Q j k
[3.15]
Q j being the transformed stiffness matrix for the layer. Note that the stresses act in the plane of the laminate. These stresses can be converted to equivalent forces (or stress resultants) acting on a unit width of plate. So, for example, from sx we get Nxj = sxj tj, tj being the thickness of layer j. If we add up the resultants for all the plies the total must be equal to the external force (per unit width) acting on the plate (see Fig. 3.5). Similarly, the equivalent force on a layer will have a moment about the midplane. Again using sx only to illustrate the process, we have Mxj = sxj tj zj, zj being the distance from the laminate midplane to the midthickness of the ply. Adding together these moments for all the plies will give the external moment (per unit width) acting on the plate (see Fig. 3.5).
Stiffness and strength of composites
25
z y
Mx
x
My Ny
Mxy
Nxy
Nxy
Mxy
Nx
3.5 Loads acting on a laminate.
This procedure allows us to relate the stress resultants to the inplane strains and curvatures, giving: k N = Ae° + Bk
[3.16]
M = Be° + Dk
[3.17]
and
Equations [3.16] and [3.17] collectively are known as the ‘plate constitutive equations’, and the associated analysis as ‘Classical Laminate Theory’. The elements of the A, B and D matrices are p
p
Ars = Â Qrs j [hj  hj 1 ] = Â Qrs j t j j =1
j =1
1 p Brs = Â Qrs j [hj2  hj21 ] 2 j =1 Drs =
[3.18]
1 p Â Qrs [hj3  hj31 ] 3 j =1 j
where r, s = 1, 3.
3.1.5 The A, B and D matrices We have already seen when considering a unidirectional composite that certain terms in the compliance, or stiffness, matrix are associated with coupling between particular deformations and loads. Examination of the plate constitutive equations [3.16] and [3.17] allows us to identify similar couplings for laminates.
26
Overview and review of composite materials
Suppose we write [3.16] and [3.17] in expanded form: È Nx ˘ ÍN ˙= Í y˙ ÍÎ N xy ˙˚
È A11 ÍA Í 21 ÍÎ A31
A12 A22 A32
A13 ˘ È e ∞ x ˘ È B11 A23 ˙ ÍÍ e ∞ y ˙˙ + Í B21 ˙ Í A33 ˚˙ ÎÍ e ∞ xy ˙˚ ÍÎ B31
B12 B22 B32
B13 ˘ È k x ˘ B23 ˙ Í k y ˙ ˙Í ˙ B33 ˙˚ ÍÎk xy ˙˚
È Mx ˘ ÍM ˙= Í y˙ ÍÎ M xy ˙˚
È B11 ÍB Í 21 ÍÎ B31
B12 B22 B32
B13 ˘ È e ∞ x ˘ È D11 B23 ˙ ÍÍ e ∞ y ˙˙ + Í D21 ˙ Í B33 ˙˚ ÍÎ e ∞ xy ˙˚ ÍÎ D31
D12 D22 D32
D13 ˘ È k x ˘ D23 ˙ Í k y ˙ ˙Í ˙ D33 ˙˚ ÍÎk xy ˙˚
[3.19]
noting, of course, that A21 = A12, etc. We can then make the following associations: •
A13 and A23 relate inplane direct forces to inplane shear strain, or inplane shear force to inplane direct strains. • B11, B12 and B22 relate inplane direct forces to plate curvatures, or bending moments to inplane direct strains. • B13 and B23 relate inplane direct forces to plate twisting, or torque to inplane direct strains. • B33 relates inplane shear force to plate twisting, or torque to inplane shear strain. • D13 and D23 relate bending moments to plate twisting, or torque to plate curvatures. In certain circumstances some of the couplings listed above can be undesirable. They can sometimes be eliminated by appropriate construction of the laminate. If A13 = A23 = 0 there will be no coupling between direct stresses and shear strains (or shear stresses and direct strains). This can be achieved if we have a laminate in which all plies have 0° and/or 90° fibre orientations (a unidirectional or crossply laminate), or if the layup is balanced, i.e. for every layer with a +q orientation there is an identical lamina with a q orientation. Bendingmembrane coupling can be avoided if the B matrix is zero. This is very easily achieved by making the laminate symmetric about its midplane. In practice laminates usually have a symmetric stacking sequence. The phenomenon of bending–twisting coupling is eliminated if D13 = D23 = 0. This is achieved with unidirectional or crossply laminates, or with balanced antisymmetric layups, i.e. for every layer at +q orientation and a given distance above the midplane there is a layer with identical thickness and properties oriented at q and the same distance below the midplane. Such a layup is not symmetric (i.e. B π 0). The preference, in practice, for symmetrical laminates means that D13 and D23 π 0. However, these terms tend to zero for thick multilayer symmetric laminates.
Stiffness and strength of composites
27
For some layups inplane behaviour of the laminate is such that it appears to be isotropic (it is then called quasiisotropic). Examples are (0/90/±45°) and (0/±60°) layups. For such laminates it can be shown that A11 = A22 A11  A12 = 2A33 A13 = A23 = 0
3.2
Micromechanics of unidirectional composites
3.2.1 Macromechanics and micromechanics In the previous section we developed equations that describe the stress–strain behaviour of a lamina and the load–deformation behaviour of a laminate. These equations were based on the elastic properties of the lamina and, as such, ignored the microscopic nature of the material. In other words we took no direct account of the fact that we are dealing with fibrereinforced materials, we merely acknowledged that they were nonisotropic. We refer to this as macromechanics analysis. Because the starting point of a significant proportion of composites’ manufacture is the combination of fibres and matrix, it would be very helpful if we could predict the behaviour of the composite (laminate) from a knowledge of the properties of the constituents alone. There are many limitations to such micromechanics analyses. However, studying performance on a micro scale is essential if we are to understand fully what controls the strength, toughness, etc., of composites.
3.2.2 Micromechanics models for stiffness We stated in Section 3.1 that the unidirectional ply forms a useful building block for many studies of composites. Much micromechanics analysis has, therefore, been devoted to this simple system. The most successful application is the prediction of the stiffness parallel to the fibres, i.e. the longitudinal stiffness or modulus. We denoted this as E11 in Section 3.1.2. It can be shown that the longitudinal modulus of the composite is E11 = Efvf + Emvm
[3.20]
where subscripts f and m refer to fibres and matrix and n is the volume fraction. A relationship of this form is known as the Rule or Law of Mixtures. The predictions from equation [3.20] agree well (within 5%) with data from carefully controlled experiments for tensile loading. Predictions are not so good for compressive loading because the experimental results are very sensitive to the design of the equipment and the alignment of the fibres in the specimen.
28
Overview and review of composite materials
The corresponding expression for the transverse modulus of the composite is 1 vf vm = + E22 Ef Em
[3.21]
It is usual to take Ef as the longitudinal value, if only because the transverse fibre modulus is extremely difficult to determine. This assumption will only be correct for isotropic fibres. Because of the enormous simplifications made in formulating the above equation [3.21] it does not give very good predictions for E22. Extremely complicated elasticity or finite element analyses are required produce a more accurate model. The inplane shear stiffness or modulus, denoted as G12 in Section 3.1.2, of a unidirectional composite can be obtained from a similar model to that used for obtaining transverse modulus. The analysis gives the result: 1 vf vm = + G12 Gf Gm
[3.22]
The model suffers from the same limitations as that used for transverse modulus, very complicated analyses being needed to give a better prediction. The longitudinal modulus model serves to provide a prediction for the major Poisson’s ratio, u12. The resulting expression is u12 = ufvf + umvm
[3.23]
3.2.3 Micromechanics models for strength It is far more difficult to obtain a prediction for strength than for stiffness. This is due to several factors: the random nature of failure and hence the need to employ statistical methods; the number of failure modes that can cause the composite’s failure (fibre, matrix or interface failure); the very local nature of failure initiation and the influence of the associated stress field, itself determined by the details of fibre packing. As for stiffness, methods for predicting longitudinal performance are better than those for transverse and shear performance. For most PMCs, a reasonable description of tensile strength capability is given by sˆ 1T = sˆ fvf, but it should be recognised that the onset of cracking (of fibres or matrix) may be a more useful design criterion. Also, fibre strength is not a unique value; it varies from one fibre to another and depends on the length over which it is measured. Thus, the choice of sˆ f is far from obvious and it is necessary to use a statistical approach. The complex nature of tensile failure, involving fibre, matrix or interface failure,
Stiffness and strength of composites
29
is also seen in compression, but with the added possibilities of fibre buckling and matrix shear deformation. Recent work which accounts for initial fibre waviness and the matrix shear yield stress gives reasonably accurate predictions: sˆ 1C = Gt (g *) i.e. the shear modulus of the composite at instability. Failure strains in compression can be very close to those seen in tension; however, results are very dependent on the test method. There is no simple relation for predicting the transverse tensile strength ( sˆ 2T), transverse compressive strength ( sˆ 2C) or inplane shear strength (tˆ12). Because of the complexities, no serious attempts have been made to model these modes of failure. Note that there is another form of shear failure, namely interlaminar shear failure. This mode of failure is seen when flexural or throughthickness loading occurs (see Section 3.4). It is, then, relevant to delamination, i.e. splitting between plies.
3.2.4 Thermal and moisture effects As already mentioned, carbon and aramid fibres have a very small, or even slightly negative, coefficient of longitudinal thermal expansion (af). One consequence of this is that residual stresses are set up in a unidirectional composite as it cools from the curing temperature. In the transverse direction these stresses can be a significant fraction of the failure stress of the matrix. Hence, any calculation which attempts to predict failure should include these thermal effects. A second consequence of the fibre and matrix having different expansion coefficients is that the composite has different coefficients in the longitudinal and transverse directions. Based on the assumption that the Poisson’s ratios uf ª um the following simple expressions have been derived: a1 =
1 (a f Ef vf + a m Em vm ) E11
a 2 = (1 + u f )a f vf + (1 + um )a m vm  a 1u12
[3.24] [3.25]
The anisotropy of thermal expansion (a1 π a2) will cause residual thermal stresses in laminates, in addition to those in each ply mentioned above. Resin matrices will absorb moisture and therefore swell during normal operating conditions. Some fibres, such as Kevlar, also absorb water. The water uptake in a resin matrix is usually by a process of Fickian diffusion and the swelling can be characterised by an absorption coefficient (b), which is directly equivalent to the thermal expansion coefficient.
30
Overview and review of composite materials
For a unidirectional PMC, reinforced with carbon or glass fibres, the swelling coefficient in the fibre direction (b1) may be taken as zero. The transverse coefficient (b2) depends on the expansion of the matrix, bm, and may be taken as: b2 =
rc (1 + um )b m rm
[3.26]
where the suffices m and c refer to matrix and composite respectively. The composite’s density, rc, was defined in equation [2.2]. Laminate analysis should be modified to take account of thermal and moisture effects. This is necessary so that a better estimate of strength may be obtained. The appropriate theory can be found in many texts, e.g. Agarwal and Broutman.1
3.3
Strength of unidirectional composites and laminates
3.3.1 Introduction In Section 3.1 we established the stress–strain relationships for an individual lamina, or ply, and for a laminate. We can use the constitutive equations to calculate the stresses in each ply when we know the values of the loads acting on the laminate. By comparing these stresses with a corresponding limiting value we can decide whether or not the laminate will fail when subjected to the service loads. There are several ways to define failure. The obvious one is when we have complete separation, or fracture; clearly, then, the component can no longer support the loads acting on it. However, a more general definition would be ‘when the component can no longer fulfil the function for which it was designed’. Such a definition includes total fracture but could also include excessive deflection as seen when a laminate buckles (basically a stiffness rather than a strength limit), or even just matrix cracking. The latter could constitute failure for a container because any contents would be able to leak through the matrix cracks in the container’s walls. As for isotropic materials, a failure criterion can be used to predict failure. A large number of such criteria exist, no one criterion being universally satisfactory.We shall start by considering a single ply before moving on to discuss laminates. We saw in the last section that there are five basic modes of failure of such a ply: longitudinal tensile or compressive, transverse tensile or compressive, or shear. Each of these modes would involve detailed failure
Stiffness and strength of composites
31
Table 3.2 Typical strengths of unidirectional PMC laminates (vf = 0.5) (values in MPa) Material
Longitudinal Longitudinal tension compression
Glass/polyester
Transverse Transverse Shear tension compression
650–750
600–900
20–25
90–120
45–60
Carbon/epoxy
850–1100
700–900
35–40
130–190
60–75
Kevlar/epoxy
1100–1250
240–290
20–30
110–140
40–60
mechanisms associated with fibre, matrix or interface failure. Some typical strengths of PMCs are shown in Table 3.2. We can regard the strengths in the principal material axes (parallel and transverse to the fibres) as the fundamental parameters defining failure. When a ply is loaded at an angle to the fibres, as it is when part of a multidirectional laminate, we have to determine the stresses in the principal directions and compare them with the fundamental values.
3.3.2 Strength of a lamina Strength can be determined by the application of failure criteria, which are usually grouped into three classes: limit criteria, the simplest; interactive criteria, which attempt to allow for the interaction of multiaxial stresses; hybrid criteria, which combine selected aspects of limit and interactive methods. Here we shall only discuss criteria that fit into the first two classes. 3.3.2.1 Limit criteria There are two limit methods, the maximum stress and the maximum strain criteria. The maximum stress criterion consists of five subcriteria, or limits, one corresponding to the strength in each of the five fundamental failure modes. If any one of these limits is exceeded, by the corresponding stress expressed in the principal material axes, the material is deemed to have failed. In mathematical terms we say that failure has occurred if: s1 ≥ sˆ 1T or s1 £ sˆ 1C or s 2 ≥ sˆ 2T or s 2 £ sˆ 2C or t 12 ≥ tˆ 12
[3.27]
(recalling that a compressive stress is taken as negative so, for example, failure would occur if s2 = 200 MPa and sˆ 2C = 150 MPa). The maximum strain criterion merely substitutes strain for stress in the five subcriteria. We now say that failure has occurred if: e 1 ≥ eˆ 1T or e 1 £ eˆ 1C or e 2 ≥ eˆ 2T or e 2 £ eˆ 2C or g 12 ≥ gˆ 12
[3.28]
32
Overview and review of composite materials
As when calculating stiffness, it is important that we can deal with the situation in which the fibres are not aligned with the applied stresses. We would use equations [3.6] to obtain the stresses in the principal material directions. Although simple to use, limit criteria do not agree well with experimental data unless the fibre angle is close to 0° or 90°. This is because at intermediate angles there will be a stress field in which both s1 and s2 can be significant. These stresses will interact and affect the failure load, a situation which is not represented in a criterion where a mode of failure is assumed not to be influenced by the presence of other stresses. Also, the maximum stress and maximum strain criteria will give different predictions when the stress–strain relation is nonlinear. This will certainly be the case for shear deformations and hence an assumption of linearity is seen to be invalid. In such cases the maximum strain criterion generally gives better agreement with experiment than does the maximum stress criterion. 3.3.2.2 Interactive criteria Interactive criteria, as the name suggests, are formulated in such a way that they take account of stress interactions. The objective of this approach is to allow for the fact that when a multiaxial stress state exists in the material failure loads may well differ from those when only a uniaxial stress is acting. There are many such criteria, of varying complexity, their success in predicting failure often being confined to one fibre/resin combination subjected to a well defined set of stresses (e.g. a tube under internal pressure). The Tsai–Hill criterion which has proven to be successful in a wide variety of circumstances is the only method that will be discussed here. There is currently much debate about the merits of the various criteria.2 The Tsai–Hill criterion was developed from Hill’s anisotropic failure criterion which, in turn, can be traced back to the von Mises yield criterion for metals. In its most general form the Tsai–Hill criterion defines failure as: 2
2
Ê s1 ˆ s1s 2 Ê s 2 ˆ Ê t 12 ˆ + + ≥1 Ë sˆ 1 ¯ sˆ 2 Ë sˆ 2 ¯ Ë tˆ 12 ¯
[3.29]
1
Because it is usually small compared with the others, the second term (s1s2/ sˆ 12) is often neglected. The modified from of the criterion is then: 2
2
2
Ê s1 ˆ Ê s 2 ˆ Ê t 12 ˆ + + ≥1 Ë sˆ 1 ¯ Ë sˆ 2 ¯ Ë tˆ 12 ¯
[3.29a]
Stiffness and strength of composites
33
The values of strength used in equation [3.29] or [3.29a] are chosen to correspond to the nature of s1 and s2. So if s1 is tensile sˆ 1T is used, if s2 is compressive sˆ 2C would be used, and so on. It should be noted that only one criterion has to be satisfied, as opposed to the five subcriteria of the limit methods. Thus, only one value is obtained for the failure stress. Another point to bear in mind is that the mode of failure is not indicated by the method, unlike with the limit criteria. This latter issue has an influence on how we predict the failure of laminates, as we shall see later. For a unidirectional composite subjected to uniaxial stress parallel to a principal direction the Tsai–Hill and maximum stress criteria will give the same failure stress. Interactive criteria usually give better predictions of strength for intermediate fibre angles.
3.3.3 Strength of a laminate 3.3.3.1 Initial failure Suppose we take a crossply laminate (0/90° layup) and apply an increasing load in the direction of the 0° fibres. At a relatively low load cracks will be seen in the matrix parallel to the fibres in the 90° plies. These cracks will increase in density until a saturation state is reached. At this point the 90° plies contribute virtually no stiffness to the laminate in the 0° direction, a fact that is shown by the change in slope of the loadextension curve for such a laminate. The commencement of transverse ply cracking is known as ‘initial failure’ or ‘first ply failure’. It is possible to predict initial failure of laminates by combining Classical Laminate Theory with a failure criterion. Clearly, the choice of criterion is crucial and, as already stated, there are many available, each one often being relevant only to a very specific situation (loading and geometry). We start with the plate constitutive equations (equations [3.16] and [3.17]), i.e. ∞ È N ˘ ÈA B ˘ Èe ˘ = Í ÍÎM ˙˚ ÍÎ B D˙˚ Î k ˙˚
[3.30]
Solution of equations [3.30] will give the plate midplane strains (ee°) and plate curvatures (k), for a known set of forces N and moments M. 1
∞ Èe ˘ ÈA B ˘ È N ˘ ÍÎ k ˙˚ = ÍÎ B D˙˚ ÍÎM ˙˚
[3.31]
The plate strains are expressed in the, global, plate x–y axes (see Fig. 3.5). Thus the strains in each ply can be found from the transformations of equation [3.7], and the ply stresses are obtained from the stiffness matrix
34
Overview and review of composite materials
(equation [3.5]). By applying, on a plybyply basis, a selected failure criterion, the occurrence of failure can be determined. 3.3.3.2 Final failure and strength The final, or ultimate, failure load of an angle ply laminate is often coincident with, or only slightly higher than, the load to cause initial failure. This is not necessarily the case for other layups and final failure can be at a considerably higher load than that to cause first ply failure. It is clear that once a ply has sustained failure its stiffness in certain directions will have been reduced. However, unless the damaged ply has completely delaminated from the rest of the laminate it will still contribute to the overall stiffness of the plate.The magnitude of this contribution depends on the amount of damage, the fibre/matrix combination and the nature of the loading on the ply. In general an iterative method is adopted, successively applying the approach described in Section 3.3.3.1 until final failure has occurred. At each step the A, B and D matrices would need to be recalculated to allow for the development of damage.1
3.4
Application to structures
3.4.1 Limitations of Classical Laminate Theory Classical Laminate Theory (CLT) (see Section 3.1.4) applies to an element of plate over which forces and moments are assumed constant, and in which throughthickness shear strains are ignored. Thus, only inplane direct and shear stresses are considered. CLT is equivalent to simple beam theory which only considers a pure moment loading (i.e. constant along the beam), which results in only a direct stress (acting parallel to the beam’s longitudinal axis). Again shear strains (through the beam depth) are ignored. In practice, of course, beams are usually subjected to bending moments which vary along the length, the resultant direct stresses causing shear stresses, which can be calculated from equations of equilibrium. Even in these circumstances shear strains can usually be ignored; they only have a significant effect on beam deflections when the beam is very short (small spantodepth ratio). For a laminated construction such shears are referred to as interlaminar shear stresses; they can give rise to interlaminar failure, or delamination. A threepoint flexure test on a short beam (spantodepth = 5) is a common way of determining the interlaminar shear strength of unidirectional composites. Plate equations can be altered to include varying moments and throughthickness shear strains. The plate constitutive equations would be modified
Stiffness and strength of composites
xy
35
x y
y
x
z xz
yz z
3.6 Stresses at laminate edge in the thickness (z) direction.
to account for the throughthickness shear resultants, by including two additional terms in the A matrix3 (see Section 5.5). The inclusion of shear strains would be appropriate for thick isotropic plates (equivalent to short beams), and also for thick composite plates. The latter, of course, will generally have a low throughthickness shear modulus (compared with inplane extensional moduli), thus making the inclusion of such shear strains generally advisable for typical composites, even if of moderate thickness.
3.4.2 Edges The limitations of CLT mentioned above (constant inplane stresses) implies that the plate is infinitely long and wide. In other words the theory ignores edges. In many real situations, of course, laminates will have edges; for example a plate of finite width (encountered in mechanical testing), a plate containing a hole (bolts, rivets) or opening (say for access), a skin/stringer joint, a skin/spar junction, etc. The stresses acting at an edge are shown in Fig. 3.6. A simple example is that of the free edge of a crossply laminate. Because of the mismatch in ply Poisson’s ratio (90/0°)s is preferred to (0/90°)s because the latter produces tensile throughthickness stresses. A problem in analysing these situations is that the high stresses occur within one or two plate thicknesses from the edge. Also, solutions can indicate singularities. Finite element models of this situation are discussed in Chapter 7.
3.4.3 Buckling In addition to the forms of failure already described, composite laminates, especially if thin, can fail by buckling when subjected to compressive or shear loading.
36
Overview and review of composite materials
The characteristic of buckling is that the panel retains its original configuration (flat or curved) until the initial buckling load is reached. At this point large outofplane displacements will occur. The magnitude of the corresponding load is determined by the stiffness of the laminate (not the strength), together with the geometry and edge supports. Most panels can continue to sustain load over and above the initial buckling strength. Final failure will be determined by the strength of the laminate. It is usual for the design load to be equal to, or less than, the initial buckling load. An extensive set of information on panel buckling can be obtained from: ESDU International plc, 27 Corsham Street, London N1 6UA, UK. An excellent comprehensive reference is that by Leissa.4 Only in a few situations is it possible to use simple formulae to calculate initial buckling loads. More often it is necessary to use graphical, or other means. In this section only a few cases will be presented, merely to indicate the general approach. For convenience it is common to cast the equations into the same form as those used for isotropic plates, i.e. critical stress s b = KE (t b)
2
where t = plate thickness, b = plate width, E = Young’s modulus and K is a buckling coefficient related to panel dimensions and edge supports. Most solutions assume that the panel buckles into a sinusoidal shape with m half waves along the length (xdirection) and n half waves across the width (ydirection). Normally n = 1. K is dependent also on m and n. So, for example, for a rectangular orthotropic plate (a ¥ b) with all edges simply supported, subjected to a uniform uniaxial compressive stress (sx), the buckling coefficient is: Kx =
s x tb 2 N x b 2 = D22 D22 2
and
[3.32] 2
K x D11 Ê b ˆ 2 Ê D12 2 D33 ˆ Ê a ˆ 1 = m +2 + + 2 Ë ¯ Ë D22 D22 ¯ Ë b ¯ m 2 D a p 22
[3.33]
Note the dependence of sx on the plate’s flexural coefficients, D11, etc. Clearly, an analysis that ignored stacking sequence would not be expected to deliver accurate predictions.
3.5
Summary
In this chapter we have seen now the conventional stress–strain equations in two dimensions are modified to account for the directional nature of composites. From this macromechanics starting point equations describing
Stiffness and strength of composites
37
the behaviour of laminated plates were derived. As pointed out at the end of the chapter, these equations have certain limitations and cannot be used to represent behaviour at boundaries (plate edges or holes). The equations of micromechanics were shown to have limitations and these should be borne in mind when using software that takes fibre and matrix properties as input data.
3.6
References
1 Agarwal B D & Broutman L J, Analysis and Performance of Fiber Composites (2nd Edition), New York, Wiley, 1990. 2 ‘Failure Criteria in FibreReinforced Polymer Composites’, Special Issue, Composites Science & Technology, 1998 58(7). 3 Vinson J R & Sierakowski R L, The Behaviour of Structures Composed of Composite Materials, Dordrecht, Martinus Nijhoff, 1986. 4 Leissa A W, Buckling of Laminated Composite Plates and Shallow Panels, US Air Force Flight Dynamics Laboratory, Technical Report AFWALTR853069, June 1985.
This page intentionally left blank
Part II Fundamentals of finite element analysis G. A. O. DAVIES
In this part of the book the basis of finite element analysis is reviewed. Starting from the underlying theoretical issues, the method is developed to show how elements are derived, a model is generated and results are processed.
This page intentionally left blank
4 Fundamentals of finite element analysis
4.1
Basic theoretical foundations
This chapter is not intended to probe deeply into the theory of finite elements. Readers of this book may be familiar with the FE method and interested only in applying it to composite materials and structures, in which case they can skip this chapter. For others, with a passing knowledge only, we shall condense the theory to the basics. It is useful to strip some of the mystery from the theory and to draw attention to what is important and what is unimportant – particularly what is exact and what is approximate. There are dangers in creating an unsound finite element model and not to recognise poor answers. However, it is counterproductive to simplify the method too much and encourage users of commercial codes to treat the FE package as a ‘black box’. User manuals encourage analysts to think of finite elements as pieces in a jigsaw, the whole of which is the complete structure. Thus the package merely has to insert the jigsaw pieces into the correct place and they will be held there by nodal displacements and nodal forces at selected nodes. In the complete structure, when loaded, the displacements at nodes will ensure continuity and the nodal forces developed as the jigsaw piece strains will be in equilibrium with themselves and with the applied forces – somehow. There are two dangers to this approach. Firstly, the user has no idea what is exact and what is approximate, and in the latter case whether the errors are significant. Secondly, what are these nodal forces and do they not cause a local stress concentration in a stress field that should otherwise be smooth and changing gradually? The answer is that these nodal forces are quite fictitious in the usual FE method, even though they are made to equilibrate each other and the applied forces. (Although the applied forces may have to be converted to a compatible but fictitious form also!) Having said we shall strip away some of the mystery, the treatment will still be brief. For readers who wish for more we shall use the methods and 41
42
Fundamentals of finite element analysis Assumptions
Equations of equilibrium or motion
Equations of compatibility (Strain ~ displacements)
(Stress ~ applied loads)
Stress–strain law
4.1 The four conditions for all structural analysis.
notation of A Finite Element Primer.1 We make a beginning by going to the very basics of structural analysis, starting with a trivial example and then generalising to a completely arbitrary structure. Basically all structural analysis can be summarised by four separate (but linked) conditions to be modelled and satisfied, as illustrated in Fig. 4.1. The basic assumptions are usually directed at simplifying the type of structure or component. Thus is the component a rod/bar, beam, plate, shell or 3D? This stage leads to the justification – fundamental to the FE method – of assuming the nature of the strain or displacement field in the element. A pinended bar in a framework may have only one axial strain component. A slender beam or thin plate may have a linear strain distribution through the thickness. A 3D continuum may not be accessible to any assumed field. Thus this stage is driven by geometry, but we delay the introduction to finite elements proper and consider the other three stages. Satisfying equilibrium results in equations that equilibrate the applied forces to the structure’s resisting stresses. These may be surface forces or internal (body) forces. If the structure is in motion then the body forces can be extended to include the ‘inertia forces’ and of course the stresses, displacements and so on are then all functions of time. In many cases (probably most) the strains are small and it is possible to write down the equations of equilibrium for the body ignoring its small changes in shape. We shall do this initially, and leave to later chapters the nonlinear behaviour due to material failure, or to buckling when changes in geometry cannot be ignored. If the equations of equilibrium are sufficient to enable us to solve completely the stresses in the structure, the structure is said to be statically determinate. In practice very few structures are made to be statically determinate. Such structures have one distinct disadvantage in that if a single
Fundamentals of finite element analysis
43
component fails, the complete structure becomes a mechanism, i.e. it falls down. A statically determinate structure is very much not ‘failsafe’. There is at least one case where statical determinacy is an advantage, and that is if thermal heating is significant. A statically determinate structure’s stresses depend only on the applied loads and are unaffected by temperature gradients. (The ribs inside Concorde are made this way, since the fuel in the wing is intended to cool down the very hot outer surfaces.) If a structure is statically indeterminate or redundant then the next two conditions and equations have to be brought in. Compatibility arises from stating that the strains are ‘compatible’ with the displacements and can be derived from them if the displacements vary continuously. We show that it simply means that a geometrical argument can be used to express strains in terms of displacements once we have defined what strain means: like the strain in a bar is its fractional change in length. The equations of compatibility have nothing to do with the equations of equilibrium nor with the stresses directly. Thus if the body is heated and strains and stresses ensue, the equations of compatibility are not affected. The stress–strain law is the relationship between stress and strain and it is based on experimental evidence. In many cases stress is proportional to strain. In other cases strain can be caused by heating (or freezing), or by moisture absorption or by electromagneticchemical effects. It is important to note that the stress–strain law has nothing to do with either equilibrium or compatibility. To illustrate these separate criteria consider the very simple example shown in Fig. 4.2 of three pinended bars subjected to loads R1 and R2 and having joint displacements r1 and r2. Let the central bar also be heated by T degrees. The assumption is that all bars are pinended, and hence only resist axial tensions T, and stretch by D. Equilibrium: T14 sin q  T34 sin q = R1 T14 cos q + T24 + T34 cos q = R2
[4.1]
Compatibility: if the displacements are small, then the displacement components at the ends of a bar, at right angles to the bar, will not stretch it. Only the components in line with the bar will produce strains. Thus strain D 14 L D 14 = r1 sin q + r2 cos q r2 D 24 = L cos q D 34 = r1 sin q + r2 cos q
e 14 = where
and
[4.2]
44
Fundamentals of finite element analysis 1
3
2 T24 D24 T34
L T14
D34 D14 q q 4
R1, r 1
R2, r 2
4.2 Simple (redundant) pinjointed frame example.
Stress–strain: s E s For centre bar e = + aT E For outer bars e =
[4.3]
where E is the extensional (Young’s) modulus and a the linear coefficient of expansion. A displacement solution is now straightforward. If all bars have the same crosssection area A, the stress–strain law becomes D14 T14 = ; L AE
D 24 T24 D 34 T34 = + aT ; = L cos q AE L AE
[4.4]
and using compatibility (equation [4.2]): AE [r1 sin q + r2 cos q] L AEr2 T24 =  AEaT L cos q AE T34 = [ r1 sin q + r2 cos q] L T14 =
[4.5]
Now we put these forces into the two equations of equilibrium [4.1] and solve for r1 and r2: 2 AEr1 sin 2 q = R1 L AE (2 cos 2 q + sec q)r2 = R2  AEaT L
[4.6]
Fundamentals of finite element analysis
45
Notice that the final set of equations (two) were just those needed to solve for the two displacement unknowns. This would have been true if there had been only two bars (statically determinate) or three or more (progressively more and more redundant). This is the attraction of the displacement method; we do not have to worry about the degree of redundancy. The only difference between this example and the conventional FE solution (apart from the small number of unknowns r1 and r2) is that the ‘elements’ are exact. No assumptions were made about the nature of the displacements since uniform pinended bars have a constant strain.
4.2
Principle of virtual displacements
The next step is to use virtual work arguments as a substitute for equilibrium conditions (the advantages will become apparent later). If a force (or a stress) moves through a displacement (or a strain) then the virtual work is defined as the product of force ¥ displacement. This avoids having to define the force–displacement (or stress–strain) law which has nothing to do with equilibrium. The force–displacement relationship may be nonlinear, as shown in Fig. 4.3 for example. We now go further and imagine virtual displacements which are hypothetical and not related to the real forces or displacements. We use a ‘bar’ to single them out; r1, r2, D , etc. The Principle of Virtual Displacements (PVD) simply equates internal virtual work to external virtual work, thus in the pinjointed framework example: T14 D14 + T24 D 24 + T34 D34 = R1r1 + R2 r2
R
[4.7]
R
r Real work
4.3 Nonlinear force/displacement behaviour.
r Virtual work
46
Fundamentals of finite element analysis
This rather important equation gives us no information at all (!) until we use the compatibility conditions. We satisfy compatibility directly and insert the values for D in terms of r into the above, and rearrange
(T14 sin q  T34 sin q  R1 )r1 + (T14 cos q  T24 + T34 cos q  R2 )r2 = 0
[4.8]
We now capitalise on the virtual nature of r1 and r2 and say for example that r1 could be zero, in which case the individual expressions in the parenthesis above must separately vanish. These are clearly the two equations of equilibrium as before (equation [4.1]) so the PVD is enforcing them indirectly. Three important points to note are: • Only because r1 and r2 are independent do we get both equilibrium equations. • If a framework had n displacements we would get n equations from the n virtual displacements to solve from. • From the displacement in the (say) horizontal direction, r1, we get the horizontal equation of equilibrium, resolving T14 and T34 in terms of R1. Having fixed the ideas we can now move to general structures with arbitrary shapes.
4.3
An arbitrary structure
The leap from a simple threebar truss to a completely general structure is a big one. We shall need more sophisticated tools to describe the structure and its loads, stresses, and displacements. It turns out that matrix notation is a great aid in defining both stress fields and displacement fields and, moreover, matrices are an ideal vehicle for reading into, or extracting from, digital computer memories. In fact, in the early days of the 1950s, finite element methods were originally known as ‘matrix methods’. Figure 4.4 indicates an arbitrary 3D solid having volume V and surface S (local normal ‘n’), subjected to surface forces ps per unit area and internal (volume) body forces pv per unit volume. We list these vector forces as having Cartesian components: p tv = [ pvx pvy pvz ] pst = [ psx psy psz ]
[4.9]
Note that the ‘t’ superscript denotes the transpose of a matrix. Similarly the displacements everywhere we write as the vector u t = [u v w]
[4.10]
Notice that these components p, u, etc., may all be functions of x, y and z. The internal stresses and strains can also be listed as column matrices in terms of the three direct and three shear components:
Fundamentals of finite element analysis
47
pv n, p s dV y
dS
x
z
4.4 A general continuum.
s t = [s xx s yy s zz s xy s yz s zx ]
[4.11]
e t = [e xx e yy e zz e xy e yz e zx ]
The reader can consult any standard text for definitions of stress notation. Suffice it to say that here the first suffix refers to the direction, and the second suffix the plane on which the stress component acts. Thus sxx is a direct stress (tensile positive, compressive negative) but sxy is a shear stress. The strain components simply correspond to the stress components. We now follow the procedure as before. The external virtual work done is
Ú (p
sx
S
u + psyv + psz w )dS + Ú ( pvx u + pvyv + pvz w )dV V
t s
[4.12]
t v
= Ú p u d S + Ú p u dV S
V
It can be shown that the internal virtual work done by the stresses over the strains is
Ú (s
V
xx
e xx + s yy e yy + s zz e zz + s xy e xy + s yz e yz + s zx e zx )dV = Ú s t e dV
[4.13]
V
The next step, as in the framework example, is to equate the two expressions for work and enforce compatibility. The general equations relating e and u are readily shown to be, using geometrical definitions of strain in terms of the displacement at a point, e xx =
∂u ∂u ∂v , e xy = + , etc. ∂x ∂y ∂x
or simply using matrix shorthand
e = ∂u.
[4.14] [4.15]
48
Fundamentals of finite element analysis
The sixbythree array of operators is given by È∂ Í∂x Í ∂t = Í 0 Í Í Í0 Î
0
0
∂ ∂y
0
0
∂ ∂z
∂ ∂y ∂ ∂x
∂ ˘ ∂z ˙ ˙ 0 ˙ ˙ ∂ ˙ ˙ ∂x ˚
0 ∂ ∂z ∂ ∂y
0
[4.16]
The PVD then becomes t
Ú s e dV = Ú s
V
t
V
∂ u dV = Ú p tv u dV + Ú pst u dS V
[4.17]
S
This most important equation is the basis behind all FE derivations. Later we show what it leads to. To show what we are actually doing when we use it, it is necessary to transform the equation by using a mathematical identity derived from Gauss’s Theorem:
Ús
t
V
∂ u dV = Ú u t [∂ t n]s dS  Ú u t ∂ t s dV S
[4.18]
V
This identity is in effect a threedimensional form of integration by parts and can be applied to any two functions, and not just to s and u as here. It is essential that the two derivatives are finite and continuous in the region V. We later apply the PVD to a volume divided into finite elements where, across the interface between elements, we recognise that the stress field s may be discontinuous and, therefore, the derivative ∂ts is not defined. However, we leave this possibility to later and now concentrate on what the PVD is delivering. So taking the framework argument as an example, we need to convert the term ∂ u in the PVD to the form u and then appeal to the virtual nature of u. Thus, substituting the Gauss identity into the PVD it becomes:
Ú u [∂ s + p ]dV  Ú u [(∂ t
t
t
V
V
t
n)s  p s ] dS = 0
[4.19]
S
Now we use the same argument as for the framework. The displacements u(x, y, z) are virtual, so their coefficients must vanish, i.e. ∂ t s + pv = 0 inside V and
(∂ t n)s = p s
[4.20]
on S. These are the equations of equilibrium inside the body and on its surface. If we examine the first equation by expanding the term in ∂ts and p, we find
Fundamentals of finite element analysis
49
we get three equations representing the stress gradients, in the directions x, y and z, which equilibrate the three body force components if they are present. The second equation takes the stresses at a point on the surface, and then the components in directions x, y and z (∂tn are direction cosines) which have to equilibrate the components of the surface pressures pvx, etc. We can therefore now rely on the PVD to satisfy equilibrium everywhere. The next step is the FE approximation.
4.4
Finite element approximations
Imagine the variation of displacement across a complex structure such as an aircraft or a cooling tower, as shown in Fig. 4.5. No simple theory can deliver this. The idea then is to divide the structure into elements which are small enough so that the displaced shape can be assumed with little error, and only the magnitudes of the displacement need be found. A crude approximation could be a linear assumption. The whole structure can be divided into elements, the elements being either 1D (bars), 2D (plates) or 3D (bricks). Figure 4.6 shows a picture of the true displacement along a row of elements in 1D, and a linear approximation which will be quite close to the truth since the elements are quite small. Modern preprocessors use very powerful (yet friendly) algorithms to divide up the most complex shapes. Figure 4.7 shows a display of hexagonal brick elements where the elements are shrunk so that the user can check whether any are missing.
4.5 Two real structures.
50
Fundamentals of finite element analysis Linear displacement True displacement Displacement
Finite element size
4.6 The ‘finite’ element approximation.
Elements shrunk
4.7 Preprocessor aid for finding missing elements.
Because we are using the PVD which is an integral, we can always write complete volume and surface integrals as a summation of all the element integrals: È
˘
Â Ú s e dV = Â Í Ú p u dS + Ú p u dV ˙ Î ˚ t
elements Vg
t v
s
elements Sg
Vg
where Sg and Vg denote the surface or volume of the gth element.
[4.21]
Fundamentals of finite element analysis
51 d6
3
d5
y x d2
1
d4
d1
d3 2
4.8 A triangular element with linear shape functions.
Now, it is not the intention in this book to delve deeply into the subtleties of the FE method, and individual elements in particular. It will suffice to describe the basic idea and mention particular aspects that the reader may need to know about when reading a manual, understanding the code, choosing elements and appreciating which errors are unimportant and which are important, and how to reduce or avoid them. For simplicity, then, suppose we cover a flat plate with a triangular mesh as in Fig. 4.8, and suppose the plate is in a 2D stress field (sxx, syy, sxy) with uniform stresses across the thickness at any point. The geometry is defined by the position of the three nodes of a typical element. If we assume that the displacement field ut = [u, v] is linear then we can write u = a + bx + cy and find the coefficients a, b and c in terms of the three horizontal displacements d1, d3 and d5 at the three corner nodes. We rewrite the resulting expression as u = N1d1 + N2d3 + N3d5
[4.22]
where the ‘shape functions’ N(x, y) are linear in this case. In Chapter 5 we shall look at more ambitious shape functions, such as quadratic, where more nodal points are required to define the field. The actual algebraic details of N1, N2 and N3, which, for N1 say, needs to be unity at node (1) and zero at nodes (2) and (3) can be found in reference 1. Similarly for the other displacement component: v = N1d2 + N2d4 + N3d6
[4.23]
For brevity we write u = Nd g
where d tg = [d1 d2 d3 d4 d5 d6 ]
[4.24]
for the gth element. It is now routine to go to the next stage and apply compatibility: e = ∂u = ∂Ndg = Bdg
[4.25]
52
Fundamentals of finite element analysis
where the 6 ¥ 6 matrix B for this example is just an array of constants since N is linear. Thus the element is a constant strain triangle. (Note that the symbol B is also used in laminated plate theory; see Chapter 3.) We now assume the stress–strain law is linear so that s = Ee
[4.26]
where E is a 6 ¥ 6 ‘material stiffness’ matrix whose elements contain Young’s modulus and Poisson’s ratio for an isotropic material. Again the details will be found in reference 1. The internal work in the element can now be evaluated t
t
t g
t
Ú s e dV = Ú e E e dV = Ú d B EBd
Vg
Vg
g
[4.27]
dV
Vg
But dg can clearly be taken outside the integral, which itself can be evaluated since B and E are known. Thus the element work = dgt kg dg, where kg =
ÚB
t
EB dV
Vg
is known as the element stiffness matrix since the work product may be viewed as dgt kg dg = (kgdg)t dg = forces ¥ displacements and force = stiffness ¥ displacement. The righthand side of the PVD similarly becomes t v
t v
t v
t s
Ú p u dV + Ú p u dS = Ú p N dV d + Ú p N dS d
V
S
V
g
g
[4.28]
S
and these integrals can also be evaluated once we know the distributions of pv and ps. This external work can also clearly be written as Pgt dg where we see that Pg =
t
t
Ú N p dV + Ú N p dS
Vg
v
s
[4.29]
Sg
must clearly be nodal forces. They are not real concentrated forces (which would produce infinite stress concentrations) and are often known as ‘kinematically equivalent’ forces since they are defined in terms of the displacement shape functions N. The above expressions for these nodal forces simply emerged naturally from our PVD and the element integrals. They are measures we find convenient to use. We see, therefore, that by assuming the displacement shape functions we have been able to evaluate the integrals for any element, and therefore for all elements. The FE method can be viewed as a way of numerically integrating. In fact the integrals are never done exactly, but as a summation of discrete values of the integrand
Fundamentals of finite element analysis
53
times the appropriate bit of volume or surface at the sampling points. It is found that it is best to sample B (if it varies) at the optimal ‘Gauss’ points; see reference 1 for where these points are. We have now converted the internal and external virtual work to simply dgt kg dg and Pgt dg and it only remains to sum
Â
d tg k g dg =
elements
Â
p tg d g
elements
In the simplest case, if all element displacements dg are aligned with the global axes, they will be able to be selected from the total global list of displacements, usually written as r t = [r1 r2 r3 . . . rn ]
[4.30]
where n may be many thousands.The total virtual work of the entire system, internal and external, may be similarly written as rtK r and R t r , where K is the whole structure’s stiffness matrix and R is the global list of kinematically equivalent forces. But these two must be equivalent to the previous summations, so if we (or the code) make sure that we relate each dg to the correct parts of r, and the associated elements in kg, we may symbolically assemble K = Â kg
and R = Â Pg
The exact details of how this is done methodically, and what transformations to kg are necessary when element local axes are different from global, can be found in reference 1. Having assembled both K and R the PVD can be rearranged as
(r tK  R t )r = 0
[4.31]
and we now use the argument that all the n components of r are virtual so their coefficients vanish, and we have n equations Kr = R
[4.32]
This set of equations is then solved as discussed in Section 4.7 whence, knowing r, we then select the particular values d for the element level and hence e = Bdg and s = Ee for the strains and stresses. This is the basis of the modern FE method. We see that the nature of the displacement field has been approximate, but that compatibility and the stress–strain law have been satisfied exactly. The use of the PVD to satisfy equilibrium therefore means that these equilibrium equations will be satisfied only approximately. It is therefore time to examine what this means. We note that, by equating local and global nodal displacements, continuity of the structure’s nodal displacements is assured. But for our triangular element the displacement variation between nodes is linear and
54
Fundamentals of finite element analysis
n
1
n
s1
2
s2
Two adjacent elements
4.9 Discontinuous stresses across an element interface.
therefore continuity across the entire element interfaces is also secured. Thus we have a continuous displacement field variation throughout the entire structure. However the strains, and therefore the stresses, are constant in any element, but the stresses will not be continuous from one element to another. Is this disastrous? Consider two triangular elements (1) and (2) adjacent to each other as shown in Fig. 4.9. If we return to the general form of the PVD after transforming it, we can examine the consequence of summing all element contributions, and look at the coefficients of the virtual displacement across the interface between (1) and (2). If this face is not a loaded surface (ps = 0) then we are grouping two contributions together with a common virtual displacement, i.e.
ÚS u t [(∂ t n)s 1  (∂ t n)s 2 ] ds = 0
[4.33]
where the minus sign arises because the normal ‘n’ is in opposite senses for each element. Thus we may not be satisfying equilibrium exactly at any point, that is
(∂ t n)s 1 π (∂ t n)s 2 but it will be satisfied in the mean by making the above integral zero. Or, to put it another way, the outofbalance error in stress components will do no net work over the displacements along the edge. Moreover, if the element shape functions are capable of representing a rigid body motion (u = constant, v = constant, and the rotation), we recall that the equation of equilibrium is always associated with the corresponding virtual displacement, so the term like u = constant will ensure that the element equilibrium is satisfied in the xdirection. The rotation freedom will ensure that there is no resultant moment on an element if there are no body
Fundamentals of finite element analysis
55
A D
Elliptic ‘annulus’
4.10 A stress concentration at point ‘D’.
or surface forces acting upon it. We therefore accept that the FE solution only satisfies equilibrium in the mean and there will be discontinuities across interfaces. This does not mean that constant strain triangles, for example, should not be used. They are popular in describing, for example, elastoplastic deformations since the whole element goes plastic and the integrals are easy. However, small elements may be needed to pick up rapidly varying strain fields. Figure 4.10 shows a test case for an elliptical hole in a plate where there is a very high stress concentration at the point D. The plate is divided into fournode quadrilateral elements and in one quarter there is a coarse mesh of six elements and a fine mesh of 24 elements. In Fig. 4.11 it is clear that three elements around the edge are insufficient. If the mesh is refined then the discontinuities are much smaller and the maximum stress is predicted to within a few percent. The ‘jumps’ in the stresses can be used as an indicator of the error, and many codes then employ this measure to refine (or adapt) the mesh automatically until the errors are uniformly small everywhere. Most codes will take an average value of the stresses at a node coming from several elements sharing this node. If this is done in Fig. 4.11 we can see that the results will be quite good; except, of course, for the maximum stress at point D which sits astride the axis of symmetry. We could further refine the mesh shown on the right of Fig. 4.11. It can be shown that if the element is capable of having a constant strain field, then successive mesh refinement will converge on the exact solution. Any element not capable of representing a constant strain field and a (strainfree) rigid body displacement is not acceptable. Another way to improve
56
Fundamentals of finite element analysis
A A D D
Analytical solution Finite element
A
Analytical solution Finite element
sss
D
A
sss
D
4.11 Effect of halving element sizes.
the description is to use higher order elements which use (say) quadratic displacement fields and twice as many nodes per element.
4.5
Brick, beam, plate and shell elements
The previous example of a triangle element, usually known as a membrane element, was selected for simplicity as an introduction to the finite element process. It is not too difficult to extend this concept to foursided (‘quad’) elements with four nodes and eight nodal displacements, or eight (and nine) noded quads with midside nodes (and a centre node). It is also possible to design curvilinear elements better able to cope with curved boundaries. The trick here is to ‘map’ the shape of the element edges in terms of the nodal coordinates in exactly the same way as the displacement field was ‘mapped’ in terms of the nodal displacements. Such ‘isoparametric elements’ are a very powerful concept. They also have the property that, if the shape and displacement fields are mapped with respect to a reference unit square using nondimensional shape functions, any rigid body movement still maps into zero strain fields. The idea for 2D plates readily converts to 3D by deploying tetrahedral or hexagonal ‘bricks’. A sixsided brick can have eight corner nodes and three displacement freedoms at each node for example. Higher order 20node bricks are popular, having 8 corner nodes and 12 midside nodes. Both the displacement field and edges of such isoparametric elements can rep
Fundamentals of finite element analysis
57
18
12
19
z3 6 z2 4
7
11
14
17
z1
8
15
5
1
20
10 2
3
4.12 A 20noded curvilinear brick element.
resent curved quadratic shapes. Figure 4.12 shows a curvilinear brick which will have 20 ¥ 3 = 60 displacement degrees of freedom in total. The variables z1, z2 and z3 indicate that the shape in the x, y, z space has been mapped into the space 1 < z < 1 which introduces the Jacobian, J, into the element stiffness. 1 1 1
kg =
t
Ú Ú Ú B EB J dz dz dz 1
2
3
[4.34]
1 1 1
All the shape functions N are now functions of z1, z2 and z3 and their contributions to the integral, via B(z), is sampled at the Gauss points for all elements, the only varying quantity being the Jacobian matrix whose elements are the derivatives ∂x/∂z1, etc. A word should be said here about distorted elements since if bricks, and other isoparametric elements, differ too much from the basic cube then accuracy suffers. One way of sampling excessive distortion is the variation in the values of J at the Gauss points; many codes will flag warning messages. It is however possible to have undistorted elements with no J variations but having a very high aspect ratio, that is the element is long and thin in one direction. If the strain variation in this direction happens to be gentle than no problems will arise, but in general this will not be so. The ability of the shape functions to cope with variations in strain in all directions then becomes fully stretched, and many codes have empirical measures to flag warnings for excessively long elements. Brick elements are expensive and produce a stiffness matrix with a high bandwidth. It is very easy to run out of computer memory when using them indiscriminately. For example, 100 elements in a row would not be unusual for a 1D or 2D problem, but if a 3D problem was modelled by 100 ¥ 100 ¥ 100 20noded bricks the degrees of freedom escalate to 60 million!
58
Fundamentals of finite element analysis q
∂w ∂x Neutral axis
z
w (x)
x, u
4.13 Slender beam bending.
However, many composite structures are thinwalled shells and plates which are nevertheless expected to react loads or pressures applied to their surfaces, i.e. they have to bend. Such structures are amenable to the assumption that the bending strains vary linearly through their thickness and any inplane (membrane) loading leads to strains which are constant through the thickness. The shell or plate bending element, therefore, has a readymade strain field assumption through the thickness so that we only need to describe variations over the plate or shell midsurface. The simplest bending element is of course the 1D beam shown displaced in Fig. 4.13. The standard ‘beam theory’ assumption is that ‘plane sections remain plane’ and in the figure the unstrained neutral axis is shown displaced by w(x), and a vertical plane, originally normal to it, has rotated clockwise by q(x) about the yaxis. Remembering that displacements are very small, we may approximate the distance above the neutral axis as z and write u = zq The application of compatibility then produces e xx =
∂u dq =z ∂x dx
e xz =
∂u ∂w dw + = q+ ∂z ∂ x dx
and [4.35]
In most cases where beams are slender we find that shear strains are negligible. We cannot get away with this in laminated composites because the shear modulus, mainly because of the matrix, is an order of magnitude
Fundamentals of finite element analysis d2
d1
X
59
d4
d3
4.14 Cubic beam element freedoms (for continuity of displacement and slope).
smaller than the flexural modulus, which is mainly due to the much stiffer fibres. However, for an isotropic material we can neglect shear strains in a slender beam, i.e. exz 2h. A standard x, y, z coordinate system is located at the midplane of the free edge. If the origin is in the gauge section (i.e. away from the ends where the load is applied), the stresses can be assumed to be independent of x. Then, the equilibrium equations take the form txy,y + txz,z = 0 sy,y + tyz,z = 0 tyz,y + sz,z = 0
[7.3]
where a comma denotes partial differentiation. Based on the numerical results of Pipes and Pagano,8 Whitney suggested the following form of sy and txy in the free edge interval 0 y h: s y (z) È k ˘ 1  e  kpy (sin npy + cos npy )˙ c ÍÎ n ˚ ( ) tx z (1  e  kpy cos npy ) = c
sy = t xy
[7.4]
Interlaminar stresses and freeedge effects
129
where
[
n
c = 1  (1) e  kp y=
]
y , k>0 h
n is positive integer, and sy (z), and txy (z) are determined from lamination theory (equation [7.2]). Substituting equation [7.4] into equation [7.3] and then integrating with respect to z yields the remaining stresses:  pt yz (z)(n 2 + k 2 )  kpy e sin npy nc p 2 s z (z)(n 2 + k 2 )e ky (n cos npy  k sin npy ) sz = nc  pt xz (z)e ky (n sin npy + k cos npy ) t xz = nc t yz =
[7.5]
where z
[t yz (z), s z (z), t xz (z)] =  Ú h 2 [s y (z), t yz (z), t xy (z)], y dz Thus, equations [7.4] and [7.5] exactly satisfy the equilibrium equations as well as the freeedge boundary conditions. In addition, lamination theory is exactly recovered at y/h = 1.0. Compatibility, however, is violated. The solution of these approximate functions compares reasonably well with the exact solution obtained by Pipes and Pagano8 (shown in Fig. 7.3). The approximate results were obtained with n = 1 and k = 2. Whitney suggested that since the character of the solution is reasonably approximated with these values of n and k, in the absence of other information they may be used for general application.
7.3
Finite element analysis of straight edges
To illustrate the approach using FE, we consider a fourply symmetric laminate with (0/90°)s stacking sequence subjected to an inplane uniaxial tensile load, as shown in Fig. 7.4(a). The x–y plane of the Cartesian coordinate system lies in the midplane of the laminate; the xdimension is assumed to be much larger than the other dimensions of the plate. The plate width is four times the ply thickness. The 0/90° layup is selected for this analysis because of the large mismatch of mechanical properties between layers. The FE77 FE package, developed at Imperial College, Department of Aeronautics,20 is used, and the analysis is based on isoparametric eightnode elements. Owing to the symmetry of the loading and layup, only oneeighth of the laminate is modelled. Because high interlaminar stress
130
Analytical and numerical modelling
0°
90°
Free edge
7.4 (a) Crossply (0/90°)s laminate; (b) associated FE mesh.
concentration is expected near the free edge, and at the 0/90° interface, a refined mesh is required in this area; Fig. 7.4(b). Each ply is treated as a homogeneous, elastic and orthotropic material with the following elastic properties: E11 = 146.9 GPa, E22 = E33 = 10.89 GPa, G12 = G13 = 10.89 GPa, G23 = 6.4 GPa, u12 = u13 = 0.38 and u23 = 0.776. A uniform tensile strain, e0 = 106, is applied in the xdirection. The distributions of the throughthickness direct stress, sz, on the laminate midplane and on the 0/90° interface along the yaxis are plotted in Fig. 7.5(a) and (b), respectively. A good agreement between the current model and previous work8,21 is achieved near the laminate free edge (0 y/b 0.9). For a small distance, 0.7 y/b 0.8, there is a larger difference between the models, probably due to a different type of element and more refined mesh used in Wang and Crossman.21 Overall, the FE solution provides reasonable results for predicting the throughthickness stresses.
7.4
Finite element analysis of curved edges
7.4.1 Introduction Cutouts and holes are widely used in carbon fibrereinforced laminates for aircraft structures. The existence of the associated stress concentration will
Interlaminar stresses and freeedge effects
131
2500 Wang and Crossman21 3D model
2000 1500
sz
1000 500 0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
0
1.0 y/b
500 1000 (a) 2000 Wang and Crossman21 3D model
1500
sz
1000 500 0
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
0
1.0 y/b
500 (b)
7.5 Variation of throughthickness tensile stress across the width of the crossply laminate: (a) at laminate midplane, (b) at 0/90° interface.
initiate matrix cracking and delamination at the hole edge, especially under fatigue loading, which will lead to the loss of strength/stiffness and to potential environmental attack. It has been seen above that the straight free edge effect has been under consideration for more than 20 years. Because of the simplicity of the straight free edge geometry as compared with a curved free edge, fewer studies have been done on the latter. The straight free edge can sometimes be analysed as a problem with only 2D variations in stresses and displacements. Unfortunately, the stress state near a circular hole in a laminate is a complex 3D problem. The only exact solution to the problem is a 2D approximation.22 Approximate analytical methods23,24 and numerical approaches such as finite difference and FE methods25–27 have been used with some success to analyse the interlaminar stress distributions around curved free edges.
132
Analytical and numerical modelling
Recently, Ko and Lin28 have developed an analytical model to determine the interlaminar stresses around a circular hole in symmetric laminates under a set of farfield inplane stresses. This method uses the Kassapoglou–Lagace technique29 for the straight free edge in conjunction with boundary layer theory. The region of interest is divided into an interior region and a boundary layer region, and each stress component is determined by superposition of the interior stress field and the boundary layer stress. In the interior region, Lekhnitskii’s theory of 2D anisotropic elasticity22 in conjunction with classical lamination plate theory is adopted. The equilibrium equations in the boundary layer region are approximated by expressing the stress components as a perturbation series. The zerothorder approximation is then used for the solution of the interlaminar stresses in the boundary layer region.
7.4.2 An example Hu and Soutis30 and Hu et al.31 calculated the interlaminar stresses using a 3D FE analysis and evaluated the accuracy of the Ko–Lin model. The study was conducted on a plate of length L = 60 mm, width w = 30 mm, containing a central hole of radius R = 2.5 mm. Crossply (90/0°)s and (0/90°)s laminates, with ply thickness h0 = 0.125 mm, were examined since they show large mismatch of mechanical properties between adjacent plies and therefore significant throughthickness stresses. The FE77 FE package20 was used and the analysis employed curved isoparametric 20node elements. Owing to the symmetry of loading, hole location and layup, only oneeighth of the laminate was modelled. Because high interlaminar stress concentration is expected near the hole edge, and at the 0/90° interface, a very high mesh refinement is required in this area. The smallest element dimension in the radial and thickness directions was 0.000 25 mm. Figure 7.6 shows the FE mesh used. This FE model consisted of 4000 elements and solved a system of 56 000 linear equations. Each ply was treated as a homogeneous, elastic orthotropic material with the same elastic properties as those in the literature of Raju and Crews.26 7.4.2.1 Interlaminar normal stresses Figure 7.7 shows the interlaminar normal stress distributions at the 90/0° ply interface around the hole (z = h0 = 0.125 mm) of the (90/0°)s laminate. Since a mathematical interlaminar stress singularity exists at the free edge between the 90° and 0° plies, the computed stresses are presented near, but not at, the hole boundary. The stresses closest to the hole are at r/R = 1.0001; that is, at a distance of 0.002h0. from the hole boundary. As the distance from the edge, (r–R), increases, the interlaminar stress sz decreases rapidly.
Interlaminar stresses and freeedge effects
133
Hole edge
Sg
7.6 Threedimensional finite element mesh for oneeighth the notched (90/0°)s laminate.31 (sg = remote applied stress.)
0.2
0.1 (r–R)/R=0.0001 (r–R)/R=0.0002 0.0 sz /S g
(r–R)/R=0.001 (r–R)/R=0.01 (r–R)/R=0.1 Raju&Crews
0.1
Ko&Lin
28
0.2
0.3 0
10
20
30
40
50
60
70
80
90
q (deg)
7.7 Normalised interlaminar direct stress distributions around the hole at the 90/0° interface of the (90/0°)s laminate.31
26
134
Analytical and numerical modelling
When (r–R) = 0.1R, i.e. 0.25 mm, or two plythicknesses away from the hole boundary, sz becomes almost zero, and is compressive for most of the region around the hole, with a small tensile region near q = 90°. The largest compressive sz occurs at about 60° from the loading axis. The predicted values at the central (0/0°) interface are twice those developed at the (90/0°) interface. For the (0/90°)s layup, sz is again compressive for most of the region around the hole boundary, but is tensile in the regions 10° q 28° and 80° q 90°. Its largest compressive value occurs at around q = 60°. The stress distributions in Fig. 7.7 have similar shapes at different (r–R) distances from the hole edge, indicating that the location in the hoop direction is an important parameter for a curved free edge. This is the main difference from the straight free edge problem. For comparison purposes, Raju and Crews’ FE results26 at (r–R)/R = 0.000 1 are plotted in Fig. 7.7. The difference between the two FE solutions is negligible. However, the stress predictions of the Ko and Lin28 analytical model are in poor agreement, both qualitatively and quantitatively. This is probably due to the zerothorder approximation that those authors used when they solved the equilibrium equations in the boundary layer region. Although their solution satisfied the equilibrium conditions at the boundary, the circumferential stress and the laminate’s stress gradients in the radial direction were ignored. For the case of a hole, there are two stress gradients to be considered: the gradient in the interlaminar stresses near the hole, similar to the straight edge case; and also the gradient in the inplane stresses due to the presence of the hole, which gives an additional contribution to the gradient in the throughthickness stresses. Also, the Ko–Lin model does not ensure interface displacement continuity and predicts a significant interlaminar shear stress at the hole boundary near q = 90° where it should be zero. This suggests that their assumed boundary layer stresses need to be amended or a higherorder approximation should be employed in their stress solution. This is another indication of how much more complex the hole problem is compared with straight free edges. 7.4.2.2 Interlaminar shear stresses The circumferential interlaminar shear stress distributions tzq at various distances, (r–R)/R, from the hole boundary are shown in Fig. 7.8. Similarly to the normal stress, sz, the interlaminar shear stress tzq decreases as the distance (r–R) from the hole boundary increases, and becomes vanishingly small within two ply thickness (0.25 mm) from the hole. Except for different signs, the tzq distributions are identical for the (90/0°)s and (0/90°)s laminates. Both of these distributions have their maximum values at about 75° from the loading axis. The largest value in Fig. 7.8 is approximately 1.65Sg
Interlaminar stresses and freeedge effects
135
2.0
1.5 (r–R)/R=0.0001 (r–R )/R=0.0002 1.0 t zq /S g
(r–R )/R=0.001 (r–R )/R=0.01 (r–R )/R=0.1 Raju&Crews
0.5
Ko&Lin
28
0.0
0.5 0
10
20
30
40
50
60
70
80
90
q (deg)
7.8 Normalised interlaminar shear stress distributions around the hole at the 90/0° interface of the (90/0°)s laminate.31
(Sg being the remote applied stress), which is about ten times larger than the largest sz value (Fig. 7.7) computed for the same distance from the hole. This comparison indicates that the tzq stress singularity is stronger than that for the sz interlaminar stress. It also suggests that the interlaminar shear stresses are mainly responsible for delamination initiation in such laminates. The shear stress component tzr is very small compared with tzq and can be neglected. Raju and Crews’ FE results26 for tzq are in very good agreement with the present FE model, while those predicted by the Ko–Lin analytical model28 are lower by almost a factor of 3. The zerothorder approximation of the Ko–Lin analysis, although giving a good qualitative agreement with the numerical models, produces considerably lower interlaminar shear stresses and therefore will predict higher delamination onset stresses.
7.5
Summary
Interlaminar normal and shear stresses can be very high (perhaps even singular) at the free edge of a laminate (as at the edges on the sides of a
26
136
Analytical and numerical modelling
laminate, cutouts, holes, etc.). A tensile value of sz at a free edge may initiate delamination. Whereas delamination is important to the overall structural performance of laminates under tensile loading, it is critical for compression and shear loads where stability is of major concern. The stacking sequence in a laminate affects the magnitude as well as the nature of the interlaminar stresses. Interlaminar stresses can be regarded as an edge effect only since they are confined to a narrow region close to the edges. The predictions of laminated plate theory (LPT) are quite accurate in regions away from the edges (i.e. a distance equal to the laminate thickness). While free edges may not necessarily be important for real components the possibility of delamination at holes and cutouts has to be considered. The FE method can be applied to any layup configuration (thin or thick) under any loading condition, tension or compression, to estimate interlaminar stresses in laminates with an open hole. Further information on LPT and freeedge effects can be found in other composites textbooks, see for example [32–34].
7.6
References
1 Curtis P T, ‘The effect of edge stresses on the failure of (0/45/90°) CFRP laminates’, TR 80054, Farnborough, UK, Royal Aerospace Establishment, April, 1980. 2 Pagano N J & Halpin J C, ‘Influence of end constraints in the testing of anisotropic bodies’, J Compos Mater, 1968 2(4) 18–31. 3 Pagano N J, ‘Exact solutions for composite laminates in cylindrical bending’, J Compos Mater, 1969 3(3) 398–411. 4 Pagano N J, ‘Extract solutions for rectangular bidirectional composites and sandwich plates’, J Compos Mater, 1970 4(1) 20–34. 5 Whitney J M & Leissa A W, ‘Analysis of heterogeneous anisotropic plates, J Appl Mech, 1969 28 261–266. 6 Whitney J M, ‘The effects of transverse shear deformation on the bending of laminate plates’, J Compos Mater, 1969 3(4) 534–547. 7 Puppo A H & Evensen H A, ‘Interlaminar shear in laminated composites under generalised plane stress’, J Compos Mater, 1970 4(2) 204–220. 8 Pipes R B & Pagano N J, ‘Interlaminar stresses in composite laminates under uniform axial extension’, J Compos Mater, 1970 4(4) 538–548. 9 Pipes N J & Daniel I M, ‘Moiré analysis of the interlaminar shear edge effect in laminated composites’, J Compos Mater, 1971 5(2) 255–259. 10 Pagano N J & Pipes R B, ‘The influence of stacking sequence of laminate strength’, J Compos Mater, 1971 5(1) 50–57. 11 Foye R L & Baker D J, ‘Design of orthotropic laminates’, presented at the 11th Annual AIAA Structures, Structural Dynamics, and Materials Conference, Denver, CO., April 1970. 12 Whitney J M & Browning E E, ‘Freeedge delamination of tensile coupons’, J Compos Mater, 1972 6(2) 300–303.
Interlaminar stresses and freeedge effects
137
13 Whitney J M, ‘Freeedge effects in the characterisation of composite materials’, in Analysis of the Test Methods for High Modulus Fibers and Composites, ASTM STP 521, Philadelphia, PA, American Society for Testing and Materials, 1973. 14 Pipes R B, Kaminski B E & Pagano N J, ‘Influence of the freeedge upon the strength of angleply laminates’, in Analysis of the Test Methods for High Modulus Fibres and Composites, ASTM STP 521, Philadelphia, PA, American Society for Testing and Materials, 1973. 15 Isakson G & Levy A, ‘Finite element analysis of interlaminar shear in fibrous composites’, J Compos Mater, 1971 5(2) 273–276. 16 Rybicki E F, ‘Approximate threedimensional solutions for symmetric laminates under inplane loading’, J Compos Mater, 1971 5(3) 354–360. 17 Pagano N J, ‘On the calculation of interlaminar normal stress in composite laminate’, J Compos Mater, 1974 8(1) 65–81. 18 Pipes R B & Pagano N J, ‘Interlaminar stresses in composite laminates – An approximate elasticity solution’, J Appl Mech, 1974 41, Series E(3) 668– 672. 19 Tang S, ‘Interlaminar stresses of uniformly loaded rectangular composite plates’, J Compos Mater, 1976 10(1) 69–78. 20 Hitchings D, Finite Element Package FE77: User’s Manual, London, Imperial College, 1996. 21 Wang A S D & Crossman F W, ‘Some new results on edge effects in symmetric composite laminates’, J Compos Mater, 1977 11(1) 92–106. 22 Lekhnitsiskii S G, Theory of Elasticity of an Anisotropic Body, Moscow, Mir Publishers, 1981. 23 Tang S, ‘Interlaminar stresses of uniformly loaded rectangular composite plates’, J Compos Mater, 1976 10(1) 69–78. 24 Tang S, ‘A variational approach to edge stresses of circular cutouts in composites’. AIAA/ASME/ASCE/AHS/SDM Conference, St Louis, MO, 326–332, 1979. 25 Rybicki E F & Schmuesser D W, ‘Effect of stacking sequence and layup angle on free edge stresses around a hole in a laminated plate under tension’, J Compos Mater, 1978 12(7) 300–313. 26 Raju I S & Crews J H, ‘Interlaminar stress singularities at a straight free edge in composite laminates’, J Computers Structures, 1981 14(1–2) 21–28. 27 Kim J Y & Hong C S, ‘Threedimensional finite element analysis of interlaminar stresses in thick composite laminates’, J Computers Structures, 1991 40(6) 1395–1404. 28 Ko C C & Lin C C, ‘Method for calculating the interlaminar stresses in symmetric laminates containing a circular hole’, AIAA J, 1992 30(1) 197– 204. 29 Kassapoglou C & Lagace P A, ‘An efficient method for the calculation of interlaminar stresses in composite materials’, ASME J Appl Mech, 1986 53(4) 744–750. 30 Hu F Z & Soutis C, ‘Evaluation of the Ko–Lin model for interlaminar stresses in composite laminates with an open hole’, Adv Compos Letters, 1996 5(5) 143–147. 31 Hu F Z, Soutis C & Edge E C, ‘Interlaminar stresses in composite laminates with a circular hole’, Compos Struct, 1997 37(2) 223–232.
138
Analytical and numerical modelling
32 Jones R M, Mechanics of Composite Materials, USA, Taylor & Francis, 1975. 33 Agarwal B D & Broutman L J, Analysis and Performance of Fiber Composites, USA. J Wiley & Sons, Inc, 1990. 34 Halpin J C, Primer on Composite Materials Analysis, USA, Technomic Publishing Company Inc, 1992.
8 Fracture and fracture mechanics
8.1
Introduction
Typical engineering fibrereinforced plastics consist of brittle fibres, such as glass or carbon, in a weak brittle polymer matrix, such as epoxy or polyester resin. However, an important characteristic of these composites is that they are reasonably tough, largely as a result of their heterogeneous nature, the manner of their construction, and the widespread modes of fracture. During deformation, microstructural damage is extensive throughout the composite, but much damage can be sustained before loadbearing ability is impaired. Beyond some critical level of damage, failure may occur by the propagation of a crack which usually has a much more complex character than cracks in metals. Crack growth is inhibited by the presence of interfaces between fibres and matrix and between separate laminae in a multiply laminate. Compared with fracture in metals, research into the fracture behaviour of composites is quite limited. Much of the necessary theoretical framework is not yet fully developed and there is no simple recipe for predicting the toughness of all composites. We are not yet able to design with certainty the makeup of any composite so as to produce the optimum combination of strength and toughness. However, it will be apparent from what follows that the layup geometry of a composite strongly affects crack propagation, with the result that some laminates appear highly notchsensitive whereas others are totally insensitive to the presence of stress concentrators. The selection of fibres and resins, the manner in which they are combined in the layup, and the quality of the manufactured composite must all be carefully controlled if optimum toughness is to be achieved. Furthermore, requirements for highest tensile and shear strengths of laminates are often incompatible with requirements for highest toughness. Final selection of a composite for a given application may therefore be a matter of compromise.1
139
140
Analytical and numerical modelling Gc ª 2g s
Gc ª 2gF
G c < 2[g Fn f  g s (1  n f )]
Metal
Composite
Local stress Distance
Brittle solid
8.1 Schematic illustration of cracking mechanisms in different kinds of solids.1
8.2
Crack tip behaviour in homogeneous solids
The principal differences between cracking mechanisms in some familiar solids are shown in Fig. 8.1.1 In an ideal brittle solid, failure is elastic by the simple breaking of bonds across the crack plane, which remains relatively flat. The work of fracturing the solid in terms of the familiar Griffith model2 is approximately the work of creating two new surfaces: G @ 2g s =
ps 2 a E
[8.1]
where gs = specific surface energy, s = applied stress, a = one half crack length and E = modulus of elasticity. Griffith rewrote equation [8.1] in the form: 1
Ê 2Eg s ˆ 2 s= Ë pa ¯
[8.2a]
for the case of plane stress (biaxial stress conditions), and: 1
È 2Eg s ˘ 2 s=Í Î pa(1  u 2 ) ˙˚
[8.2b]
for the case of plane strain (triaxial stress conditions associated with the suppression of strains in one direction). The Poisson ratio, u, for most materials is between 0.25 and 0.33.
Fracture and fracture mechanics
141
It is important to recognise that the Griffith relation was derived for an ideal elastic material containing a very sharp crack. Although equations [8.2a] and [8.2b] do not explicitly involve the crack tip radius, r, that radius is assumed to be very sharp. As such, the Griffith relation, as written, should be considered necessary but not sufficient for failure. The crack tip radius would also have to be atomically sharp to raise the local stress above the cohesive strength. In materials such as metals and plastics, even relatively brittle ones, energy is dissipated in nonelastic deformation mechanisms in the region of the crack tip. This energy is lost in moving dislocations in a metal and in viscoelastic flow or craze formation in a polymer.The zone around the crack tip in which these deformation processes occur is called the ‘process zone’. In such real cases the fracture energy, G, is found to be several orders of magnitude greater that the material surface energy gs. Orowan3 recognised this fact and suggested that equation [8.1] be modified to include the energy of plastic deformation gp in the fracture surface, so that: G = 2( g s + g p ) = 2 g F
[8.3]
where gF is known as the ‘work of fracture’. Irwin4 also considered the application of Griffith’s relation, equation [8.2a], to the case of materials capable of plastic deformation. Instead of developing an explicit relation in terms of the energy sink terms, gs or (gs + gp), Irwin chose to use the energy source term (i.e. the elastic energy per unit increment of crack length, ∂U/∂a). Denoting ∂U/∂a as G, Irwin showed that a microcrack, or growth defect, may propagate at a nominal applied failure stress given by: 1
Ê EGIc ˆ 2 K Ic sf @ = Ë pa ¯ pa
[8.4]
where GIc and KIc are the critical elastic energy release rate and fracture toughness, respectively; KIc2 = EGIc for isotropic materials. The KIc parameter is a material property and can be measured in the laboratory with sharply notched test specimens. Equation [8.4] is one of the most important relations in the literature of linear elastic fracture mechanics (LEFM). Fracture mechanics has been used successfully in the development of structural materials in two complementary ways: firstly, by relating KIc to microstructure; secondly, by identifying the origins of cracking. The strength of a component can then be maximised by optimising the microstructure through careful control of manufacturing conditions to reduce flaw size and increase KIc. This requires an understanding of the dependence of KIc (or GIc) on microstructure.
142
Analytical and numerical modelling
In general, materials that show some ductility can fail in one of two competing ways, depending on the site of any crack or notch they may contain. A material containing a short notch fails by general damage, in which ductile fracture occurs at a net section stress which is independent of notch length. Alternatively, the localised stresses at the tip of a long notch or crack may be large enough to cause crack propagation, while deformation in the bulk of the material remains __ elastic. In this case fracture occurs at a stress that is proportional to 1// a (equation [8.4]). We call this the regime of single crack propagation. In composite materials, the fibres interfere with crack growth, but their effect depends on how strongly they are bonded to the matrix (resin). For example, if the fibre/matrix bond is strong, the crack may run through both fibres and matrix without deviation, in which case the composite toughness would be low and approximately equal to the sum of the separate constituents’ toughness: G @ 2[(g F ) f vf + (g F )m (1  vf )]
[8.5]
where (gF)f and (gF)m are the fibre and matrix work of fracture, respectively. The fibre volume fraction is vf. On the other hand, if the fibre/matrix bond is weak the crack path becomes very complex and many separate damage mechanisms may then contribute to the overall fracture work of the composite. These fracture processes are controlled by the constituent materials of the composite and the manner of their combination. For example, a brittle polymer or epoxy resin with GIc @ 0.1 kJ/m2 and brittle glass fibres with GIc @ 0.01 kJ/m2 can be combined together in composites some of which have energies of up to 100 kJ/m2. For an explanation of such a large effect we must look beyond simple addition.
8.3
Crack extension in composites
Many authors have attempted to apply fracture mechanics to fibrereinforced composites and have met with mixed success. Conventional fracture mechanics methodology assumes a single dominant crack that grows in a selfsimilar fashion; i.e. the crack increases in size (either through stable or unstable growth), but its shape and orientation remain the same. Fracture of a fibrous composite, however, is often controlled by numerous microcracks distributed throughout the material, rather than a single macroscopic crack. There are situations where fracture mechanics is appropriate for composites, e.g. for delamination, but it is important to recognise the limitations of theories that were intended for homogeneous materials. Figure 8.25 illustrates various failure mechanisms in fibrereinforced
Fracture and fracture mechanics
143
1. Fibre pullout. 2. Fibre bridging. 3. Fibre/matrix debonding. 4. Fibre failure. 5. Matrix cracking.
(a) Inplane damage
(c) Fibre microbuckling
(b) Delamination
(d) Delamination buckling
8.2 Examples of damage and fracture mechanisms in fibrereinforced composites.5
composites. One advantage of composite materials is that fracture seldom occurs catastrophically without warning, but tends to be progressive, with substantial damage widely dispersed throughout the material. Tensile loading, Fig. 8.2(a), can produce matrix cracking, fibre bridging, fibre rupture, fibre pullout and fibre/matrix debonding. Ultimate tensile failure of a fibrous composite often involves several of these mechanisms. Outofplane stresses can lead to delamination, Fig. 8.2(b), because the fibres do not contribute significantly to strength in this direction. Compressive loading can produce microbuckling of fibres, Fig. 8.2(c); since the polymer matrix is soft compared with the fibres, the fibres are unstable in compres
144
Analytical and numerical modelling
(a)
(b)
(d)
(c)
(e)
8.3 Schematic representation of stages in crack growth in a fibre composite.1
sion. Compressive loading can lead also to macroscopic delamination buckling, Fig. 8.2(d), particularly if the material contains a preexisting delaminated region. All these failure mechanisms absorb energy and contribute to the fracture toughness of the composite. In order to distinguish the separate micromechanisms of toughening due to true composite action, it is convenient to consider a simple model in which a crack travelling in the resin approaches an isolated fibre; Fig. 8.3a.1 A crack propagating in the matrix phase is effectively stopped by a fibre; Fig. 8.3(b). As the load on the composite is increased, matrix and fibre at the crack tip deform differentially and a large local stress builds up in the fibre. This stress causes local Poisson contraction which, exacerbated by the tensile stress normal to the interface ahead of the crack tip, initiates fibre/resin debonding (or decohesion); Fig. 8.3(c). The interfacial shear stress resulting from fibre/matrix modulus mismatch will then cause extension of the debond along the fibre in both directions away from the crack
Fracture and fracture mechanics
145
plane. This permits further opening of the matrix crack beyond the fibre, and the process is repeated at the next fibre. An upper limit to the energy of debonding is given by: Wdebond =
Npd 2 s 2f y 8Ef
[8.6]
for a composite with N fibres of diameter d, failure stress sf and modulus Ef. The mean bonded length is y. After debonding, the fibre and matrix move relative to each other as crack opening continues and work must be done against frictional resistance during this process. One estimate, assuming that the interfacial frictional stress, t, acts over a distance equal to the fibre failure extension, suggests that this contribution is equal to: Wfriction =
Npdy 2 pe f 2
[8.7]
where ef, the fibre failure strain, contributes substantially to the toughness of fibre/resin composites. After debonding a continuous fibre is loaded to failure over a distance equal to the debonded length and it may break at any point within this region; Fig. 8.3(d). The broken ends retract and regain their original diameters and they are regripped by the resin. In order to permit further opening of the crack, and ultimately separate the two parts of the sample, these broken ends must be pulled out of the matrix; Fig. 8.3(e). Further frictional work is needed to accomplish this. Crude estimates of the pullout work give: Wpullout =
Npdlc2 t 12
[8.8]
where lc is the critical length, and the distance over which the fibre end is pulled out is given approximately by lc/4. It can be shown that, in aligned short fibre composites, the work of pullout will be at a maximum when the reinforcing fibres are exactly of the critical length. It should be noted that composite toughness ought to be increased by raising the fibre volume fraction, vf, increasing the fibre diameter, d, or using stronger fibres. Contrary to expectation, however, improving the fibre/ matrix bond will usually reduce the toughness because it inhibits debonding and therefore reduces pullout. The behaviour of many types of composite has been reasonably well explained in terms of summation of the contributions from these mecha
146
Analytical and numerical modelling
nisms but it is not yet possible to design a composite to have a given toughness. Clearly, ease of cracking in unidirectional laminates will be strongly dependent on fibre orientation. In GRP and CFRP, for example, the energy for fracture parallel to the fibres is two orders of magnitude less than that normal to the fibres. The same is true of wood. Simple crack interactions rarely occur in practical composites made by bonding together several plies with differing fibre orientations. The variation of axes of anisotropy from lamina to lamina results in coupling shear stresses in the plane of the plate when the composite is loaded and, since the interlaminar planes are always planes of weakness, it follows that interlaminar shear stresses may easily become so large as to delaminate the composite well before fibre fracture can occur. Cracks are also caused to deviate along these planes of weakness. Because of the increased surface area associated with this form of cracking the composite toughness is substantially increased. Delamination can be considered as a special case, and is dealt with separately in the next chapter.
8.4
Application of fracture mechanics to composites
8.4.1 Notched strength and notch sensitivity Frequently the design of composite structures includes holes introduced either intentionally as cutouts and as fastener holes, or unintentionally due to damage events. Several investigators (e.g. Waddoups et al.6 and Soutis et al.7) have examined the behaviour of notched composite laminates and found that open holes reduced the tensile or compressive strength of the laminate by more than 50%. However, the remote failure stress is well above the value one might predict from the elastic stress concentration factor, indicating that the composite material is not ideally brittle and some stress relief occurs around the hole.7,8 In Fig. 8.4 the remote compressive failure stress, sn, normalised by the unnotched failure strength, sun, of the laminate is plotted as a function of hole radius R normalised by semiwidth W of the specimen. The high stresses at the hole boundary initiate localised damage which results in a redistribution of stresses. Such damage will take the form of delamination, matrix cracking, splitting, fibre fracture (fibre microbuckling in compression). It is reasonable to expect that fast fracture of the laminate will occur when the size of the delaminations, or the length of the crack tip split, or size of the damage zone, exceeds some critical value. Various theoretical models have been developed to predict notched tensile fracture.6,9 Some of the models have been extended to include compressionloaded laminates.10 More recently the progressive development of fibre microbuckling leading to ultimate compressive failure has been modelled successfully by Soutis and coworkers.7,8
Fracture and fracture mechanics
147
L1: [( ± 45 04) 2 ] s , L2: [( ± 45 02) 3 ] s, L3: [ ( 0 902 0 ) 3 ] s, L4: [± 45 02 902 02 902 02 ] s, L5: [( ± 45 0 90) 3 ] s ,L6: [( ±45) 2 0 ( ±45) 2 0 ±45] s Lay–up 1.0
s•
L4 L5 L6
L1 L2 L3
2R 0.8
No
0.6
tc h
in s
en
2W s it
iv e
sn s un
s•
0.4 R sn = (1 ) W s un
0.2 Notch sensitive,
sn 1 = s un k †
0.0 0.0
0.2
0.4
0.6
0.8
1.0
R W
8.4 Effects of hole diameter on the compressive strength of T800/924C laminates.8
8.4.2 Inherent flaw model Waddoups et al.6 postulated the existence of a ‘highintensity energy region’, adjacent to a circular hole in a composite plate under uniaxial tensile load; Fig. 8.5. The high intensity energy region is presumed to behave like a crack of length a0. The fracture strength of the laminate sn, is taken from the toughness KIc and a0, given the geometry and stress intensity factor, KIc. Waddoups made use of Bowie’s solution11 for the stress intensity factor, for the problem of cracks emanating from a circular hole in an isotropic homogeneous infinite plate. It was shown that the flawed, or notched, strength (sn) and unflawed, or unnotched, strength (sun) of the composite are related by: s un = f (a0 r ) sn
[8.9]
where the correction factor, f(a0/r), from Bowie is given in Table 8.1. Waddoups considered a (0/±45°)2s carbon fibre/epoxy laminate containing
148
Analytical and numerical modelling
Table 8.1 Correction factors f(ao /r)11 a/r
0.1
0.2
0.3
0.4
0.5
0.6
0.8
1.0
f(ao /r)
2.73
2.41
2.15
1.96
1.83
1.71
1.58
1.45
s•
a0
R
s•
8.5 Damage zone of size ao, at edge of a hole or cutout.6
a circular hole, the strength data for which are given in Table 8.2. Inserting values of sun = 524 MPa and sn = 192 MPa into equation (8.9) gives: f (a0 r ) =
s un 524 = = 2.72 sn 192
From Table 8.1 we see that a0/r = 0.1 and therefore a0 = 1.27. We now calculate KIc using: 1
K Ic = s n (pa0 ) 2 f (a0 r ) @ 31 MPa m Assuming that KIc is a laminate property, we can then determine the notched strength for specimens containing holes of diameters 63 mm and 75 mm. Values of sn calculated this way are 166 MPa and 164 MPa, respectively, which compare favourably with experimental measurements of 157 MPa and 156 MPa given in Table 8.2.
Fracture and fracture mechanics
149
Table 8.2 Hole data summary6 Specimen (965 mm ¥ 125 mm)
Static strength (MPa)
Control (no hole)
524
25 mm diameter hole
192
63 mm diameter hole
157
75 mm diameter hole
156
8.4.3 Stress intensity factors for a cracked hole laminate For isotropic materials the subject of linear elastic fracture mechanics (LEFM) is highly developed and the plane strain fracture toughness, KIc, is treated as a material property. Paris and Sih12 developed expressions for the crack tip stress field for a linear elastic anisotropic material for the case of plane strain and pure shear. The crack tip stress field exhibits the same r1/2 singularity with distance r from the crack tip as for the isotropic case. Also the stress intensity factors (SIF), KI, KII, KIII, have the same meaning as for the isotropic case. Linear elastic fracture mechanics can be applied to composite laminates provided the damage zone at the crack tip is contained within the Kfield, i.e. provided the damage zone is small compared with other dimensions of the specimen. The stress intensity factor for a finite 2D isotropic plate, subjected to mode I loading and containing a cracked hole, Fig. 8.5, is given by K I = s • p (r + a0 ) f (a0 r )F (r , a0 , w)
[8.10]
where s• is the applied far field stress and the factor f(a0/r) reflects the influence of the cracked hole on the SIF. Function F is the finite width correction factor that also depends upon material anisotropy. Using FE analysis, KI for an orthotropic T800/924C carbon fibre/epoxy laminate, with cracks emanating symmetrically from a circular hole, is now determined. A number of techniques are currently used for evaluating SIFs. Here, the Virtual Crack Extension (VCE) procedure in the FE77 finite element package, with an eightnode isoparametric element, is used to obtain the SIF for the problem shown in Fig. 8.5. The fundamental difficulty in a crack problem is the singularity in the strain field at the crack tip. The finite element mesh must be such that the singularity is approximated with sufficient accuracy. Many methods have been devised to arrive at such an approximation; one commonly used method is the quarter point element where a degenerate form of the stan
150
Analytical and numerical modelling
8.6 FE mesh around circular cutout.
6 4 1
7
8
100 5 2
101
102
3
8.7 FE representation of crack.
dard eightnode quadrilateral element is employed. This isoparametric element produces the r1/2 singularity when it degenerates to a triangular element and the midside nodes are moved to the quarter point adjacent to the crack tip node.13 In the FE77 code a refined mesh is required, Fig. 8.6, where the ‘interface disconnect’ subroutine is used to represent the crack, Fig. 8.7. The FE77 program allows the evaluation of the Jintegral by disconnecting nodes in certain elements ahead of the crack tip, Fig. 8.8, to represent a differential crack advance, dl, and measuring the change in strain
Fracture and fracture mechanics
6 4 1
8 6
7
7
8 102
100 5 4 101 5 2
3 1
2
151
3
8.8 Incremental advance of crack.
8.9 Deformed mesh for cracked hole.
energy dU. The Jintegral is the negative differential of strain energy with respect to crack advance. For an elastic body J is identical to the elastic strain energy release rate G. Hence; G=J=
dU dl
[8.11]
A typical deformed configuration of the plate with a cracked hole loaded in tension is shown in Fig. 8.9.
152
Analytical and numerical modelling
Analytical solution (isotropic material) FE method simulation orthotropic material
8.10 Variation of stress intensity factor with crack length.
For an orthotropic laminate the energy release rate GI is related to the stress intensity factor KI by: Ê a11a12 ˆ GI = Ë 2 ¯
1 2
ÈÊ a22 ˆ ÍË Î a11 ¯
1 2
2a12 + a66 ˘ + ˙ 2a11 ˚
1 2
K I2
[8.12]
where aij are the coefficients of the laminate compliance matrix, related to elastic constants Ex, Ey, Gxy and uxy.7 Of course, GI = K 2I /E for isotropic materials. In order to investigate the accuracy of the FE model an elastic stress analysis is performed. The SIF for a T800/924C quasiisotropic (±45/0/90°)s cracked hole specimen, with r/W = 0.25, is shown in Fig. 8.10 and is compared with the analytical solution for an isotropic plate. It is clear from these results that the singularity in the stress field at the crack tip is approximated with sufficient accuracy, and the difference in the solution for KI is small. Of course, the SIF cannot strictly be implemented in the inherent flaw fracture model described in Section 8.4.2 to predict the ultimate tensile strength of any orthotropic notched laminate, since the Bowie correction factor in Table 8.1 is for an isotropic plate. For the quasiisotropic (±45/0/90°)s laminate, however, the anisotropic effect is negligible and the isotropic SIF can be employed. The method described here is more useful for anisotropic layups where an analytical solution does not exist.
Fracture and fracture mechanics
153
s•
y
sy s0 d0 a0
R
x
s•
8.11 Point and average stress failure criterion.9
8.4.4 Point stress and average stress failure criteria Whitney and Nuismer9 have extended the Waddoups model6 to explicitly include the anisotropy of the material. In their analysis, orthotropic symmetry is assumed. For a plate containing a circular hole of radius R, the ratio of notched strength to the unnotched strength is given by: sn 1 = 2[2 + z12 + 3z14  (K T•  3)(5  z16  7z.8 )] s un
[8.13]
where z = R/(R + d0) and KT• = stress concentration factor for an orthotropic laminate. As in the Waddoups’ analysis, the assumption is that failure occurs when the stress at a point, a distance d0 from the hole edge, reaches a critical value; Fig. 8.11. We can, in an alternative model, assume failure to occur when the average value of sy over a distance a0 in front of the hole exceeds the unnotched tensile strength of the material; Fig. 8.11. In this case: sn 1 = 2(1  z 2 )[2  z 22  z 42 + (K T•  3)(z 62  z82 )] s un where z2 = R/(R + a0).
[8.14]
154
Analytical and numerical modelling
1.0 d0 = 1mm a0 = 3.8 mm s un = 494 MPa
0.8
s n /s un
0.6
0.4
0.2
0
2.5
5.0
7.5
10.0
12.5
Notch half length, a (mm)
8.12 Comparison of predicted and experimental failure stresses for centre cracks in (0/±45/90°)2s HTS carbon fibre/epoxy resin.
For an infinite anisotropic plate containing a centre crack of length 2c, subjected to a uniform uniaxial tensile load, the point stress failure criterion gives: 1 sn = (1  z 32 ) 2 s un
[8.15]
and the average stress failure criterion gives: 1
sn Ê 1  z4 ˆ 2 = s un Ë 1 + z 4 ¯
[8.16]
Here, z3 = c/(c + d0) and z4 = c/(c + a0). In the Whitney–Nuismer models the characteristic length a0 (or d0) is used as a free parameter to be fixed by best fitting the experimental data. An example of a comparison between theory and experimental data is shown in Fig. 8.12 for centre notched (0/±45/90°)2s laminates made from high tensile strength (HTS) carbon fibre/epoxy. Here sn/sun is plotted against notch length c. The theoretical curves of sn/sun against notch size are computed using equations [8.15] and [8.16]. Values of d0 = 1 mm and a0 = 3.8 mm provided the best fit to these and other data for laminates with both circular holes and central cracks.
Fracture and fracture mechanics
155
The models described above assume that KIC and a0 (or d0) are invariant material properties. However, the fracture toughness and characteristic lengths depend on fibre and resin type, ply distribution and layer thickness. It is probably better to consider these parameters as laminate rather than ply properties, that have to be determined experimentally.
8.5
Progressive failure models
Recently, more interest has been placed on progressive failure modelling.14–16 The mechanisms for damage progression and accumulation in notched laminates are so complicated (combinations of matrix cracking, longitudinal splitting, delamination and fibre breakage) that analytical methods are impractical and, perhaps, unable to model them. The most suitable tool is probably the FE method. The damage progression around a hole can be determined by performing a plybyply and elementbyelement stress analysis and applying appropriate stress or strainbased failure criteria. If no laminae have failed, the load must be determined at which the first lamina fails, that is, violates the failure criterion. The load parameter is increased until some lamina fails. That lamina is then eliminated from the laminate by assigning zero stiffness (ply discount technique), or reduced properties (stiffness degradation factors), to the failed layer and new laminate extensional, coupling and bending stiffnesses (ABD) are calculated. Laminae stresses are recalculated to determine their distribution after a lamina has failed (the stresses will increase to maintain equilibrium). Then it must be verified that the remaining laminae, at their increased stress levels, do not fail at the same load that caused failure of the lamina in the preceding pass through the analysis. If no more laminae fail, then the load can be increased until another lamina fails and the cycle is repeated until last ply failure. The overall procedure for strength analysis is independent of the failure criterion, but the results of the procedure, the maximum loads and deformations, will depend on the specific failure criterion. The laminate behaviour could be piecewise nonlinear if the laminae behaved in a nonlinear elastic manner. The results of such models include the whole field stress–strain relationship, the laminate stiffness degradations and the extent of damage at any stress level. The computing time varies significantly from one mesh design to another, depending on the number of elements. Although a finer mesh predicts failure progression better than does a coarse mesh, it needs more computing time. The increase in computing time may not be worth the increase in accuracy after the number for elements reaches a certain value. Figure 8.13(a) and (b) illustrate damage growth, in the form of matrix cracking, developed in the 90° ply of a (0/90°)s carbon fibre/epoxy laminate at uniaxial tensile loadings of 43.8 kN and 97.18 kN, respectively.
156
Analytical and numerical modelling
8.13 Finite element modelling of matrix cracking growth in the 90° ply of a cracks in (0/90°)s CFRP laminate: (a) applied load of 43.8 kN; (b) applied load of 97.18 kN.
8.6
Summary
We have seen that a number of parameters such as the critical strain energy release rate, GIc, and the critical stress intensity factor, KIc, may specify the toughness of a material. Fracture toughness parameters enable the critical flaw size in a component subjected to a given stress to be determined. Under some circumstances linear elastic fracture mechanics (LEFM) can be used directly to describe fracture behaviour in composites and measure their notch sensitivity. Typically this applies to 0° dominated laminates of brittle composites (e.g. (0/±45°)s, (0/90°)s) with high fibre/resin bond strengths and brittle matrices. In such laminates crack paths may be planar, or nearly so, and damage zones small (e.g. 1–2 mm). LEFM seems to predict notched strength reasonably well in quasiisotropic (0/±45/90°)s laminates where there is a lower percentage of 0° fibres. The methods of LEFM become invalid for angleply dominated laminates, e.g. (±45°)s, which are commonly notch insensitive. For these laminates the damage is diffuse in nature, and a cracklike representation of damage becomes inappropriate.
Fracture and fracture mechanics
157
The important message is that generalisations should not be made. There is always likely to be uncertainty over the question of validity of LEFM for any given case.1 The FE method can be used successfully to predict the orthotropy effect on SIFs that are required in stress based failure criteria. It can also be used to model damage progression around open holes by performing plybyply and elementbyelement analysis, taking into account geometric and material nonlinearities.
8.7
References
1 Harris B, Engineering Composite Materials, London, Institute of Materials, 1986. 2 Griffith A A,‘Fracture’, Phil Trans Roy Soc, London, 1920 Ser. A221 163 (Republished with additional commentary in Trans ASM, 1968 61, 871). 3 Orowan E, Fatigue and Fracture of Metals, Cambridge, MA, MIT Press, 1950. 4 Irwin G R, Fracturing of Metals, Cleveland, OH, ASM, 1949. 5 Anderson T L, Fracture Mechanics: Fundamentals and Applications, Boca Raton, CRC Press, 1991. 6 Waddoups M E, Eiseman J R & Kaminski B E, ‘Macroscopic fracture mechanics of advanced composite materials’, J Compos Mater, 1971 5(10) 446–454. 7 Soutis C, Fleck N A & Smith P A, ‘Failure prediction technique for compression loaded carbon fibreepoxy laminate with open holes’, J Compos Mater, 1991 25(11) 1476–1498. 8 Soutis C & Fleck N A, ‘Static compression failure of carbon fibre T800/9246 composite plate with a single hole’, J Compos Mater, 1990 24(5) 536–558. 9 Whitney J M & Nuismer R J, ‘Stress fracture criteria for laminated composites containing stress concentrations’, J Compos Mater, 1974 8(7) 253–265. 10 Rhodes M D, Mikulus M M & McGowan, ‘Effects of orthotropy and width on the compression strength of graphite/epoxy panels with holes’, AIAA J, 1984 22(9) 1283–1292. 11 Bowie O L,‘Analysis of an infinite plate containing radial cracks originating from the boundary of an internal circular hole’, J Maths Phys, 1956 35(1) 60–71. 12 Paris P C & Sih G C, ‘Stress analysis of cracks, fracture toughness testing and its implications’, ASTM STP 381, Philadelphia, PA, American Society for Testing and Materials, 1965. 13 Marti V & Valliappon S, ‘A universal optimum quarter point element’, Engineering Fracture Mechanics, 1986 25(2) 237–258. 14 Tan S C, Stress Concentrations in Laminated Composites, Lancaster, PA, Technomic Publishing Co Inc, 1994. 15 Chang F K & Chang K Y, ‘A progressive damage model for laminated composites containing stress concentrations’, J Compos Mater, 1987 21(9) 834–855. 16 Tan S C & Nuismer R J, ‘A theory for progressive matrix cracking in composite laminates’, J Compos Mater, 1989 23(10) 1029–1047.
9 Delamination
9.1
Introduction
The fracture processes in composite laminates under tensile monotonic and fatigue loading involve a sequential accumulation of damage in the form of matrix cracking, local delamination and edge delamination prior to catastrophic failure.1–4 Edge delamination initiates at loadfree edges of the composite plate due to Poisson’s mismatch (see Chapter 7), whereas local delamination originates from the interaction of matrix ply cracks at ply interfaces.5 These ‘resindominated’ failure modes can be detrimental to the strength of the laminate since they can cause fibre fracture in the primary loadbearing (0°) plies. It is therefore important to be in a position to predict their onset strain and growth. Over the years a number of researchers have shown that the strain energy release rate, G, associated with local delamination can be compared with an appropriate value of interlaminar fracture toughness, obtained experimentally,6 to estimate the initiation and propagation of delamination. O’Brien3,4 derived a closedform equation for G which, for certain layups, can successfully predict the delamination onset strain. However, the author neglected the effect of matrix ply cracking which becomes important for laminates containing thick 90°plies where local delaminations usually develop. More recently, Zhang and Soutis7 modelled the matrix crack tip delamination and its effect on the stiffness properties of carbon fibre/epoxy laminates. A 2D shear lag approach was followed to obtain the microstress field in the damaged laminate. These resulting microstresses were used in an in situ damage effective function (IDEF) which was derived explicitly in terms of matrix crack density and relative local delamination area. Then, expressions for the strain energy release rates for matrix cracking and local delamination were derived, taking into account residual hygrothermal stresses and the interaction effect between the two damage modes. Further details are given below. As mentioned in Chapter 6, FE analyses have used a number of 158
Delamination
159
±q
(90)n
±q
Matrix crack
Local delamination
9.1 The (±qm/90°n)s laminate with matrix cracks and local delamination.
approaches to represent delamination, including the Virtual Crack Closure (VCC) method, as well as employing special ‘delamination’ elements (Sections 6.8 and 6.10). Again, results from such analyses will be given below.
9.2
A continuum model
When a (±qm/90°) n s balanced symmetric laminate is under static or fatigue tensile loading, matrix cracking in the transverse plies (90°) is the first damage mode observed and multiplies with increasing applied load or number of cycles. Subsequently, either edge delamination will form at the q/90° interface, or local delamination will initiate from the transverse ply crack tips due to high local stresses at the crack tip. A schematic of the damage configuration is shown in Fig. 9.1. The midregion is made of 90° plies, while the constraining layers (sublaminate) consist of multiorientation plies (±q). Transverse ply cracks are assumed to exist in the 90° plies with uniform crack spacing of 2s; local delaminations initiate and grow from both tips of each transverse crack and span the width of the specimen. Following previous work,7–9 in order to examine the effect of these damage modes on the laminate loading capacity, a representative threelayer segment, Fig. 9.2, containing a single transverse ply crack and two stripshaped delaminations is considered. This element can be segregated into a locally delaminated region 0 y ld and a nondelaminated region ld y s. The effect of the cracking and the delaminations is to reduce the stiffness of the laminate.
9.2.1 Stiffness reduction The modified stiffness matrix of a cracked lamina has been derived8 by introducing the IDEF, Lij, and is given by:
160
Analytical and numerical modelling z
– s y
w
– s y
h1 2h2 h1
2ld
y
1 2 1
2s
x
9.2 A threelayer element with local delamination growing from a 90° matrix crack.
( 2) ÈQ11 ÍQ ( 2) Í 12 ÍÎ 0
Q12( 2) ( 2) Q22 0
0 ˘ ÈQ110 Q120 0 0 ˙˙ = ÍQ120 Q22 Í ( 2) Q33 ˙˚ ÍÎ 0 0
0 ˘ 0 ˙ ˙ 0 ˙˚ Q33
È 0 2 ˘ [9.1] Í (Q12 ) ˙ 0 Q L 12 22 0 ˙ Í Q 0 L 22 ˙  Í 220 0 Q22 0 ˙ L 22 Í Q12 L 22 Í ˙ 0 Q33 0 0 L 33 ˙ ÍÎ ˚ where Q0ij is the inplane stiffness matrix of the 90° (ply 2) uncracked lamina. The L22 and L33 parameters describe the stiffness loss of the 90° ply caused by matrix cracking; they are functions of the average matrix crack density, Cd, and also of the in situ constrained conditions of the 90° plies. In order to calculate L22 and L33 a 2D shearlag analysis was proposed,7,8 where the outofplane shear stresses varied linearly across the thickness of the constraining layers (ply 1); Fig. 9.3. Combining this shear stress variation with outofplane stress/strain and strain/displacement relations, and taking the average values across the ply thickness, the interface shear stresses were expressed in terms of inplane displacements. Once the microstress field in the cracked laminate was obtained the macro stresses in the cracked 90° plies could be determined by integrating over the laminate length. Substituting these stresses into the damaged constitutive equation of the 90° plies, the L22 and L33 were derived as functions of matrix crack density. When delamination is present, growing from the transverse ply crack tips, the locally delaminated portion of 90° plies is not able to carry normal load in the ydirection and shear loads in xz and yzplanes; the overall laminate stiffness properties are further reduced by the local delaminations. The influence of the local delamination and matrix cracking on the overall laminate response was considered5 by including the two damage modes in the
Delamination
161
tx ,ty
(1)
(2)
(1)
(2)
sxz , syz
sxz , syz
hs h1
h2
1
2
z
9.3 Outofplane shear stress variation across the thickness of the 90° ply (ply ‘2’) and the constraining layer (ply ‘1’).
reduced lamina stiffness matrix of the 90° plies; equation [9.1]. The L22 and L33 coefficients are given by
L 22
Ê l1 (1  D ) ˆ F1 (1  Dld ) + F 2 Dmc tanh Ë ¯ Dmc = 1ld ( ) l 1 D Ê 1 ˆ F1 (1 + z1 Dld ) + F 3 Dmc tanh Ë ¯ Dmc
[9.2a]
L 33
Ê l 2 (1  D ) ˆ G1 (1  Dld ) + G2 Dmc tanh Ë ¯ Dmc = 1ld ( )ˆ l 1 D Ê 2 G1 (1 + z 2 Dld ) + G3 Dmc tanh mc Ë ¯ D
[9.2b]
ld
ld
where Dmc(= h2/s = 2h2Cd) and Dld(= ld/s = 2ldCd) are the relative matrix crack density and the relative local delamination area, respectively. The parameters Fi, Gi, zi and li are functions of laminate elastic constants. When delamination is ignored, equations [9.2a] and [9.2b] reduce to the corresponding relations for pure matrix cracking derived in reference 7.
9.2.2 Constitutive relationship of the damaged laminate Let a laminate be subjected to inplane loading under isohygrothermal conditions, and be deformed and cracked progressively. Following previous
162
Analytical and numerical modelling
work8,9 the macrostress or total stress vector in the kth ply group can be written in terms of the strain vector and the reduced lamina stiffness properties (k ) (k ) Ès x ˘ ÈQ11 Ís (k ) ˙ = ÍQ (k ) Í y ˙ Í 12 (k ) (k ) ÎÍs xy ˚˙ ÍÎQ13
Q12(k ) Q22(k ) Q23(k )
Q13(k ) ˘Ê È e x ˘ È e (xk ) RT ˘ È e (xk ) RH ˘ˆ Q23(k ) ˙˙Á Í e y ˙ + Í e (yk ) RT ˙ + Í e (yk ) RH ˙˜ ˙ Í ˙˜ ÁÍ ˙ Í Q33(k ) ˙˚Ë ÎÍg xy ˙˚ ÍÎg (xyk) RT ˙˚ ÍÎg (xyk) RH ˙˚¯
[9.3a]
or s k = Qk (e + e kRT + e kRH )
[9.3b]
RH are the residual thermal and hygroscopic (moisture) where e RT k and e k strain vectors in the laminate due to the temperature and moisture difference between the stressfree state and the ambient state. They can be computed using Classical Laminate Theory. The constitutive equation of the damaged laminate is found to be:
È N x ˘ È A11 Í N ˙ = ÍA Í y ˙ Í 12 ÍÎN xy ˙˚ ÍÎ 0
A12 A22 0
0 ˘Ê È e x ˘ È e xp ˘ˆ 0 ˙Á Í e y ˙  Í e yp ˙˜ ˙Á Í ˙ Í ˙˜ p ˙˚¯ A33 ˙˚Ë ÍÎg xy ˙˚ ÍÎg xy
[9.4a]
or N = A(e  e p )
[9.4b]
with e p = A 1 (N T + N H  A 01N 0T + N 0H )
[9.5]
where A is the extensional stiffness matrix of the damaged laminate, and N T and N 0T are the equivalent thermal loads in the damaged and undamaged states, with N H and N 0H the respective equivalent moisture loads. It is observed that the laminate develops permanent strains due to the interaction effect between damage and residual hygrothermal stresses.
9.2.3 Energy release rate The potential energy method of Zhang and Soutis9 is used here to derive expressions for the energy release rates associated with local delamination, matrix cracking and their interaction. The potential energy (PE) of the equivalent damaged laminate element with a finite length 2l and width w is: PE = U  N te2lw
[9.6]
Delamination
163
where U is the total strain energy stored in the laminate element which is a function of matrix cracking density and local delamination area. Its calculation requires a plybyply analysis in order to take into account the contribution of residual hygrothermal stresses.The energy release rate associated with a particular damage mode is equal to the first partial derivative of the potential energy with respect to the crack surface area of the respective damage. The applied laminate loads, N, are fixed and the other damage modes remain unchanged. So, the strain energy release rates due to matrix cracking and local delamination are, respectively: Ê ∂ PE ˆ Ë ∂ A mc ¯ {N } ,Ald
[9.7a]
Ê ∂ PE ˆ Ë ∂ A ld ¯ {N } ,Amc
[9.7b]
G mc = G ld = 
After some mathematical manipulation, it may be shown that, for specified stress resultants, the energy release rates for matrix cracking and local delamination are, respectively: ∂ Q2 Ê ˆ G mc (N , Dmc , D ld ) =  h2 N t A 1 A 1N Ë ¯ ∂ Dmc ∂ Q2 RT [9.8a] (e k + e RH + 2N t A 1 + ep) k ∂ Dmc ∂ Q2 RT t t t (e k + e kRH + e p ) + (e kRT + e kRH + e p ) ∂ Dmc h2 Ê t 1 ∂ Q2 1 ˆ NA A N ¯ 2 Ë ∂ D ld ∂ Q2 RT (e k + e RH + 2N t A 1 + ep) k ∂ D ld ∂ Q2 RT t t t (e k + e kRH + e p ) + (e kRT + e kRH e p ) ∂ D ld
G ld (N , Dmc , D ld ) = 
[9.8b]
The second and third terms on the righthand side of equation [9.8] are due to residual hygrothermal stresses and their interaction with damage. These expressions for the strain energy release rate are general and simple to use. Knowing the inplane stiffness matrix of the cracked lamina for a given matrix crack density, Cd, and relative local delamination area, Dld, the energy release rate is directly evaluated from equations [9.8a, b] by differentiating the reduced stiffness matrix with respect to the corresponding damage variable.The effect of interaction between matrix cracking and local delamination is explicitly included in the expression of the in situ damage __ effective function, Lij, which is used to obtain the reduced stiffness matrix, Q.
164
Analytical and numerical modelling
9.3
Twodimensional finite element analysis
9.3.1 Virtual crack closure approach In this section a 2D FE analysis of the threelayer laminate considered above is performed to obtain the interlaminar stresses and the strain energy release rate associated with a local delamination starting from the transverse ply cracks. This will assess the analytical model presented in the previous section and O’Brien’s simple equation for G.4 We assume the laminate to be subjected to a uniform axial tensile strain ey. Because of symmetry, only a quarter of the laminate, defined by 0 y s and 0 z h, is considered. Transverse ply crack density, Cd, determines the length of the quarter, s (s = 0.5Cd; half crack spacing), while the relative local delamination area, Dld, defines the interface crack length, ld (ld = s Dld). The FE package ABAQUS10 was employed to obtain the microstress field in the region of the crack tip. The quarter model is preliminarily divided into the 24 rectangles (4 ¥ 6) shown in Fig. 9.4(a). The rectangles are then subdivided into smaller regions using the eightnode quadrilateral plane strain element with 4Gauss points. The detailed mesh of the OO¢–AA¢ region is shown in Fig. 9.4(b). Five divisions are imposed in the interval AB. Multipoint constraints are used at the perfectly bonded section of the q/90° interface. Symmetry conditions are applied by imposing zero nodal displacement in the zdirection at z = 0 plane and in the ydirection at y = 0 plane. Load is applied by specifying uniform displacement in the ydirection at y = s plane.
9.3.2 Evaluation of strain energy release rate The energy release rate, Gld, in the finite element model is evaluated by using the VCC technique,11 as described in Section 6.9, and running the model twice. In the first run the model is loaded with nodes e, f and g, h held together (Fig. 9.5a) by employing the multipoint constraints (MPC) command in the ABAQUS package. The forces to hold these nodes together are evaluated. In the second run the model is loaded in the same manner but nodes e, f and g, h are allowed to move apart (Fig. 9.5b) and the relative displacements of the nodes recorded. If Fefy and F zef are the components of force in y and zdirections required to hold nodes e and f together in the first run, respectively, and d efy and d zef are the relative displacement components between nodes e and f in the second run, the mode I and mode II strain energy release rate can be evaluated as GIld =
1 z (Fefz d efz + Fghz d gh ) 2Dld
[9.9a]
Delamination
165
z O¢
t
ld
2t
s –3t –ld
B¢
A¢ Constraining layer (sublaminate)
t 0.9t t 0.9t Delamination tip
90°n ply group
O A
B
(a)
y
A¢
O¢
Delamination tip
O
A
(b)
9.4 FE meshes for crackedlayer laminate: (a) coarse mesh and, (b) refined mesh at crack tip.
GIIld =
1 (Fefy d efy + Fghy d ghy ) 2Dld
[9.9b]
with the total energy being taken as: G ldT = GldI + G IIld
[9.10]
In equation [9.9] Dld is the increment of delamination growth (virtual crack extension). Rybicki and Kanninen11 suggested that the value of the nodal forces in equations [9.9a, b] could be replaced by the corresponding components of
166
Analytical and numerical modelling
a
c d
b
g h
e f
Run 1
i j
k l
i j
k l
Delamination tip
Dld
z
(a)
y
a
y
z
Run 2
def b
z
def e
c
d
f
dgh g h y
dgh
(b)
9.5 Calculation of G using Virtual Crack Closure technique.
nodal force of nodes i and k (or nodes j and l) in run 2. In this case only the second run, Fig. 9.5(b), is required. In theory, the two values of the energy release rate, obtained from the two approaches, should tend to the same value for small virtual crack growth, Dld. It is suggested that any discrepancy between the two values could be used to check if the FE mesh is fine enough to provide a reliable and stable value of the strain energy release rate.
9.3.3 An example In order to compare the two virtual crack closure methods the nodal forces and the energy release rates are evaluated for a glass fibre/epoxy (02/904°)s laminate. The lamina stiffness properties are:12 E11 = 50.33 GPa, E22 = E33 = 14.48 GPa, G12 = G13 = G23 = 6.068 GPa, u12 = u13 = u23 = 0.275 and the ply thickness t = 0.254 mm. The transverse ply crack halfspacing, s, is assumed to be 10.16 mm (= 40 plythicknesses); this corresponds to a matrix crack density Cd = 0.492 cm1. The local delamination halflength is taken equal to Dld = 1.016 mm (= 4 plythicknesses), which is equivalent to relative delamination area Dld = 10%. Figures 9.6 and 9.7 illustrate the variation of the interlaminar normal stress, sz, and shear stress, syz, at the 0°/90° interface along the loading y
167
–200
Interface normal stress (MPa) –150 –100 –50 0
50
Delamination
0.0
Run 1 Run 2
0.5
1.0
1.5
2.0
2.5
Distance from local delamination tip (mm)
Interface shear stress (MPa) 200 300 400 500
600
9.6 Variation of direct stress at the 0/90° interface of a (02/90°4)s CFRP laminate.
0
100
Run 1 Run 2
0.0
0.5
1.0
1.5
2.0
2.5
Distance from local delamination tip (mm)
9.7 Variation of shear stress at the 0/90° interface of a (02/90°4)s CFRP laminate.
168
Analytical and numerical modelling
Table 9.1 Energy release rate evaluated using the Virtual Crack Closure technique FE models
GIld ey2 (106 J/m2)
GIIld ey2 (106 J/m2)
G Tld GT1d (106 J/m2)
Two runs
0.792
9.222
10.014
One run
0.799
9.195
9.994
Error between the
0.9%
0.3%
0.2%
two methods
axis. It can be seen that the variation of the interlaminar normal and shear stresses ahead of the delamination crack tip in the two configurations shown in Fig. 9.5 are in a good agreement, suggesting that with a fine mesh one run can successfully evaluate the energy release rate due to local delamination. Results for GT and its components are shown in Table 9.1; the maximum relative error between the two methods is only 0.9%. Going back to the stress results, Fig. 9.6 and 9.7 show a sharp increase in interfacial shear and normal stresses near the local delamination crack tip. The normal stress, sz, at the 0°/90° interface is compressive (Fig. 9.6), suggesting that opening mode delamination does not exist. In Fig. 9.8 the distribution of the interfacial normal stress, sz, ahead of the delamination tip is presented for four different local delamination areas. It can be seen that for delamination lengths greater than oneply thickness, sz is compressive, indicating that the shear mode (mode II) dominates delamination growth.
9.4
Discussion of VCC results
9.4.1 Comparison between the analytical models and FE method In this section, the analytical model described above is compared with the 2D finite element solution and O’Brien’s simple model;4 the energy release rate associated with local delamination is calculated for the T300/924 CFRP system with (±25/90°4)s layup. The FE analysis for local delamination is carried out for two different matrix crack densities; Cd = 0.947 cm1 and Cd = 4.38 cm1. The stiffness properties of the T300/924 system are taken as: E11 = 144.8 GPa, E22 = E33 = 11.38 GPa, G12 = G13 = 6.48 GPa, G23 = 3.45 GPa, u12 = u13 = 0.3 and ply thickness t = 0.132 mm.
169
–200
Interface normal stress (MPa) –150 –100 –50 0
50
Delamination
0.0
D ld=2.5% D ld=5% D ld=7.5% D ld=10%
0.1
0.2
0.3
0.4
0.5
0.6
0.7
0.8
0.9
Distance from local delamination tip (mm)
9.8 Variation of direct stress at the 0/90° interface of a (02/90°4)s CFRP laminate as a function of relative local delamination area, Dld.
In Fig. 9.9 the energy release rate normalised by the applied strain is plotted against the relative local delamination area, Dld, for the laminate with the two matrix crack densities. It can be seen that the strain energy release rate for delamination is reduced with increasing matrix crack density. The present analytical model agrees well with the FE solution in the steadystate growth of delamination. The predictions based on O’Brien’s simple equation, which ignores the effect of matrix crack density, are far away from the FE results.
9.4.2 Effect of thermal residual stresses on G In Fig. 9.10 the values of G with and without residual thermal stress effects are plotted against the relative delamination area. The applied axial strain is 1% and the matrix crack density Cd = 4.38 cm1. The thermal coefficients parallel and perpendicular to the fibres are: a1 = 0.36 ¥ 106 C1 and a2 = 28.8 ¥ 106 C1. The temperature difference between the stressfree state and ambient is assumed to be 125 °C and the specimen is assumed to be dry. It can be concluded that residual thermal stresses substantially increase the available energy to extend local delamination, and they should be included in predicting the local delamination onset strain (or stress).
1200 1000 800 600 400 200 0
Normalised energy release rate (¥104 J/m2)
2D FE method (mode II) Present analytical model O’Brien’s simple equation
0
2
4
6
8
10
12
Relative local delamination area, D ld (%)
s =8.46t s =20t s =40t
400
600
Including curing stress effect
200
Without curing stress effect
0
Energy release rate of local delamination (J/m2)
800
9.9 Variation of normalised energy release rate of local delamination with relative local delamination area, for the T300/914 graphite/epoxy (±25/90°4)s laminate (matrix crack spacing, 80t).
0
5
10
15
Relative local delamination area,
20 D ld
25
(%)
9.10 Variation of normalised energy release rate of local delamination with relative local delamination area, for the T300/914 graphite/ epoxy (±25/90°4)s laminate, with and without thermal stress (applied strain, 1%).
171
1.0
1.5
2.0
Predicted local delamination (Gcld=310J/m2) Experimental edge delamination Experimental transition point2 Experimental local delamination
0.0
0.5
Delamination onset strain (%)
2.5
3.0
Delamination
0
1
2
3 4 5 6 Number of the 90 plies (n)
7
8
9
9.11 Delamination initiation strain for T300/914 graphite/epoxy (±25/90°n)s laminates.
9.4.3 Local delamination initiation In order to evaluate the critical load for local delamination initiation, the interlaminar fracture toughness, Gcld, of the composite material was taken as 310 J/m2. For the (±25/90°n)s laminates tested by Crossman and Wang,2 the matrix crack density at which local delamination initiates can be inferred from the delamination onset strain and transverse ply crack density/strain data given in their paper. In Fig. 9.11 the dashed line gives the delamination onset strain as a function of the number of 90° plies in the laminate. In the experiments, the damage undergoes a transition from edge delamination (n 4) to local delamination (n 4). The prediction is in good agreement with experimental data for n 4. For n 4, the edge delamination is the dominant damage mode and has been analysed in Zhang et al.13
9.5
Finite element analysis using interface elements
The interface element described in Chapter 6 has been used to model several CFRP fracture mechanics test specimens.14 To undertake the analyses, the linear interface element was implemented in ABAQUS and the
172
Analytical and numerical modelling Experimental 140
Reaction force (N)
120 100
ABAQUS A
LUSAS Analytical linear part B
Analytical delamination part (A–C)
80 60 40 C 20 0 O0
5 10 15 Opening displacement (mm)
20
9.12 Load/displacement response for DCB. Point ‘B’ denotes the onset of delamination growth.14
quadratic element in LUSAS. The meshes used were such that there was roughly the same number of nodes in each case. The results indicated a faster convergence rate with the linear elements, although otherwise the two packages gave comparable results. The situations modelled were the basic pure mode I test, the double cantilever beam (DCB), the pure mode II test, the endloaded split (ELS), and the fixed ratio mixed mode (FRMM) test. The load–displacement response was computed and compared with experimental data, and with a closed form solution using modified beam theory.15 As can be seen from Fig. 9.12, the comparison is excellent for the DCB specimen. The results for the ELS specimen were also good, although there was some difficulty in getting, simultaneously, a close agreement for both the initial (linear) and ‘propagating’ parts of the load–displacement response. Similar, but not such pronounced, differences were encountered with the FRMM model. These issuse could be overcome by modifying the values of E11 input to the analysis, but such an approach is not satisfactory and indicates that more work is required in developing these elements.
9.6
Summary
The modelling of cracking in laminates has been illustrated with reference to laminates with (±qm/90°) n s layups. A new theoretical model and a 2D finite element analysis were used as a basis for comparison. The total GT
Delamination
173
was seen to consist primarily of the GII component, and the FE result using the VCC method was in good agreement with theoretical predictions for large delaminations. It was substantially affected by the matrix crack density and the residual thermal stresses. The recently developed interface element has been shown to offer considerable promise, despite much development being needed, especially for application in complex structures.
9.7
References
1 Jamison R D, Schulte K, Reifsnider K L & Stinchcomb W W, ‘Characterization and analysis of damage mechanisms in tensiontension fatigue of graphite/epoxy laminates’, ASTM STP836, Philadelphia, PA, American Society for Testing and Materials, 1984. 2 Crossman F W & Wang A S D, ‘The dependence of transverse cracking and delamination on ply thickness in graphite/epoxy laminates’, ASTM STP775, Philadelphia, PA, American Society for Testing and Materials, 1982. 3 O’Brien T K, ‘Characterization of delamination onset and growth in a composite laminate’, ASTM STP775, Philadelphia, PA, American Society for Testing and Materials, 1982. 4 O’Brien K T, ‘Analysis of local delaminations and their influence on composite laminate behaviour’, ASTM STP876, Philadelphia, PA, American Society for Testing and Materials, 1985. 5 Zhang J, Soutis C & Fan J, Strain energy release rate associated with local delamination in cracked composite laminates, Composites, 1994 25(9) 851–862. 6 Martin R H & Murri G B, ‘Characterization of Mode I and Mode II delamination growth and thresholds in graphite/PEEK composites’, ASTM STP1059, Philadelphia, PA, American Society for Testing and Materials, 1990. 7 Zhang J, Fan J & Soutis C, ‘Progressive matrix cracking in composite laminates loaded in tension’, Adv Composites Lett, 1992 1 (1) 12–15. 8 Zhang J, Fan J & Soutis C, ‘Analysis of multiple matrix cracking in [±qm/90n]s composite laminates: Part I, Inplane stiffness properties’, Composites, 1992 23(5) 291–297. 9 Zhang J, Fan J & Soutis C, ‘Analysis of multiple matrix cracking in [±qm/90n]s composite laminates: Part II, Development of transverse ply cracks’, Composites, 1992 23(5) 299–304. 10 ABAQUS User’s Manual, Hibbitt, Karlesson & Sorensen, Inc, Providence, RI, 1992. 11 Rybicki E F & Kanninen M F, ‘A finite element calculation of stress intensity factors by a modified crack closure integral’ Engineering Fracture Mechanics, 1977 9(4) 931–938. 12 Salpekar S A & O’Brien K T, ‘Combined effect of matrix cracking and free edge on delamination’, ASTM STP1110, Philadelphia, PA, American Society for Testing and Materials, 1991. 13 Zhang J, Soutis C & Fan J, ‘Effects of matrix cracking and hygrothermal stresses on the strain energy release rate for edge delamination in composite laminates’, Composites, 1994 25(1) 27–35.
174
Analytical and numerical modelling
14 Chen J, Crisfield M A, Kinloch A J, Matthews F L, Busso E & Qui Y ‘Predicting delamination of composite material specimens via interface elements’, J Mech Composite Mater Structures, 1999 6(1) 1–17. 15 Kinloch A J, Wang Y, Williams J G & Yayla P, ‘The mixedmode delamination of fibre composite materials’, Compos Sci Tech, 1993 47(3) 225–237.
10 Joining
10.1
Introduction
Joints in components or structures incur a weight penalty, are a source of failure and cause manufacturing problems; whenever possible, therefore, a designer will avoid using them. Unfortunately it is rarely possible to produce a construction without joints owing to limitations on material size, convenience in manufacture or transportation and the need for access in order to inspect or repair the structure.1 This chapter describes various fastening methods commonly employed with composite materials, the types of joint failure, and the kind of problems that arise in the joint design because of the heterogeneous and anisotropic nature of composite materials. Basically, there are two types of joint commonly employed with composite materials: adhesively bonded joints and mechanically fastened joints. Welding is also a possibility for thermoplastic composites, but this technique is not well developed for loadcarrying joints. In the following paragraphs, the first two types of joint are discussed.
10.2
Adhesively bonded joints
10.2.1 Introduction Bonded joints can be made by bonding (glueing) together precured laminates with a suitable adhesive or by forming joints during the manufacturing process, in which case the joint and the laminate are cured at the same time (cocured or cobonded). Loadcarrying joints often have an overlap configuration; see Fig. 10.1. Such joint forms would be appropriate for joining flat laminates or tubular members. Because the strength of a joint is sensitive to a large number of parameters it is vital that consideration is given to the joints at the outset of any design. Failure to do so may result in the component being otherwise of adequate performance but impossible to join. In the development of bonded joints for structures, a simple 175
176
Analytical and numerical modelling
(a) Single lap
(b) Double lap
(c) Scarf
(d) Bevel
(e) Step
(f) Butt strap
(g) Double butt strap
10.1 Some common engineering adhesive joints.1
joint can be fabricated first and tested for its suitability in structures. The size of the joint can be estimated from a knowledge of the part sizes to be joined, the allotted space for the joint, and a general idea of how much overlap is required to carry the load. With such knowledge, preliminary joint designs can be made that can be refined using an iterative analysis procedure.
10.2.2 Stress distributions A joint represents a discontinuity in a structure, and the resulting high stresses often initiate failure. Therefore, knowledge of the stresses in joints is vital if we are to understand the failures that occur in practice and hence improve designs and predict strength. Even relatively simple theories can be useful if they allow the important parameters to be identified. There are many publications concerned with the stress analysis of bonded joints,2–11 and analyses have been carried out for various joint configurations and for different properties of the adherends and adhesives. Results have been obtained in closed form or from numerical analyses. Important results are
Joining
177
20 15 10 5 0 50.8 mm 175 kN/m 1.27 mm
0.127 mm
10.2 Adhesive shear stress distribution in bonded joints.2
qualitatively described here, and the conclusions affecting the joint design are also discussed. The primary purpose of a joint is to transfer load between the two items being joined. In most bonded joints the load transfer takes place through interfacial shear, which gives rise to high interlaminar stresses in the adhesive layer. An idealised (elastic) variation of interlaminar shear stress in a double lap joint is shown in Fig. 10.2. It can be observed in the figure that the interlaminar shear stress has a large concentration near the end of the joint. In the remainder of the joint the stress is low and uniformly distributed. Because the load transfer zones occur at the ends and eventually reach a constant length, no increase in joint strength will be achieved once these zones are fully developed. There is no point in increasing the overlap beyond a critical value since no significant enhancement in strength will result. Typically, for carbon fibre/epoxy systems the limiting overlap is 30ta, where ta is the thickness of the adherend. Since high stresses are developed in the adhesive layer at the ends of the overlap, high stresses are produced in the adjacent plies of the adherends. Therefore, failure may initiate in these plies. HartSmith12 suggested that an effective way of reducing the local high stresses in the plies adjacent to the adhesive layer is to increase the adhesive thickness at the edge of the overlap. However, it is important to remember that good adhesive bonds can be produced only in small range of thicknesses (typically 0.1–0.25 mm) since thick bonds tend to be porous and weak while ultrathin bonds are too stiff and brittle. In contrast to double lap joints, the shear characteristics of the adhesive have little influence on the strength of single lap joints, which are determined mainly by adherend properties, peel stresses and overlap length. The
178
Analytical and numerical modelling
25
25
1.0
25
0.1
275
0.357 2.5
2.5
0.5 0.125 3.0
0.1
0.125
0.05
0.833
Adherend Adhesive Adherend
0.5 1.5
10.3 Typical single lap joint geometry and FE model (dimensions in mm).13
length of the plastic zone in the adhesive is only one half that in equivalent double lap joint and the elastic trough carries a significant proportion of the total load. Peel stresses are an order of magnitude greater than in a double lap joint and, in contrast to the latter situation, their effect can be minimised by increasing the lap length. For acceptable efficiency the overlap should be at least 80ta. A typical FE mesh for a single lap joint between eightply laminates is shown in Fig. 10.3. There is one element through the depth of each ply, and two through the thickness of the adhesive. Notice the increase in mesh
Joining
179
density at the ends of the overlap.13 Continuum and FE analyses of such joints give the same results for comparable situations.14 Scarf joints (Fig. 10.1) between identical adherends will have a uniform distribution of adhesive shear stress and hence will show a higher strength than the other joint types. With nonidentical adherends such stress uniformity is not obtained and the scarf joint will usually fail at the tip of the stiffer adherend. The same situation can occur with stepped joints. To restrict creep deformation the scarf angle must be kept small (1–3°), resulting in long joints. Stress analysis of both stepped and scarf joints between dissimilar adherends (e.g. composite and metal) must include the influence of the different adherend stiffnesses and thermal expansion coefficients.
10.2.3 Failure modes and strength Micromechanical damage occurs first and will eventually lead to macromechanical damage. Thus micromechanical damage can be the basis for the selection of ultimate load prediction techniques and the prediction of failure modes of the joints. The micromechanical damage may initiate in the adhesive layer, at the adhesive/adherend interface, or in the adherends. Adherend failure can be tensile, interlaminar or transverse, in the last two cases either in the resin or at the fibre/resin interface. Cohesive failure within the adhesive layer or in the surface layer of the adherend matrix may occur by brittle fracture or by a rubbery tearing, depending on the type of adhesive used. This results in cracking perpendicular to the load and causes a reduction in the load–transfer capability of the joint. This situation is analogous to the cracks in the 90° plies of a crossply laminate.Adhesive/adherend interface failure usually occurs on a macro scale at low loads when processing (surface treatment) or material quality are poor; it should not take place in properly prepared joints. Interlaminar failure in the laminate (not related to edge effects) may be caused by poor processing, voids, delaminations or thermal stresses. The weakest joints are those where failure is limited by interlaminar failure of the adherend or peel of the adhesive. The next strongest joints are those in which the load is limited by the shear strength of the adhesive, while the strongest will fail outside the joint area at a load equivalent to the strength of the adherend. Such failures can be related to the stress distributions described earlier.Further details on the different types of joint failure,joint analysis procedures and joint design allowables can be found in HartSmith.12
10.2.4 FE analysis of scarf joint In this section we consider a joint that has identical adherends, uses a relatively brittle adhesive and has small scarf angles, Fig. 10.4. The FE77
180
Analytical and numerical modelling
w P
P t
q tA
10.4 Scarf joint geometry.
10.5 Refined FE mesh near scarf tip.
finite element package15 is employed to determine the stress field in the scarf joint, using an isoparametric eightnode solid element. Because a high stress concentration is expected near the sharp tip, a fine mesh is required in this area; Fig. 10.5. The smallest element dimension is 0.012 5 mm.16 The (±45/0/90°)2s carbon fibre/epoxy laminate is treated as an homogeneous elastic material with the following stiffness/strength properties: Exx = Eyy = 53.8 GPa, Ezz = 11.3 GPa, Gxy = 20.5 GPa, Gxz = Gyz = 4.85 GPa, uxy = 0.31, uxz = uyz = 0.19 and compressive strength sun = 454 MPa. The epoxy adhesive layer of thickness tA = 0.129 mm has the following properties: E = 3.40 GPa, G = 1.26 GPa, u = 0.35 and ts = 40 MPa. 10.2.4.1 Stress results It is found that the dominant stress components are the inplane stress, sx, along the xaxis (load axis) in the parent laminate, and the shear stress tangential to the tapered bond surface. Other stress components are relatively small and could be neglected in any failure load calculations.The axial stress distribution has a steep gradient near the tip of the scarf, suggesting the existence of a stress singularity, and approaches the applied remote stress, Sg, within eight plies (1 mm); Fig. 10.6. Since a mathematical stress singularity exists at the scarf tip due to stiffness discontinuity, the computed stresses are taken near, but not at, the tip of the scarf. The elastic stress concentration factor, at a distance of 0.01 mm from the scarf tip, for the laminate examined, is approximately 2.3. As the distance from the tip increases, the inplane direct stress rapidly decreases. The shear stress in the adhesive is quite uniformly distributed; Fig. 10.7. Its magnitude is nearly proportional to the scarf angle; for q = 9°, it is almost three times higher than the value obtained for q = 3°.
Joining
181
sx /sg
dX=0.1h dX =0.2h dX =0.5h dX =h dX =2h
x/h
10.6 Distributions of sx/Sg in the parent plate along xaxis from the scarf tip; Sg is the remote stress.
t /Sg
3° 6° 9°
Tip x (mm)
10.7 Distributions of normalised shear stresses, t/Sg, in the adhesive layer along xaxis when the scarf angle equals 3, 6 and 9°.
10.2.4.2 Scarf joint strength and optimum scarf angle For the simple scarf joint case, a simple stress analysis16 predicts that the optimum scarf angle qopt for a maximum strength joint is a function of the adhesive shear strength ts and laminate strength sun, given by
Analytical and numerical modelling Strength of repaired laminates (MPa)
182
400 Adhesive failure 300 Adherend failure 200
100
0 0
1
2
3
4 5 6 7 Scarf angel (degree)
8
9
10
10.8 Failure stress variation with scarf angle based on maximum stress criterion.
qopt @ tan 1
Ê ts ˆ Ë s un ¯
[10.1]
For small q the failure stress, Sgf, of the scarf joint is determined by the maximum stress failure criterion, and is given by Sgf =
s un ts = K L K A sin q
[10.2]
where KA and KL are the stress concentration factors (SCFs) in the adhesive and adherend, respectively. From the FE analysis, KA @ 2.88 and KL @ 2.3 for q 10°. The loadcarrying capability of the adhesive and the adherend is plotted in Fig. 10.8 as a function of scarf angle. The optimum scarf angle occurs when the adhesive failure load is equal to the laminate failure load. For the composite system examined (ts = 40 MPa and sun = 454 MPa), equation [10.2] results in a failure stress of @ 200 MPa and an optimum scarf angle qopt of 4°. Since stress redistribution, owing to material nonlinearities and resin plasticity, may occur in the scarf region before final failure, using elastic SCFs could substantially underestimate the failure load. An alternative approach is that of averaging the stresses over a distance from the tip of the scarf, suggesting that the exact values of the stresses at the tip are not too important, see Section 8.4.4. This approach accounts for material nonlinearities and plasticity of the adhesive, which reduce local peak stresses in the scarf region, and stress redistribution mechanisms, which are not considered in the elastic FE analysis.
Joining
10.3
183
Mechanically fastened joints
10.3.1 Introduction In structures where parts are removed for inspection or maintenance bolted joints will be required. The behaviour of bolted connections, for composite laminates made from unidirectional prepreg material, has been extensively examined by several workers,17–29 who investigated a wide range of variables such as layup, fastener type (screw, rivet, bolt), friction effects, clearance and their influence on the failure mode. A full theoretical description of the stresses in such a joint must include their threedimensional nature, a fact that has limited the analytical treatment given to such connections. The prediction of failure loads is, at the moment, mostly done semiempirically. Improvement will depend on the development of failure criteria that are more generally applicable, together with an easytouse 3D stress analysis. In the latter context, FE analysis is clearly important, and some recent work is discussed below.
10.3.2 Failure modes In addition to fastener failure, in shear and/or bending, there are essentially four modes of failure, namely tension, shear, bearing and cleavage, as illustrated in Fig. 10.9. Failure will be dependent upon many factors, such as fibre type, fibre orientation, surface treatment and matrix properties. It follows that knowledge of a wide range of variables is needed if favourable joint conditions are to be achieved and unwanted failure modes avoided. Composite materials may have low bearing strength and low inplane shear strength. The tensile strength of the material in the reduced crosssection can be improved by increasing the spacing between bolts and transferring the load through several rows of bolts so that the net shear area of the bolts is sufficient.
Tension
Shear
Bearing
Cleavage
10.9 Modes of failure for mechanical joints in FRP composites.
184
Analytical and numerical modelling
The low inplane shear strength of the composite presents quite a few problems. Unidirectional composites have low shear strength in the longitudinal direction, which results in the shear out mode of joint failure. An improvement for this mode of failure can be made by the use of ±45° fibre orientations, but this can result in low net tension capability.The use of quasiisotropic fibre orientations combines improved shear and tensile strength, but at the same time reduces considerably the efficiency of the joint. Besides the preceding problems related to conventional strength criteria, there are problems peculiar to composite materials. The holes in the laminate cause stress concentrations that vary with the fibre orientation relative to the load direction. The stress concentration factors may sometimes be well above those occurring in a similar metal structure. Composite materials do not plastically deform, so that stresses are not easily redistributed around the stress concentration and are thus a cause of concern. The holes also give rise to the edge effects, as discussed in Chapter 7, which promote local interlaminar failures that may become critical in the presence of a corrosive environment. A detailed discussion of current joint design practices can be found in other works.29,30
10.3.3 Bearing strength prediction There are three significant inplane stresses in the laminate: the compressive (bearing) stress on the loaded side of the pin, the tensile stress across the net section and the shear stress on the shear out planes; Fig. 10.10.
y r x
(a)
(b)
(c)
10.10 Typical inplane stress distributions around a pinloaded hole: (a) radial compression stress, sr; (b) tensile stress on net section, sy; and (c) shear stress on shear out planes, sxy.
Joining
185
Table 10.1 Measured and predicted bearing strengths of woven CFRP laminates Laminate
Failure load, Pf (kN) sb
Strengths (MPa) sth, Eqn [10.4]
sth18
(0/90°)8s
12.6
553
315 (567)
620
(0/90/± 45°)4s
16.5
723
363 (653)
402
Note: number in parentheses are strengths obtained by reducing the SCF.29
Provided certain geometric requirements are met joint failure will be in bearing. Smith24 and Smith et al.26 related the maximum tensile stress concentration factor (SCF) at a loaded hole, Kb, to the maximum stress concentration factor at an unloaded hole in a finite width orthotropic laminate under a remote tensile stress by the following expression: K b = KT• [0.31 + 0.5Y (d w)]
[10.3]
Kb is defined as the maximum tensile stress normalised by the nominal bearing stress, Y is a finite width correction factor, d is the hole diameter and w is the plate width. K•T is related to the laminate elastic constants (E, u, G) and is given by Lekhnitskii.31 For the woven carbon fibre (T300 2 ¥ 2 twill)/epoxy (135 °C curing toughened epoxy, LTM49) (0/90°)8s orthotropic and (0/90/±45°)4s quasiisotropic laminates investigated by Andreasson et al.,32 Kb is equal to 2.063 and 1.188, respectively. These values could be used with the maximum stress criterion to predict the bearing strength (in the net tension mode of failure); i.e. s th =
s ult Kb
[10.4]
where sult is the ultimate tensile strength of the laminate. Equation [10.4] predicts that failure would occur at 315 MPa for the (0/90°) layup and at 363 MPa for the (0/90/±45°) laminate; Table 10.1. Both values are much lower than the measured strengths, sb. This suggests that some load redistribution is occurring and a simple stress concentration factor underestimates considerably the notched strength. A simple means of incorporating the load redistribution is to apply the point stress or average stress failure criterion,33 or just reduce the elastic SCF by a constant C (@1.8; determined from the best fit to experimental data) as suggested by HartSmith.29
186
Analytical and numerical modelling
Note that the parameter C for the nonwoven laminates (XAS/914 carbon fibre/epoxy system) examined by Smith24 and Smith et al.26 was taken as 2.1, independent of stacking sequence and thickness. In order to predict the bearing strength, in the bearing mode of failure, the semiempirical technique developed by Collings18 could be used. The method underestimates the bearing strength of the quasiisotropic laminate by more than 40%, but in general the agreement is acceptable considering the complex nature of damage initiation and growth observed in the experiments.32 It would be more appropriate to use Collings’ expressions to estimate damage initiation rather than final fracture. The average or point stress criterion could be applied to account for the local damage occurring around the hole, but knowledge of the stress distribution is required. This can be achieved by performing a 2D FE stress analysis.
10.3.4 2D FE analysis The stress field in the region of a loaded hole in a composite laminate is quite complicated, even if the problem is treated as being twodimensional (load transfer friction and throughthickness clamping effects ignored). The stress distributions are influenced by the elastic constants of the laminate, the joint width and end distance, pin elasticity, friction and clearance between the pin and the hole. Andreasson et al.32 used the commercial FE package IDEAS to model a pin joint (i.e. a bolt with no throughthickness restraint or tightening) as a 2D contact problem which incorporated the bolt/hole friction and an appropriate contact region between the bolt and the plate. Orthotropic (0/90°)8s and quasiisotropic (0/90/±45°)4s laminates were examined. For linear static problems IDEAS makes use of laminate plate theory to determine ply and laminate stresses. A typical FE mesh is shown in Fig. 10.11(a). The optimised mesh consisted of about 760 quadratic thin shell elements (Mindlin shell element) and 55 contact elements with 2393 nodes in total. The mesh is much finer in the region close to the hole since large stress variations are expected; Fig. 10.11(b). The model, when run on a Sun Superstation 5 with 64 Mb main memory, takes just over 5 minutes CPU time. In order to simulate the no contact region behind the bolt, a gap is left between 101° and 101°. For the rest of the interface special gap elements are employed which prevent penetration of the bolt elements into the plate elements, and allow the contact region between the bolt and plate to be modelled with friction. The load is applied at the centre of the bolt as a point load (linearly increasing from zero to 12 kN in 2 kN increments) along the xaxis. The radial degree of freedom of the boundary nodes in the bolt, between 90° and 270°, is fixed to avoid any rigid body movement.
Joining
187
10.11 Plate with a pinloaded hole: (a) overall mesh and (b) refined mesh around hole.
The FE load/strain curves corresponding to the net tension and bearing planes for the orthotropic and quasiisotropic laminates are plotted in Fig. 10.12, and compared with experimental values obtained from strain gauges attached near the hole on a representative test specimen. Differences are due to the fact that the strain gauges measure an average value rather than a point value, and the FE analysis is 2D elastic, ignoring throughthickness effects. For the (0/90°) orthotropic plate the maximum stress criterion predicts damage initiation at approximately 12 kN applied load, owing to high shear stress developed at q = 45° from the direct contact point between the bolt and the plate. No damage is observed in the bearing plane; the compres
188
Analytical and numerical modelling 14 12 10 Load 8 (kN) 6 4 2 0
14 12 10 Load 8 (kN) 6 4 2 0 0
0.1 ex (%)
0
0.2
0.1
0.2
0.3
ey (%) Numerical (FE) Experimental
(a) 12
12 10 Load 8 (kN) 6 4 2 0
10 8 Load (kN) 6 4 2 0 0
0.05
0.1
0.15
0
ex (%)
(b)
0.05 ey (%)
0.1
Numerical (FE) Experimental
10.12 Load–strain curves corresponding to strain on the nettension plane (left) and bearing plane (right): (a) the orthotropic laminate and (b) quasiisotropic laminate.32
sive stress at the edge of the hole is below the critical compressive strength value of 520 MPa. In the (0/90/±45°) laminate failure initiates first in the offaxis plies (±45° layers) at 45° from the direct contact point, owing to high shear, while the (0/90°) plies fail both in nettension and bearing mode. A 12 kN applied load introduces stresses at the edges of the hole which exceed the ultimate tensile (650 MPa) and compressive strength (520 MPa) of the system, and therefore damage (nettension and bearing) is expected to occur in these layers. The measured failure load for this layup is 16.5 kN, suggesting that the damage reduces the local stresses (load redistribution) and therefore delays final failure. The point stress failure criterion (PSFC) predicts nettension failure in the quasiisotropic laminate successfully. With the characteristic length d0 from the hole edge taken equal to 1 mm, the predicted failure load is 16 kN compared with 16.5 kN for the measured value. For the orthotropic layup the theoretical failure load is 12 kN, which is very
Joining
189
close to that observed (13 kN). However, final failure occurred in the bearing plane. With the PSFC, the linear elastic stress analysis is presumed to be valid outside some empirically determined softened zone adjacent to the hole. The basic drawback is that the socalled characteristic length varies considerably with bearing stress, and failure is predicted at some place other than where it is known to occur. The value chosen for d0, although not determined analytically, correlates quite well with the value used for the strength of carbon fibre/epoxy laminates with an open hole.
10.3.5 3D FE analysis As already mentioned, there are many factors that influence the performance of mechanical joints, and their complete representation, in any model, requires a 3D analysis. Necessarily, this will mean an FE model. In this section a particular approach is presented.34 10.3.5.1 Model formulation Stacked, eightnode, reduced integration, brick elements were chosen as they are adequate to capture the 3D stresses around the hole boundary. The ABAQUS system35 was used for the analysis, with IDEAS36 used as a preprocessor. The choice of element was also related to the contact algorithm used in ABAQUS. The mesh around the hole boundary is shown in Fig. 10.13; there is one element per ply thickness. Special care was taken to avoid element distortions due to aspect ratio and skew angular deformations. Nevertheless, the use of one element per ply will give high aspect ratios away from the fine mesh region, where accurate stresses are not so important. Because of symmetry, only one quarter of the laminate was modelled.
10.13 Typical 3D finite element mesh for a FRP laminate with a pinloaded hole.34
190
Analytical and numerical modelling
The FE results were compared with experimental data obtained from single fastener specimens, with fingertight washers, loaded in double shear. The washer was assumed to be rigid, and constraints imposed at the corresponding nodes in the model to prevent throughthickness expansion. 10.3.5.2 Representation of damage Extensive experimental characterisation was carried out to identify the failure modes that occurred as the fastener load was increased from zero to final failure.34 Matrix cracking in tension, compression and shear, fibre failure in tension and compression, and delamination were all seen. From this work it was concluded that a 3D failure criterion would be needed, together with a procedure for reducing the elastic properties in damaged elements. The latter was based on the approach of Tan and coworker,37,38 and the criterion of Hashin39 was used to indicate the onset and type of damage within a ply. The initiation of delamination was modelled, but not its growth. Besides predicting the onset of noncritical damage, a procedure was also needed to indicate final failure. For the tension and shear out modes, total failure of the joint was taken to be when predicted fibre damage extended to the free edge of the laminate. For the bearing mode failure was when fibre damage reached the outer edge of the washer. These representations were in accord with experimental observations. 10.3.5.3 Comparison of predictions with experiment To illustrate the success of the approach, the predicted and experimental load–displacement (from a linear voltage displacement transducer, LVDT) curves are shown in Fig. 10.14 for the bearing failure specmen. Comparisons for tension and shear out modes were equally good. There is significantly more extension from the experimental results simply because the tests were continued long after effective failure had occurred.
10.4
Summary
In this chapter, fastening methods commonly employed with composite materials, the types of joint failure and the kinds of problems that arise in the joint design because of the heterogeneous and anisotropic nature of composite materials have been discussed. Adhesive bonded joints and mechanically fastened joints are the two types of joint mainly used with these materials. In the development of bonded joints for structures, a simple joint can be fabricated first and tested for its suitability in structures. The size of the joint
Joining
191
Load (N) 8000 7000 6000 5000 4000 3000
Experimental (LVDT)
2000
3D FE model
1000 0 0
0.25
0.5
0.75
1
Bolt displacement (mm)
10.14 Experimental and predicted load–displacement relation for the bearing failure specimen.34
can be first estimated from a knowledge of the part sizes to be joined, the allotted space for the joint, and a general idea of how much overlap is required to carry the load. With such knowledge, preliminary joint designs can be made that can be refined using an iterative analysis procedure. The FE method is a powerful numerical tool that can be used to estimate direct and shear stress distributions required in the failure analysis. In structures where parts are removed for inspection or maintenance bolted joints are required. A wide range of variables such as layup, fastener type (screw, rivet, bolt), friction effects, clearance and their influence on the failure mode of a bolted (or riveted) connection need to be carefully examined for a successful design. The stress analysis in such a joint must include their 3D nature, a fact that has limited the analytical treatment given to such connections. The prediction of failure loads is, for the moment at least, generally semiempirical. However, it has been shown that the use of appropriate failure criteria that are more generally applicable, in combination with stiffness reduction laws, together with an easytouse 3D FE stress analysis can result in improved strength predictions.
10.5
References
1 Matthews F L & Rawlings R D, Composite Materials: Engineering and Science, Cambridge, Woodhead, 1999. 2 Goland M & Reissner E, ‘The Stresses in Cemented Joints’, J Appl Mech, 1944 A17–A27. 3 Berg K R, ‘Problems in the Design of Joints and Attachments,’ in Wendt F W, Liebowitz H and Perrone N, Eds., Mechanics of Composite Materials, New York, Pergamon, 1970.
192
Analytical and numerical modelling
4 Haddock R N, ‘Joints in Composite Structures’, Proceedings of Conference on Fibrous Composites Vehicle Design, AFFDLTR7213, 1972. 5 HartSmith L J, ‘Design & Analysis of Adhesive Bonded Joints’, Proceedings of Conference on Fibrous Composites Vehicle Design, AFFDLTR7213, 1972. 6 Fehrle A C, ‘Fatigue Phenomena of Joints in Advanced Composites’, Proceedings of Conference on Fibrous Composites Vehicle Design, AFFDLTR7213, 1972. 7 Grimes G G & Greimann L F, ‘Analysis of Discontinuities, Edge Effects, and Joints’, in C C Chamis, Ed., Structural Design and Analysis Part II, New York, Academic Press, 1975. 8 Ishai O & Gali S, ‘Twodimensional interlaminar stress distribution within the adhesive layer of a symmetrical doubler model’, J Adhes, 1977 8(4) 301– 312. 9 Ishai O, Peretz D & Gali S,‘Direct determination of interlaminar stresses in polymeric adhesive layer’, Exp Mech, 1977 17(7) 265–270. 10 Amijima S, Fujii T & Yoshida A, ‘TwoDimensional Stress Analysis on Adhesive Bonded Joints’, Proceedings of Twentieth Japan Congress on Materials Research, The Society of Materials Science, Japan, 1977. 11 Amijima S, Fujii T, Yoshida A & Amino H, ‘Dynamic Response of Adhesive Bonded Joints’, Proceedings of Twentieth Japan Congress on Materials Research, The Society of Materials Science, Japan, 1977. 12 HartSmith L J, Further developments in the design of adhesivebonded structural joints. Douglas Paper 6922, Douglas Aircraft Corp., Long Beach, CA,April, 1980. 13 Kairouz K C & Matthews F L, ‘A finite element analysis of the effect of stacking sequence on the failure mode of bonded composite single lap joints’, Proc CADCOMP2, Brussels, Springer Verlag, 1990. 14 Matthews F L, Kilty P F & Godwin E W, ‘A review of the strength of joints in fibrereinforced plastics, Part 2: Adhesively bonded joints’, Composites, 1982 13(1) 29–37. 15 Hitchings D, FE77 Users’ Manual, Dept of Aeronautics, Imperial College, London, 1995. 16 Soutis C & Hu FZ, ‘A 3D failure analysis of scarf patch repaired CFRP plates’, 39th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference, Long Beach, CA, Paper No. AIAA981943, 3 1971–1977, 20–23 April, 1998. 17 Collings T A,‘The strength of bolted joints in multidirectional CFRP laminates’, Composites, 1977 8(1) 43–54. 18 Collings T A, ‘On the bearing strengths of CFRP laminates’, Composites, 1982 13(3) 241–252. 19 Wong C M S & Matthews F L, ‘A finite element analysis of single and twohole bolted joints in fibre reinforced plastic’, J Compos Mater, 1981 15(9) 481–491. 20 Matthews F L, Wong C M S & Chryssafitis C, ‘Stress distribution around a single bolt in fibrereinforced plastic’, Composites, 1982 13(3) 316–22. 21 Kretsis G & Matthews F L, ‘The strength of bolted joints in glass fibre/epoxy laminates’, Composites, 1985 16(2) 92–102. 22 Agarwal B L, ‘Static strength prediction of bolted joints in composite materials’, AIAA J, 1980 18(11) 1371–1375. 23 Zhang K & Ueng C E S,‘Stresses around a pinloaded hole in orthotropic plates’, J Compos Mater, 1984 18(9) 119–143.
Joining
193
24 Smith P A, Aspects of the Static and Fatigue Behaviour of Composite Laminates, Including Bolted Joints, PhD Thesis, Cambridge University Engineering Department, 1985. 25 Eriksson I, ‘Contact stresses in bolted joints of composite laminates’, Composite Structures, 1986 6(1–3) 57–75. 26 Smith P A, Pascoe K J, Polak C & Stround D O, ‘The behaviour of singlelap bolted joints in CFRP laminates’, Composite Structures, 1986 6(1–3) 41–55. 27 Hyer M W, Klang E C & Cooper D E, ‘Effects of pin elasticity, clearance and friction on the stresses in a pinloaded orthotropic plate’, J Compos Mater, 1987 21(3) 190–206. 28 Chen W H, Lee S S & Yeh J T, ‘Threedimensional contact stress analysis of a composite plate with a bolted joint’, Composite Structures, 1995 30(3) 287–297. 29 HartSmith L J, ‘Mechanicallyfastened joints for advanced compositesphenomenological considerations and simple analyses’, Proc. 4th Conf. on Fibrous Composites in Structural Design, San Diego, USA, 1978. 30 Camanho P P & Matthews F L, ‘Stress analysis and strength prediction of mechanically fastened joints in FRP: A review’, Composites Part A, 1997 28A(6) 529–547. 31 Lekhnitskii S G, Theory of Elasticity of an Anisotropic Elastic Body, San Fransisco, HoldenDay Inc., 1963. 32 Andreasson N, Mackinlay P & Soutis C, ‘Tensile strength of bolted joints in woven CFRP laminates’, The Royal Aeronautical J, 1998 102(1018) 445–450. 33 Whitney J M & Nuismer R J, ‘Stress fracture criteria for laminated composites containing stress concentrations’, J Compos Mater, 1974 8(7) 253–265. 34 Camanho P P, Application of Numerical Methods to the Strength Prediction of Mechanically Fastened Joints in Composite Laminates, PhD Thesis, Centre for Comp Matls, Imperial College, London University, 1999. 35 ABAQUS 5.6 Users’ Manual, Hibbitt, Karlsson & Sorensen Inc, Pawtucket, USA. 36 IDEAS Master Series Release 2 Users’ Manual, Structural Dynamics Research Corporation, Milford, Ohio. 37 Nuismer R J & Tan S C, ‘Constitutive relations of a cracked composite lamina’, J Compos Mater, 1988 22(4) 306–321. 38 Tan S C & Nuismer R J, ‘A theory for progressive matrix cracking in composite laminates’ J Compos Mater, 1989 23(10) 1029–1047. 39 Hashin Z, ‘Failure criteria for unidirectional fiber composites’, J Appl Mech, 1980 47(2) 329–334.
11 Fatigue
11.1
Introduction
Fatigue in metals occurs by the initiation of a single crack and its intermittent propagation until catastrophic failure occurs with little warning and no sign of gross distortion, even in highly ductile metals, except at the final tensile region of fracture. In contrast to homogeneous materials, composites accumulate damage in a general rather than a localised fashion, and fracture does not always occur by propagation of a single macroscopic crack. The microstructural mechanisms of damage accumulation, including fibre/matrix debonding, matrix cracking, delamination and fibre fracture, occur sometimes independently and sometimes interactively, and the predominance of one or other of them may be strongly affected by both materials’ variables and testing conditions.1,2 Fatigue damage in composites leads to permanent degradation in mechanical properties, notably laminate stiffness and residual strength, often at an early stage in the fatigue life. In this chapter, we describe the fatigue damage accumulation in unidirectional and multidirectional fibrereinforced polymer laminates, and discuss some of the methods which have been used to model composite fatigue behaviour. A more elaborate discussion on the subject can be found in references 1–7.
11.2
Damage modes in composite laminates
In multidirectional laminates, the 0° plies carry most of the load and provide most of the stiffness while the 90° and +45° plies give transverse and shear strength and stiffness, respectively. Under an applied load (mechanical, thermal, static or cyclic) a complicated state of damage develops in the offaxis plies, causing load redistributions which lead to eventual fracture of the loadbearing plies. Damage in (0/90°) crossply and (0/90/±45°) quasiisotropic laminates is of three main types: matrix cracking parallel to the fibres in the longitudi194
Fatigue
195
nal and offaxis plies, delamination between plies and fibre fracture with associated debonding. The general sequence of damage is similar under tensile static and fatigue loading. Fibre/matrix debonds initiate around fibres lying at an angle to the loading direction, initially in the 90° plies, extend to form microcracks which, in turn, form matrix cracks across the thickness and the width of the plies. The number of cracks in all of the offaxis plies increases with increasing static stress or number of fatigue cycles, reaching a maximum density which remains stable until fracture. This has been termed the ‘characteristic damage state’ (CDS) and depends on ply thickness and orientation and on laminate stacking sequence.8 Matrix cracking parallel to the fibres in the 0° plies occurs at strains close to failure under static loading or may develop throughout fatigue cycling (owing to the mismatch between Poisson’s ratios of adjacent plies).9,10 Delaminations initiate between plies of different orientation and grow inwards from the laminate edges across the width of a test coupon. The tendency to delaminate results from outofplane interlaminar shear and normal stresses which exist at free edges and depends on the stacking sequence of the offaxis plies within the laminate,9 as described in Chapter 7. Final failure of the laminate is due to tensile fracture of the 0° fibres. The variation in fibre strength is related to the statistical distribution of flaws along the fibre length. Progressive fibre failure and debonding of the broken fibres (due to the high shear stresses at the fibre/matrix interface close to the break) causes a redistribution of the applied load, increasing the probability of fracture in neighbouring fibres and reaching a critical number of fibre failures to cause fracture. A higher concentration of fibre breaks has been observed at the intersection of transverse ply cracks with the longitudinal plies under cyclic loading.11 In compression, although the fibres remain the principal loadbearing elements, they must be supported from becoming locally unstable and undergoing a microbuckling type of failure.4,12 This is the task of the matrix and the fibre/matrix interface, the integrity of both being of greater importance in compressive loading than in tensile loading. Matrix and interfacial damage develop for much the same reasons as for tensile loading, but because of the greater demand on the matrix and the interface in compressive loading, compressive fatigue loading generally has a greater effect on the residual strength of composite materials than does tensile loading. In addition, local resin and interfacial damage leads to fibre instability in compressive loading which is more severe than the fibre isolation mode which occurs in tensile loading. Generally, fewer studies are available on the compressive fatigue of composites, mainly because compression testing of these materials presents many problems, not the least of which is the need to support the specimen from undergoing global macrobuckling, com
196
Analytical and numerical modelling
2.0
Peak stress, MPa
1.6
1.2
0.8
Carbon fibre/epoxy Glass fibre/epoxy Aramid fibre/epoxy
0.4
–1
0
1
2
3
4
5
6
7
Log cycles to failure
11.1 SN fatigue data for unidirectional composite materials.4
bined with limitations imposed on specimen geometry by the anisotropic nature of the materials.4
11.3
Fatigue of unidirectional laminates
11.3.1 Fatigue lifetime Typical plots of peak tensile stress versus log cycles to failure, the traditional stresscycles (S–N) presentation of data, are shown in Fig. 11.1.4 Data for three unidirectional materials are presented: carbon fibre, glass fibre and aramid fibrereinforced epoxy resin. The slope and shape of the S–N curve is a measure of the fatigue resistance of the material. Since, for unidirectional composite materials under tensile loading, the fibres carry virtually all the load, the tensile fatigue behaviour might be expected to depend solely on the fibres, and since the fibres themselves are not usually particularly sensitive to fatigue loading, good fatigue behaviour should result. However, experimental evidence has shown that the slopes of the curves are determined principally by the strain in the matrix13,14 when the fatigue limit of the matrix is less than that of the fibres, which is nearly always the case. Consequently, plots of mean strain rather than stress vs log cycles to failure are frequently more meaningful for composite materials. The resulting e–N diagram, Fig. 11.2, would show regions of dominance of
Fatigue
Matrix fatigue strain limit
Fibre breakage and interface debonding Maximum strain
Composite static failure strain
197
ec
Progressive matrix cracking and interface damage Matrix microcrack initiation only
em Log (fatigue life)
11.2 A generalised strain–fatigue life diagram for unidirectional composites loaded parallel to the fibres showing dominant regions of tensile fatigue damage.14
individual damage mechanisms in the fibre, matrix and interface from which the contribution of each to the overall fatigue response can be evaluated.14 In unidirectional fibre/epoxy laminates, fatigue failures tend to occur only within a narrow band of stress close to the static strength of the laminate, and the number of cycles to failure can vary over several decades of cycles inside this band. Load is carried mainly by the stiff fibres and there is little permanent damage until fibre fracture is initiated. Fatigue damage may accumulate as a result of stress redistribution from broken fibres but this is only significant at stresses close to the static ultimate strength. Comparison of the S–N curves shown in Fig. 11.1 illustrates that fatigue performance is ranked in the order of modulus and strain to failure of the fibres. The use of very stiff fibres, such as carbon fibres (typically with modulus of 220–700 GPa and failure strains of 0.6–2%), limits the strain in the composite and so prevents large elastic and viscoelastic deformations in the matrix which lead to initiation of damage. The lower modulus of glass fibres (70–80 GPa) permits composite strains large enough to cause early matrix damage and hence precipitate fatigue failure. Consequently, the S–N curve falls more steeply than for CFRP. The fatigue performance of Kevlar fibre composites is intermediate to CFRP and GFRP. However, the fatigue damage mechanism is complicated in this material since aramid fibres are themselves fatigue sensitive and can defibrillate during fatigue loading. The lowcycle behaviour compares well with GFRP but deteriorates at intermediate to long lifetimes.
11.3.2 Fatigue damage accumulation Some of the weakest fibres fail in the first few cycles since the cyclic stress falls within the statistical fibre strength distribution determined by flaws.15 This gives rise to locally enhanced stresses in the matrix and at the
198
Analytical and numerical modelling
100
Normalised peak stress
80
60 100% 0° fibres 50% 0° fibres 25% 0° fibres 0% 0° fibres (all 45° )
40
20
–1
0
1
2
3
4
5
6
7
Log cycles to failure
11.3 Normalised S–N curves for (0/±45°) CFRP laminates with varying percentage of 0° fibres.4
fibre/matrix interface, which lead to the development of fatigue damage with increasing number of cycles. Damage may also develop at local microdefects, such as misaligned fibres, resinrich regions or voids.4 Resin cracks frequently develop between the fibres, isolating them from adjacent material and rendering them ineffective load carriers, causing fibres to become locally overloaded and further fibre failures to occur. Close to failure, the matrix may show extensive longitudinal splitting parallel to fibres caused by resin and interfacial damage, leading to the brushlike failure characteristic of most unidirectional materials.4 The rate of this degradation process in the matrix and at the interface is a function of the bulk strain in the resin as well as the nature of the matrix.
11.4
Fatigue of multidirectional laminates
11.4.1 Fatigue lifetime On increasing the percentage of nonaxial plies in a laminate, the static tensile strength and stiffness are reduced since fewer fibres are available to support the mean applied loads.The slope of the tensile S–N curve increases in relation to the static strength, Fig. 11.3, as the layers with offaxis fibres,
Fatigue
199
whose mechanical properties are resindependent, are more easily damaged in fatigue.4 Both CFRP and GFRP multidirectional laminates undergo progressive accumulation of fatigue damage at rates that are reflected in the slope of the S–N curves, as explained in Section 11.2. The damage will lead to a general loss of integrity with potential for environmental attack, and certainly to a reduction in compressive strength.15,16 Ultimate tensile fatigue failure of composite laminates is usually determined by the 0° layers; thus the tensile S–N curves for multidirectional laminated composite materials are still relatively shallow, although steeper than for 100% unidirectional material. In general, the poorer fatigue performance observed in unidirectional materials through the use of tough matrices is less marked in multidirectional laminates.
11.4.2 Progressive damage in multiply laminates The general sequence of damage events in a multidirectional laminate under fatigue loading is similar to that observed under static loading, as explained above. At high fatigue stresses, cracks can initiate on the first loading cycle and then accumulate with increasing number of cycles. However, cracks can develop even when the maximum cyclic stress is well below the static cracking threshold, although only after an ‘incubation period’ of hundreds of thousands of cycles (depending on peak stress); Fig. 11.4.17 Cracks generally initiate at the free edge of the specimen but can also initiate away from the edge. Transverse ply cracks are observed to grow stably across the width of the ply under fatigue loading at a rate which depends on the cyclic stress level and on interaction with neighbouring cracks. The early initiation of matrix cracking in fatigue relative to static loading consequently leads to a decrease in the threshold for the onset of other types of damage. Delaminations can propagate over many thousands of cycles, resulting in separation of the laminate into discrete laminae (which will continue to support tensile load via the 0° plies). Analysis of the stresses at the intersection of matrix cracks in adjacent plies of different orientation18 shows that there is a highly localised region of increased interlaminar normal and shear stress around the point of intersection, which could be an initiation point for failure of the laminate. The final stage of damage development is dominated by fibre failures that result from these locally enhanced stresses.19,20 Ultimately fracture occurs when the locally failed regions have sufficiently weakened the laminate to cause failure at the maximum applied load. The progression of damage in woven fabric composites in the initial stage of tension–tension fatigue shows basically the same features that are
200
Analytical and numerical modelling 1.2 Carbon/epoxy 0.68% strain 1.0
Transverse ply crack density (mm–1)
Maximum static crack density 0.8 0.6% strain
0.6 0.5%
0.4
0.4% 0.2 0.25% 0 1
2
3 4 5 Log (number of cycles)
6
7
11.4 Variation of transverse ply crack density with cycles for CFRP (0/90°3)s specimens, fatigued at maximum stresses between 105 and 285 MPa (static cracking threshold, 0.45%).17
observed in crossply laminates,21 i.e. cracks initiate in the weft (transverse) direction along the fibres. Further on in the lifetime, longitudinal cracks appear between warp fibres in the undulation region where the fibres cross over. Crack densities increase with cycling and a uniform pattern of orthogonal cracks develops. After further cycling, delaminations occur confined to the undulation regions and, thereby, attain a uniform distribution in the interlaminar planes. Towards the end of the fatigue life fibre bundles fail in the undulation regions and lead to general weakening and subsequent failure. The S–N curve falls more steeply than for equivalent nonwoven material.4 Thus, although woven composites have many processing advan
Fatigue
201
tages, their mechanical properties, particularly in fatigue loading, are generally poorer than unidirectional tape materials.
11.5
Fatigue damage effects on mechanical properties
11.5.1 Stiffness The progressive damage sustained by a laminate during fatigue will affect the macroscopic mechanical properties of the material to an extent which depends on the specimen geometry, laminate stacking sequence and mode of testing. For example, in unidirectional, highmodulus carbon fibre/epoxy laminates, subjected to tension–tension fatigue, no significant change in composite stiffness is expected prior to failure. By contrast, in crossply laminates transverse ply cracking occurs early in the life of the specimen, causing a stiffness reduction that will increase with number of cycles. Stiffness reduction in composite laminates has been studied extensively and very good correlations have been obtained with the level of matrix cracking.22 The curve of normalised modulus versus cycles consists of three distinct regions;18 Fig. 11.5. The initial rapid stiffness reduction of Stage I is
Normalised stiffness
100%
I
0
II
Fatigue life
I: Rapid accumulation of offaxis ply cracks
II: Reduced rate of cracking, linear stiffness decrease
III
100% III: 0° fibres failure, localisation of damage leading to failure
11.5 Schematic stiffness–fatigue life curve for a multiply laminate showing three characteristic stages of stiffness reduction.18
202
Analytical and numerical modelling
1.0
Residual strength, GPa
CFRP smax=700 MPa
0.5 GFRP
KFRP 400 MPa
400 MPa
200 MPa
0
1
2
3
4 Log cycles
5
6
7
8
11.6 Residual strength of three kinds of 0/90° laminates following fatigue cycling at the stress level indicated: R = 0.1.2
dominated by the formation of offaxis ply cracks, although some edge delamination (in a 0/90/45° laminates) and 0° fibre fracture (in 0/90/0°) may also occur. Throughout the approximately linear region of Stage II, the matrix crack density is still increasing but much more slowly, and further fibre fracture is accompanied by 0° ply splitting (0/90/0°) and edge delaminations (0/90/45°). In Stage III, the final rapid stiffness reduction is associated with localisation of the damage processes to form a macrocrack which precipitates ultimate failure.
11.5.2 Residual strength The effect of fatigue loading on laminate residual strength can be described by the concepts of ‘wearout’ and ‘sudden death’. The wearout model assumes that the residual strength of the laminate falls gradually with cycles until failure occurs when the residual strength equals the applied cyclic stress; Fig. 11.6. This behaviour is observed in crossply GFRP and Kevlar fibre composites.23 The suddendeath model proposes that instead of progressively decreasing the residual strength, some other material property changes (such as matrix properties) which does not reduce the strength significantly until very close to failure. This type of behaviour is generally shown by CFRP laminates; Fig. 11.6.
Fatigue
11.6
203
Fatigue damage modelling
Although the details of the damage mechanisms in the various composite systems are quite varied, it is possible to identify certain general features in the damage development. As an overall generalisation damage development may be considered to take place in two stages: the distributed damage stage and the localised damage stage.24 Furthermore, the distributed damage stage is initially noninteractive, i.e. the individual damage entities initiate and grow uninfluenced by the others. The degree of interaction increases, first gradually, and eventually becomes severe enough to cause localised damage development in some preferred zones. Further development of damage involves instability and loss of integrity, and is statistically governed. The present state of damage modelling, using a micromechanics25–27 or continuum damage approach,28,29 has come as far as to model the distributed damage stage. Localised damage development is not yet sufficiently understood to attempt realistic modelling, including, for example, multiple delaminations. Earlier studies on damage accumulation during cyclic loading attempted to obtain useful working relationships of the Miner’s rule type, that might be used in design. Howe and Owen30 who studied CSM/polyester composites suggested that although debonding did not itself cause reductions in strength it did serve to initiate resin cracks which weakened the material. For resin cracking during fatigue, the authors proposed a nonlinear damage law, independent of stress level, which gives the damage, D, as 2
È Ê nˆ Ê nˆ ˘ D = Â ÍA +B Ë ¯ Ë N ¯ ˙˚ Î N
[11.1]
where n is the number of cycles sustained by the composite at a stress level which would normally cause failure after N cycles, and A and B are constants. D is equal to unity at failure. Fong31 proposed an alternative singleparameter stressindependent damage model in which the damage factor D was given by D=
(e kx  1) (e k  1)
[11.2]
for k ª 0 and 0 < x < 1, where k and x are constants determined from experimental data. This model implies that the rate of accumulation of damage (matrix cracking), dD/dt, depends linearly on t as a first approximation, t being the nonlogarithmic cycle ratio n/N. For different values of k this function generates a family of exponential curves. A similar approach to quantify and predict the effect of damage on fatigue life was used by Beaumont and coworkers,32 where all the individual damage mechanisms, e.g. splitting, delamination and matrix cracking,
204
Analytical and numerical modelling
are assumed to contribute to a global damage parameter, D. This parameter can be related to a measurable change in laminate property such as stiffness to find the rate of change of D with cycles and then integrated to give D after N cycles at a given load. A suitable failure criterion is then applied to determine the critical value of D. Also, the rate of growth of individual types of damage (e.g. transverse ply cracking) have been considered. A fracture mechanics parameter, the strain energy release rate G, has been used to relate fatigue crack growth to the change in laminate compliance33 using the relationship between G and the change in laminate compliance with transverse ply crack length.Wang et al.34 assumed a simple power law dependence of the rate of growth of full plywidth flaws across the ply thickness on the strain energy release rate (calculated by FE analysis). The energy release rate depends on crack spacing and is reduced by crack interactions, which is relevant to experimental observations of the effect of the proximity of neighbouring cracks on growth rate as the crack density increases.35 The strain energy release rate has also been used to model fatigue delamination growth in angleply laminates.36 A different fracture mechanics approach to modelling matrix crack growth is taken by Bader et al.17 in which an approximate expression is derived for the stress intensity factor at the tip of a full plythickness transverse crack growing across the ply width. The stress intensity factor also depends on crack spacing and decreases as the spacing decreases. A Paris Law relationship gave good correlation between total crack growth rate (inferred from the measured rate of stiffness reduction) and the maximum stress intensity factor. In some recent work, Behesty et al.37 have developed a constantlife model which is able to describe the stress/life/Rratio failure surface of a given laminate in terms of the monotonic tensile and compressive strengths of the material and three empirical parameters, referred to as f, u and v. It was found that for a CFRP laminate the values of u and v are close to 2 and do not vary greatly with life or material characteristics. The parameter, f, on the other hand, is a function of the ratio of the compressive and tensile strengths, and varies with life. The model appears to be valid for glass fibrereinforced plastics as well as for the carbon fibre composites for which it was originally developed.
11.7
A finite element model for fatigue life prediction of CFRP components
11.7.1 Introduction Very little FE modelling of the fatigue of composite structures appears to have been undertaken. In this section a particular case of a webnotched
Fatigue P/2
133 mm
117 mm
383mm
205
P/2
117 mm
46 mm
60 mm
P/2
P/2
11.7 A webnotched Ibeam subjected to a fourpoint bending load.38
Ibeam subjected to the fourpoint bending load illustrated in Fig. 11.7 is described.38 The basis of the method is first to use a fracture mechanics approach to obtain experimentally the relationship between the maximum strain energy release rate experienced during a fatigue cycle and the rate of growth of the damage. For the beam, the latter was mainly matrix cracking, as determined by observations during a series of fatigue tests. The component is then analysed using FE analysis, the local stresses and strains around the notch determined, the energy release rate calculated and then combined with the fracture mechanics data to give the lifetime, which is compared with experimental results.
11.7.2 Outline of predictive method The model is based on a combination of FE stress analysis and fracture mechanics. The FE analysis (using the ABAQUS system, with 2D shell elements) is used to get a detailed stress distribution in the structure when subjected to a static load equal to the maximum load applied in the fatigue cycle. Interrogation of the output allows identification of strains above a designated threshold (for matrix cracking), and the elements and plies within the element in which these strains occur. The elastic properties in the damaged plies are then reduced and the analysis repeated. Further damage is identified and the process continued until final failure is indicated. In the experimental work fibre fracture was identified as being the ultimate cause of failure. Hence, in the model, fibre strains are monitored and when the ultimate fibre failure strain is reached, at any location, the analysis is halted. At each iteration of the analysis the strain energy release rate, G, in the structure is calculated. So, at the conclusion of the analysis a relationship between G and damage area, A, is available. This information is then combined with fracture mechanics in the form of the Paris Law, and from this the lifetime is found. n An initial model was based on the simple Paris Law: dA/dN = DGmax linking damage area, A, number cycles, N, and maximum strain energy
206
Analytical and numerical modelling
release rate in a cycle, Gmax, via ‘materials’ parameters D and n. This information would typically be determined from the double cantilever beam test. From the above equation, the lifetime is found by integration as Nf = Ú
Af
0
dA n
D[G( A)]
where the final damage area Af corresponds to fibre fracture. The lifetime predictions from the initial model proved to be extremely sensitive to values of n and D and to overcome this a modified form of the Paris Law was used: n
dA n = DGmax dN
È Ê Gth ˆ 1 ˘ ˙ Í1  Ë Gmax ¯ ˚ Î n È Ê Gmax ˆ 2 ˘ Í1  Ë ˙ Gc ¯ ˚ Î
where Gth is a threshold value of Gmax, below which no cracking occurs, and Gc is the critical value above which instantaneous failure occurs. The terms n1 and n2 are additional ‘materials’ parameters. The integration to get lifetime was performed numerically. Data for stiffness reduction due to matrix cracking were obtained from published work on a similar material to that from which the beams were fabricated (CFRP: XAS/914 from Hexcel Composites).39
11.7.3 Results from model A key issue proved to be the availability, and quality, of fracture mechanics data, essentially the Paris Law constants (n and D (and n1 and n2 if appropriate)). Owing to scatter in the results of DCB, and similar tests, a spread of n and D is always apparent. The values chosen, by curve fitting the experimental points, have a major influence on the predictions. Another factor that influences the outcome of the predictions is the values of elastic constants that are input to the FE model. The most critical parameter seems to be the modulus (E22) at right angles to the fibres in the unidirectional ply, although Poisson’s ratio and shear modulus also play a part. The best estimate, from the modified Paris Law, was 3.3 ¥ 106 cycles to failure, which compares with the experimental value for the lifetime, Nf, of 4.78 ¥ 106 cycles. The predicted growth of damage area compared well with experiment. A typical FE mesh is shown in Fig. 11.8 and a comparison of predicted and measured damage growth is seen in Fig. 11.9.
Fatigue
207
P/2
P/2
60 mm
P/2
P/2
46 mm
11.8 FE mesh of notched Ibeam.38
4.00E+02
Damage area (mm2)
3.50E+02 3.00E+02 2.50E+02 2.00E+02 1.50E+02 1.00E+02 Experiment
5.00E+01 0.00E+00 0.00E+00
Prediction 1.00E+06
2.00E+06
3.00E+06
4.00E+06
5.00E+06
6.00E+06
Fatigue cycles
11.9 Comparison of experimental and predicted damage growth in Ibeam.38
11.8
Summary
In contrast to metals, composites accumulate damage in a general rather than a localised fashion, and fracture does not usually occur by propagation of a single macroscopic crack. The microstructural mechanisms of damage accumulation, including fibre/matrix debonding, matrix cracking, delamination and fibre fracture, occur sometimes independently and sometimes interactively, and the predominance of one or other of them may be strongly affected by both materials’ variables and testing conditions. Fatigue damage leads to a permanent degradation in laminate stiffness and residual strength. The fatigue resistance of composites is reduced when the applied load is other than tensile and in the fibre direction. Compression, flexure and torsion subject the relatively weak matrix and fibre/matrix interface to shear stresses, reducing the contribution of the fibres to the fatigue resistance and allowing compressive fibre buckling initiated by local matrix
208
Analytical and numerical modelling
shear and longitudinal splitting. Fatigue lives in tension–compression loading are usually shorter than for zerocompression or zerotension fatigue. The effect of exposure to moisture and changes in temperature on the fatigue response depends on the sensitivity of the laminate to matrix properties, since it is usually the matrix or fibre/matrix interface that is affected. Thus carbon fibre laminates, having a strong fibre/matrix interface, show little sensitivity to moisture content or a rise in temperature. It should be noted that the test method, specimen design, edge effects and stress concentrations such as notches, holes, fasteners, impact damage and other imperfections may affect the fatigue strength. However, because of relatively low static design allowables, fatigue strength is not usually a serious design criterion for current carbon fibre composite structures. Finally, a fracture mechanics parameter, the strain energy release rate (calculated by finite element analysis) is commonly used to relate fatigue crack growth (matrix cracking or delamination) to the change in laminate stiffness. This information can then be combined with a simple power law (usually the Paris Law) to predict the fatigue life of composite structures. All existing fatigue models require extensive experimental data.
11.9
References
1 Harris B, ‘Fatigue and accumulation of damage in reinforced plastics’, Composites, 1977 8(4) 214–220. 2 Harris B, Engineering Composite Materials, London, Institute of Metals, 1986. 3 Konur O & Matthews F L, ‘Effect properties of the constituents on the fatigue performance of composites: a review’, Composites, 1987 20(4) 317–328. 4 Curtis P T, ‘The fatigue behaviour of fibrous composite materials’, J Strain Analysis, 1989 24(4) 47–56. 5 Talreja R, Fatigue of Composite Materials, Ed L L Reifsinider, New York, Elsevier Science Publishers, 1991. 6 O’Brien T K (Ed), Composite Materials: Fatigue & Fracture, 3rd Volume, ASTM STP1110, American Society for Testing and Materials, Philadelphia, PA, 1991. 7 Carlson R L & Kardomateas G A, An Introduction to Fatigue in Metals and Composites, London, Chapman & Hall, 1996. 8 Reifsnider K L & Jamison R D,‘Fracture of fatigueloaded composite laminates’, Int J Fatigue, 1982 4(4) 187–197. 9 Pagano N J & Bryon Pipes R, ‘Influence of stacking sequence on laminate strength’, J Compos Mater, 1971 5(1) 50–57. 10 Bailey J E, Curtis P T & Parvizi A, ‘On the transverse cracking and longitudinal splitting behaviour of glass and carbon fibrereinforced epoxy crossply laminates and the effect of poisson and thermally generated strain’, Proc Royal Society London, 1979 A366(1727) 599–623. 11 Jamison R D, ‘The role of microdamage in tensile failure of graphite/epoxy laminates’, Composites Sci Tech, 1985 24(2) 83–99.
Fatigue
209
12 Purslow D, ‘Some fundamental aspects of composites fractography’, Composites, 1981 12(4) 241–247. 13 Curtis P T, ‘An investigation of the tensile fatigue behaviour of improved carbon fibre composites materials’, Proc ICCM6, Elsevier Applied Science London, 1987. 14 Talreja R, ‘Fatigue of composite materials: damage mechanisms and fatigue life diagrams’, Proc Royal Society London, 1981 A387(1775) 461–475. 15 Jamison R D, Schulte K, Reifsnider K L & Stinchcomb W W, ‘Characterisation and analysis of damage mechanisms in fatigue of graphite/epoxy laminates’, ASTM STP836, American Society for Testing and Materials, Philadelphia, PA, 1983. 16 Reifsnider K L & Jamison R D, ‘Fracture of fatigue loaded composite laminates’, Int J Fatigue, 1982 4(4) 187–198. 17 Bader M G & Boniface L, ‘Damage development during quasistatic and cyclic loading in GRP and CFRP laminates containing 90° plies’, Proc Conf ICCMV, The Metallurgical Society Inc, Warrendale, PA, 1985. 18 Highsmith A L & Reifsnider K L, ‘Internal load distribution effects during fatigue loading of composite laminates’, Debonding of Materials ASTM STP907, Philadelphia, PA, American Society for Testing and Materials, 1986. 19 Schulte K, ‘Development of microdamage in composite laminates during fatigue loading’, Proc Int Conf Testing, Evaluation & Quality Control of Composites, Butterworths, 1983. 20 Jamison R D, ‘On the interrelationship between fibre fracture and ply cracking in graphite/epoxy laminates’, Debonding of Materials ASTM STP907, Philadelphia, PA, American Society for Testing and Materials, 1986. 21 Curtis P T & Bishop S M, ‘An assessment of the potential of woven carbon fibre reinforced plastics for high performance use’, Composites, 1984 15(4) 259–265. 22 Highsmith A L & Reifsnider K L, ‘Stiffness reduction mechanisms in composite laminates’, ASTM STP775, American Society for Testing and Materials, Philadelphia, PA, 1982. 23 Adam T, Dickson R F, Jones C J, Reiter H & Harris B, ‘A power law fatigue damage model for fibrereinforced plastic laminates’, Proc Inst Mech Engs, 1986 200(3) 155–166. 24 Talreja R, ‘Damage development in composites: mechanisms and modeling’, J Strain Analysis, 1984 24(4) 27–34. 25 Laws N, Dvorak G J & Hejazi M, ‘Stiffness changes in unidirectional composites caused by crack systems’, Mech Materials, 1983 2, 123–137. 26 Hashin Z, ‘Analysis of cracked laminates: a variational approach’, Mech Materials, 1985 4, 122–136. 27 Aboudi J, ‘Stiffness reduction in cracked solids’, Eng Fracture Mech, 1987 26(5) 637–650. 28 Talreja R, ‘A continuum mechanics characterisation of damage in composite materials, Proc Roy Soc, London, 1985 A399(1817) 195–216. 29 Allen D H, Groves S E & Harris C E, ‘A cumulative damage model for continuous fibre composite laminates with matrix cracking and interply delaminations’, ASTM STP972, Philadelphia, PA, American Society for Testing and Materials, 1988. 30 Howe R J & Owen M J, Proc Eighth Int Reinforced Plastics Congress, London, British Plastics Federation, 1972.
210
Analytical and numerical modelling
31 Fong J T, Damage in Composite Materials, ASTM STP775, Ed K L Reifsnider, Philadelphia, PA, American Society for Testing and Materials, 1982. 32 Poursartip A, Ashby M F & Beaumont P W R, ‘The fatigue damage mechanisms of a carbon fibre composite laminate: Development of the model’, Compos Sci Tech, 1986 25(3) 193–218. 33 Beaumont P W R, ‘The failure of fibre composites: an overview’, J Strain Analysis, 1989 24(4) 1–17. 34 Wang A S D, Chou P C & Lei S C, ‘A stochastic model for the growth of matrix cracks in composite laminates’, J Compos Mater, 1984 18(3) 239–254. 35 Boniface L & Ogin S L, ‘Application of the Paris equation to the fatigue growth of transverse ply cracks’, J Compos Mater, 1989 23(7) 735–754. 36 O’Brien T K, ‘Characterisation of delamination onset and growth in a composite laminate’, ASTM STP775, Philadelphia, PA, American Society for Testing and Materials, 1982. 37 Behesty M H, Harris B & Adam T, ‘A general fatigue life model for highperformance fibre composites with and without impact damage’, Composites: Part A, 1999 30(8) 971–987. 38 Matthews F L, Kinloch A J, Feng X & Attia O, Modelling the Fatigue Damage Growth in Fibrereinforced Plastic Composite Components, Final Report, Centre for Composite Materials, Imperial College, 1999. 39 Tong J, Guild F J, Ogin S L & Smith P A, ‘On matrix crack growth in quasiisotropic laminates – I: experimental investigation’, Compos Sci Tech, 1997 57(11) 1527–1535.
Index
A B D matrices, 25, 85, 86, 99, 100, 114 adaptivity, 61, 65, 66 average stress criterion, 153 bandwidth, 57 buckling, 35, 76, 88 Classical Laminate Theory (CLT), 25 limitations, 34 compatibility, 43 composite constituents matrix, 6 phases, 6 reinforcement, 6 cracking mechanisms, 140, 190 delamination, 146 fibre bridging, 143 fibre debonding, 143 fibre fracture, 143, 146 fibre pullout, 143 matrix cracking, 143, 146 microbuckling, 143, 146 propagation, 142 toughening, 144 cutouts, 129 damage general, 140 fatigue, 194, 199 damaged laminate, 161 delamination, 125, 127, 158, 195 density, 9 direction cosines, 49 double cantilever beam (DCB), 111, 172 edges, 35, 71, 123 3D stress state, 123, 132 delamination, 125, 127 finite difference analysis, 126 interlaminar stresses, 123, 132, 134 singularity, 126 transverse shear stress, 124, 134
element types, 46, 62, 71 beam, 58, 81 brick, 57, 71, 86, 103 hexagonal brick, 49 interface, 109, 112, 171 isoparametric, 56 membrane, 71 Mindlin, 59, 74, 85 beam, 60 plate, 60, 89 shell, 74, 76, 77, 87, 103 plate, 60, 71, 86 quadrilateral 4node, 55, 71, 72, 79, 83 8node, 79 quarterpoint element, 149 semiLoof, 76, 85, 89 shell, 71 solid shell, 77, 78, 86, 87 triangular, 54, 72, 83 equilibrium, 42 examples of finite element analysis buckling, 88 coupling, 92 crack propagation, 112 effect of layup, 90 energy release rate, 66, 108, 110, 151 failure, 107 fibre orientation, 96, 97 fracture mechanics, 110 geometry & topology, 94 conical surfaces, 94 double curvature, 95 filament winding, 95 interface element, 109, 171 Jintegral, 110, 150 joints, 178, 180 laminated plate, 87 micromechanics, 113 piezoelectric effects, 116 ply dropoff, 100
211
212
Index
real structures, 101 element choice, 103 mirroring, 102 offsets, 102 rigid links, 102 smart composites, 116 surface stresses, 87 thickness variation, 99 virtual crack closure (VCC), 111, 164 virtual crack opening, 112 volume fraction variation, 99 zero thickness ply, 101 failure criteria, 30 average stress, 153 ChangChang, 108 interactive, 32 limit, 31 point stress, 153, 188 TsaiHill, 32 fatigue, 194 damage mechanisms, 194 damage modelling, 203 FE modelling, 204 multidirectional laminates, 198 progressive damage, 199 residual strength, 202 stiffness reduction, 201 unidirectional laminates, 196 fibre/matrix interface, 6, 10, 142 fibres, 11 aramid, 12 carbon, 13 glass, 13 polyethylene, 12 finite element analysis approximations, 41, 49 assumptions, 42 basics, 41 compatibility, 43, 51 displacement solution, 44 equilibrium, 42, 48, 54 errors, 41 examples, 87 Gauss points, 53, 57, 97, 99, 108 kinematically equivalent forces, 52, 59 material stiffness matrix, 52 nodal forces, 52 rigid body motion, 54, 55 shape functions, 51, 54, 73, 86 stressstrain, 43, 52 structural stiffness matrix, 53 finite element equations accuracy of solution, 78 coarse mesh, 79 convergence, 79 fine mesh, 79 mesh fineness/density, 78, 82 negative stiffness, 109, 113
results, 65 adaptivity, 65, 66 errors, 65 numerical integration, 65 solution, 63 Cholesky factorisation, 64 conditioning number, 63, 64 conjugant gradient technique, 64 direct methods, 64 Gaussian elimination, 64 illconditioning, 71 indirect methods, 64 Lagrangian methods, 104 Lanczos method, 118 ‘locking’, 63 rounding error, 78 trace, 64 finite element mesh automatic refinement, 110 density, 82 generation, 62, 99, 102 geometry, 62 hrefinement, 82 moving mesh, 110, 113 multipoint constraints, 83 Pavé method, 83 prefinement, 82 refinement, 104 finite element modelling techniques 3D stresses, 132 composites, 84 A B D matrices, 85 Classical Laminate Theory (CLT), 84 Mindlin elements, 85 semiLoof elements, 85 solid shell element, 86 transverse shear strain, 85, 89 curved edges, 130 delamination, 81, 158, 171 fatigue, 204 fracture, 139 joints, 175, 179, 186, 189 multipoint constraints (MPCs), 81, 104 progressive failure, 155 rigid links, 81, 102, 104, 108 straight edges, 129 virtual crack closure, 164 finite elements; general ‘drilling’ rotation/freedom, 74, 77 ‘hour glass’ nodes, 76 interpolation functions, 86 numerical integration, 76 ‘patch’ test, 74 shape functions, 51, 54, 73, 86 shear correction factor, 74, 89 transverse strains, 74, 77, 85 fracture mechanics, 110, 139, 141, 149, 205
Index inherent flaw model, 147 fracture toughness, 141
notch sensitivity, 139, 146 notched strength, 146
Gauss’s theorem, 48
orthotropy general, 22 special, 22
holes, 129 in situ damage effective function (IDEF), 158 isotropy, 10 transverse, 17 Jintegral, 110, 150 joints, 175 bonded, 175 failure, 179 FE analysis, 179 scarf, 179 single lap, 177 stresses, 176 mechanically fastened, 183 bearing strength, 184 failure modes, 183 FE analysis, 186, 189 Kirchhoff theory, 73 laminates, 8, 17 antisymmetric, 26 balanced, 26 plate constitutive equations, 25 coupling, 22, 25, 90, 96 quasiisotropic, 27 stiffness, 23 bending strain, 23 inplane strain, 23 layup, 23, 96 stacking sequence, 23, 96 stress resultants, 25 strength, 33 final failure, 34 initial (first ply) failure, 33 symmetric, 26 matrices element stiffness, 52 Jacobian, 57, 73 material stiffness, 52 ply compliance, 20 ply stiffness, 20 structural stiffness, 53 determinant of, 60, 63 transformation, 21 Mindlin theory, 73 modelling damage, 190 modelling delamination, 158 continuum model, 159, 168 FE model, 164, 168 nonlinear problems, 76, 78, 89, 104, 106, 107
213
Paris law, 205, 206 point stress criterion, 153, 188 polymer matrices, 14 curing, 15 properties, 15 thermoplastics, 14, 16 thermosets, 14, 15 preprocessor, 61 Principle of Virtual Displacements (PVD), 45 external virtual work, 47 internal virtual work, 47 total virtual work, 53 virtual work, 45 residual stresses, 29, 169 shear strength inplane, 29 throughthickness (interlaminar), 29, 34 stiffness matrix element, 52, 59 ply, 20 structural, 53 strain energy release rate, 151, 158, 162, 163, 205 stress intensity factors, 149 stressstrain law, 43 unidirectional composites compliance matrix, 20 macromechanics, 17 micromechanics, 17, 27, 113 HalpinTsai equations, 114 stiffness, 27 strength, 28 thermal & moisture, 29 modulus longitudinal, 18 shear, 18 transverse, 18 offaxis loading, 20 Poisson’s ratio, 18 rotated layer, 20 stiffness, 17 stiffness matrix, 20 strength, 30 stressstrain relations, 18 transformation matrix, 21 transformed compliance, 22 transformed stiffness, 22
214
Index
Virtual Crack Closure (VCC), 111, 159, 164 FE modelling, 164, 168 Virtual Crack Extension (VCE), 149 volume fraction, 9
weight fraction, 9 work of fracture, 141 debonding, 145 friction, 145 pullout, 145